SELFCOMPACTING HIGH AND ULTRA HIGH PERFORMANCE CONCRETES. Akbar Ghanbari


 Melvyn Cobb
 3 months ago
 Views:
Transcription
1 SELFCOMPACTING HIGH AND ULTRA HIGH PERFORMANCE CONCRETES Akbar Ghanbari Ph.D. 2011
2 UMI Number: U All rights reserved INFORMATION TO ALL USERS The quality of this reproduction is dependent upon the quality of the copy submitted. In the unlikely event that the author did not send a complete manuscript and there are missing pages, these will be noted. Also, if material had to be removed, a note will indicate the deletion. Dissertation Publishing UMI U Published by ProQuest LLC Copyright in the Dissertation held by the Author. Microform Edition ProQuest LLC. All rights reserved. This work is protected against unauthorized copying under Title 17, United States Code. ProQuest LLC 789 East Eisenhower Parkway P.O. Box 1346 Ann Arbor, Ml
3 SELFCOMPACTING HIGH AND ULTRA HIGH PERFORMANCE CONCRETES Akbar Ghanbari B.Sc., M.Sc. Submitted for the degree of Doctor of Philosophy C a r d if f UNIVERSITY PRIFYSGOL CaeRDY[ > Department of Civil Engineering Cardiff University, UK April 2011 I
4 In the Name of God the Most Compassionate and the Most Merciful II
5 DECLARATION This w ork has not previously been accepted in substance for any degree and is not concurrently subm itted in candidature for any degree. S i g n e d. (candidate) D a t f STATEMENT 1 This thesis is being subm itted in partial fulfilment of the requirem ents for the degree of Doctor of Philosophy. Signed../) (can didate) Date. J zy.. STATEMENT 2 This thesis is the result of my own independent w ork/investigations, except where otherw ise stated. O ther sources are acknow ledged by explicit references. S ig n e d.tt. (candidate) Date.. STATEMENT 3 I hereby give consent for my thesis, if accepted, to be made available for photocopying and for interlibrary loan, and for the title and sum m ary to be made available to outside organisations. Signed. (candidate) Dat Ill
6 IV To Forouzan and Parinaz
7 ACKNOWLEDGEMENT My deepest gratitude is to my supervisor, Professor B.L. Karihaloo. It has been an honour to be his Ph.D. student. He has been always ready to listen and give advice. I am grateful to him for sharing his valuable time and knowledge. He offered me so much advice, patiently supervising me, and always guiding me in the right direction. I have learned a lot from him, without his help I could not have finished my dissertation successfully. I am also thankful to him for encouraging the use of correct grammar and consistent notation in my writings and for carefully reading and commenting on revisions o f this dissertation. My cosupervisor, Dr S. Kulasegaram has been always helpful. I am deeply grateful to him for valuable discussions we had during my research project. Sincere thanks are conveyed to Faculty of Civil Engineering at Cardiff University and my friends. I am also grateful to my parents who helped me stay sane through these years. Their support and care helped me to overcome setbacks and stay focused on my graduate study. Last but not least, I am greatly indebted to my devoted wife Forouzan and my daughter Parinaz. They form the backbone and origin o f my happiness. Their love and support without any complaint or regret has enabled me to complete this Ph.D. project. Being both a mother and father while I was away was not an easy thing for my wife. She took every responsibility and suffered all the bitterness to take care of my daughter and my family. I owe my every achievement to both of them. V
8 SYNOPSIS This thesis describes the steps taken to develop selfcompacting high and ultra highperformance concretes with (SCHPFRC/SCUHPFRC) and without steel fibres (SCHPC/SCUHPC). For the selfcompacting concrete mixes without steel fibres the fulfilment o f the flow and cohesiveness criteria are found to be sufficient for the mix design. However, for the design of selfcompacting concrete mixes with steel fibres it is found that they must additionally meet the passing ability criterion. Micromechanical constitutive models are used to predict the plastic viscosity of SCHPFRC/SCUHPFRC from the measured plastic viscosity of the paste. The concrete is regarded as a twophase suspension in which the solid phase is suspended in a viscous liquid phase. The liquid matrix phase consists of cement, water and any viscosity modifying agent (VMA) to which the solids (fine and coarse aggregates and fibres) are added in succession. The predictions are shown to correlate very well with available experimental data. A Lagrangian particle based method, the smooth particle hydrodynamics (SPH), is used to model the flow of SCHPC/SCUHPC with or without short steel fibres. An incompressible SPH method is employed to simulate the flow of such nonnewtonian fluids whose behaviour is described by a Binghamtype model, in which the kink in the shear stress versus shear strain rate diagram is first appropriately smoothed out. The basic equations solved in the SPH are the incompressible mass conservation and NavierStokes equations. The solution procedure uses predictioncorrection fractional steps with the temporal velocity field integrated forward in time without enforcing incompressibility in the prediction step. The resulting temporal velocity field is used in the mass conservation equation to satisfy incompressibility through a pressure Poisson equation derived from an approximate pressure equation. The results of the numerical simulation are benchmarked against actual slump tests carried out in the laboratory. The numerical results are in excellent agreement with test results, thus demonstrating the capability of SPH and a proper Theological model to predict selfcompacting concrete flow behaviour. The simulations o f SCC mixes are also used as an aid at the mix design stage of such concretes. Selfcompacting high and ultrahigh performance concrete (SCHPC/SCUHPC) mixes with and without steel fibres (SCHPFRC/SCUHPFRC) are proportioned to cover a wide range of plastic viscosity. All these mixes meet the flow and passing ability criteria, thus ensuring that they will flow properly into the moulds. VI
9 TABLE OF CONTENTS DECLARATION AKNOWLEDGEMENT SYNOPSIS TABLE OF CONTENTS III V VI VII Chapter 1: Introduction Research background Research objectives Research methodology Outline of the thesis... 6 Chapter 2: SelfCompacting Concrete Introduction Historical development of selfcompacting concrete Definitions of selfcompacting concrete Basic properties of selfcompacting concrete How to achieve the required properties of selfcompacting concrete? Different mix designs of selfcompacting concrete Superplasticiser Action of superplasticisers Cement replacement materials and microsilica Cement replacement materials Ground granulated blast furnace slag Fly ash Microsilica...23 VII
10 2.8.3 Benefits of CRMs Effect of fibres on the behaviour of fresh selfcompacting concrete Characteristics of the fibres Properties of fresh selfcompacting concrete Flowing ability Passing ability Segregation resistance Tests on fresh selfcompacting concrete Flowability test Slump flow test Is there any relationship between rheological characteristics o f selfcompacting concrete and slump flow test measurements? Passing ability tests Lbox test JRing test Segregation tests Visual examination Sieve stability test Examples of structures made with selfcompacting concrete Concluding remarks...41 VIII
11 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow Introduction Classification of workability Rheological characteristics of selfcompacting concrete Measuring the rheological parameters Rheology of cement paste Rheology of selfcompacting concrete Coaxial cylinder rheometers Parallel plate rheometers Impeller rheometers Mathematical description of selfcompacting concrete rheology Is there any consistency in the rheological properties o f concrete? Effect of concrete constituents on the Bingham constants Basic terms and equations used in the general flow simulation Finite control volume Infinitesimal fluid element Material derivative Physical meaning of v V The continuity equation The momentum equations Disregarding energy conservation equations Fluid classifications Newtonian and NonNewtonian fluids Bingham plastic model IX
12 HerschelBulkley model Compressible and incompressible fluids Artificial compressibility PressurePoisson equation Simulation of the flow of concrete FEM modelling techniques Homogeneous fluid simulation Nonhomogeneous fluid simulation Disadvantages of meshbased numerical simulations Meshless particle based simulation Introduction to smooth particle hydrodynamics (SPH) Key characteristics of SPH method Nodes or particles in SPH Support domain Essential formulation of SPH Integral representation Kernel function Particle approximation Corrected SPH integration Incompressibility in SPH Concluding remarks...82 X
13 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres Introduction Development of SelfCompacting HighPerformance FibreReinforced Concrete (SCHPFRC) Mix preparation Flowability test SCHPC and SCHPFRC mixes Influence of the type of superplasticiser Passing ability test Development of SelfCompacting Ultra HighPerformance FibreReinforced Concrete (SCUHPFRC) Flowability test SCUHPC and SCUHPFRC Selfcompacting ultrahigh performance concrete (SCUHPC) Selfcompacting ultrahigh performance fibre reinforced concrete (SCUHPFRC) Passing ability test Concluding remarks XI
14 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Introduction Methodology...I l l 5.3 Plastic viscosity o f selfcompacting concrete without steel fibres Selfcompacting concrete as a concentrated suspension of solid particles in a viscous liquid Low concentration ( ^ <0.1) High concentration f 0.1 < $ < </>m) Are the expressions for the viscosity o f a suspension o f solid particles in a viscous fluid applicable to cement paste? Effect of fibres on the viscosity of SCC Replacing ensemble average by volume average Random distribution of fibres Calculation of the fibre fabric tensor Comparison o f the proposed formulae with test results Plastic viscosity of cement paste Plastic viscosity o f selfcompacting fibre reinforced concrete Comparison of the predicted and measured plastic viscosity with respect to first fibre parameter <j>f ld Predicted vs. measured plastic viscosity with respect to second fibre parameter 1 / In ( 21 d ) Discussion of the results Estimation o f the plastic viscosity o f selfcompacting high and ultrahigh performance concretes with and without steel fibres Practical usefulness of the proposed micromechanical model Concluding remarks XII
15 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Introduction Governing Equations D discretisation o f mass and momentum conservation equations Mass conservation equation Momentum conservation equations Discretisation o f mass and momentum conservation equations in the cylindrical coordinate system Mass conservation equation Momentum conservation equations D discretisation of mass and momentum conservation equations Axisymmetric discretisation o f mass and momentum conservation equations Numerical solution procedure Prediction step Correction step SPH discretisation of the governing equations Gradient of pressure Divergence of velocity Laplacian Viscosity Time step Numerical simulation results Slump flow test Initial configuration and boundary conditions Numerical test results XIII
16 6.6.2 Fibre positions and orientations Lbox test Initial configuration and boundary conditions Numerical test results Simulation time Slump flow time Lbox time Concluding remarks Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Introduction Types ofscc mixes Slump flow test Lbox test Mix proportioning Method of estimating the volume fractions of solid particles Typical SCHPFRC mix proportions Typical SCUHPFRC mix proportions Concluding remarks An example of the application of the mix proportioning Remarks on the choice o f f Chapter 8: Conclusions and Recommendations for Future Research Conclusions Recommendations for future research XIV
17 References 190 Appendix A Appendix B Appendix C Appendix D XV
18 List of Figures 2.1: Proposed rational model o f Ozawa (After Ouchi, 1999) : A typical mix proportioning of SCC and normal vibrated concrete : Typical volumes o f constituents in normal HPC and SCCs : Methods to achieve selfcompacting ability (After Ouchi et al., 1996) : Excess paste layer around aggregates (After: Oh et al., 1997) : A typical mix design o f SCC based on the Okamura and Ozawa procedure (Brite, 2000) : Development in admixture technology (After Dransfield, 2003) : Effect o f dispersing admixtures in breaking up cement floes (After Dransfield, 2003) : Effect of aggregate size on fibre distribution (After Johnston, 1996) : Schematic of blocking (After RILEM TC 174 SCC, 2000) : Schematic of ways to achieve SCC (After Liu, 2009) : Apparatus for Slump Flow test (After David and Shah, 2004). All dimensions in mm : The relationship between slump and slump flow measurements (After Domone, 2003) : A typical relationship between slump flow diameter and yield stress for different mixes of selfcompacting concrete (After Grunewald, 2004) : A typical relationship between flow time (T500) and plastic viscosity o f SCC (After Grunewald, 2004) : Schematic of Lbox (top), (After Thrane, 2007), with heights at either end of horizontal trough (bottom). All dimensions in m m : JRing apparatus : Akashi Kaikyo (Straits) Bridge (After Ouchi and HibinoNagaoka, 2000) : Midsummer place in London (After Goodier, 2003) : A coaxial cylinder rheometer (After Domone, 2003) : Fanshaped curves for different watercement ratio (After Domone, 2003) : Typical effect o f watercement ratio on Bingham constants for cement paste (After Domone and Thurairatnam, 1988)...47 XVI
19 3.4: Typical effect of superplasticiser on Bingham constants for cement paste (After Domone and Thurairatnam, 1988) : Yield stress vs. plastic viscosity for cement paste with different watercement ratios and superplasticiser dosage (After Domone, 2003) : A BML rheometer (After Wallevik and Gjorv, 1990; RILEM, 2002) : A BT RHEOM rheometer (After de Larrard et al., 1997; RILEM 2002) : Two systems for the impeller rheometer (After Domone, et al., 1999; RILEM, 2002) : Two different responses for a single SCC mix tested by two rheometers (After Feys, 2007 ) : The effect of mix constituents on Bingham constants (After Domone, 2003) : Effect of some constituents on the rheological characteristics of SCC (After Dietz and Ma, 2000) : Bingham constants for mixes containing various amount o f microsilica (After Gjorv, 1997) : Finite control volume approach with fixed control volume (left) and moving control Volume (right) (After Wendt, 1992) : Infinitesimal fluid element approach with fixed control element (left) and moving control element (right) : Physical meaning o f the divergence of velocity (After Wendt, 1992) : A fluid element with components o f the force in x direction (After Wendt, 1992) : Fluid sample as tested by a parallel plate device at two time instant, ti (left) and t2>ti (right) : The fluid velocity profile varies linearly : Subdivision of nonnewtonian fluids : Types o f generalized nonnewtonian flow behaviour (After Chhabra and Richardson, 2008 ) : Behaviour o f shear thinning and shear thickening fluids in relation to viscoplastic fluids behaviour (After Domone, 2003) : Scattered nodes to represent the problem and boundary domains with two shapes of the support domain...75 XVII
20 3.23: Particle approximations using particles within the support domain o f the smoothing function W for a particle at centre : Approximation of an arbitrary function ^ (x )in terms o f kernel function Wb (x) (After Kulasegaram et al., 2002) : Horizontal spread of SCHPC mix : 30 mm long glued steel fibres : Horizontal spread of SCHPFRC mix : Flow and passing ability o f SCHPC Mix : Flow and passing ability of SCHPFRC Mix : Procedure to create a flowable SCUHPC : Horizontal spread o f SCUHPC mix : Procedure for achieving the SCUHPFRC : Horizontal spread of SCUHPFRC mix 13. The fibres are evenly distributed : Horizontal spread o f SCUHPFRC mix : SCUHPC mix 12 flows smoothly through the gaps between the steel rods : SCUHPFRC mix 13 did not satisfy the passing ability test. The fibres are nested around the steel rods : Flow and passing ability of SCUHPC mix : Flow and passing ability of SCUHPFRC mix : Hierarchy o f twophase liquidsolid suspensions constituting a SCC mix with fibres, showing the liquid (L) and solid (S) phases in each suspension : Dependency o f relative viscosity on the shear rate in a suspension at zero and infinite shear rates and fit to the Krieger and Dougherty equation (After Struble and Sun, 1995) : Comparison of different formulas for high volume fraction of spherical particles with $m=0.708 and [77] = : Rigid body translation and rotation of a single fibre resisted by the viscous SCC. The resistive concentrated force (F) is shown at the centroid of the fibre : The ensemble average can be replaced by volume average if the fibres are homogeneously and randomly distributed XVIII
21 5.6: Comparison o f the plastic viscosity with experimental results vs. first fibre parameter, <f>ld2 for the seven main mixes with M and P indicating measured and predicted plastic viscosity : Predicted vs. experimental plastic viscosity as a function o f the second fibre parameter l/ln(2/,) for the seven main mixes : Combination of the data in Figure 5.7 for all the second fibre parameters 1 / ln(2ld) : The yield stress of SCC mixes is nearly constant over a large range of plastic viscosity. (After Dransfield, 2003) : A bi1 inear Bingham fluid constitutive model replaced by the continuous function (5.43). On the scale o f the figure, the discontinuity at Ty cannot be distinguished for m=5000 and However, at a magnification of 100 on the horizontal scale as shown in the inset, it is clear that the continuous approximation is better for m= : Initial configuration o f the Slump Test in the twodimensional (Top) and axisymmetric configurations (Bottom) : Boundary conditions for the slump cone (Ppressure, vn  normal velocity, vt tangential velocity and C j  dynamic coefficient of friction) : Axisymmetric numerical simulation o f slump flow test for SCUHPC without fibres : Axisymmetric numerical simulation o f slump flow test for SCUHPC with fibres : Plan view of axisymmetric numerical simulation of slump flow test for SCUHPC with fibres at four different heights (z) along the axis o f symmetry : Numerical simulation o f slump flow test for SCUHPC with fibres in 2D approximation : Fibre distributions (dark spots) and their velocity fields (arrows) at various times during the flow of SCUHPFRC : Initial configuration of the Lbox concrete casting Boundary conditions (Ppressure, vn  normal velocity, v( tangential velocity and c y  dynamic coefficient of friction) : Numerical simulation of Lbox casting for SCUHPC mix without fibres : Numerical simulation of Lbox casting for SCUHPFRC mix : Numerical simulation of slump flow test for SCUHPC in 2D approximation using 4000 (left) and 7000 (right) particles XIX
22 7.1: Simulated T500 vs. plastic viscosity o f different mixes with steel fibres : Fanshaped correlation between plastic viscosities o f SCHPFRC and steel fibre volume fractions (tinf is the plastic viscosity o f SCHPC mix without fibres) : Fanshaped correlation between plastic viscosities o f SCUHPFRC and steel fibre volume Fractions (t] Nf is the plastic viscosity o f SCUHPC mix without fibres) : T200, T400 and the leveloff times vs the plastic viscosity of mixes for various fibre volume fractions XX
23 List of Tables 4.1: Mix proportions (kg) of a standard vibrated highperformance mix : Composition o f SCHPC and SCHPFRC mixes (kg) with naphthalene sulfonatebased superplasticiser : Composition o f SCHPC and SCHPFRC mixes (kg) with Glenium ACE 333 superplasticiser : Composition o f SCHPC mixes (kg) with 0.5% steel fibres for the JRing test : SCHPC and SCHPFRC mixes (kg) that met both workability and passing ability tests : Original CARDIFRC mix I (kg/m3) : Composition of the trial mixes (kg) of SCUHPC : Composition of SCUHPC mixes (kg) with a constant amount of solid constituents : Effect of the variation of the waterbinder and SPwater ratios on the flowability of SCUHPC : Composition of SCUHPFRC mixes (kg) with steel fibres : Mix proportions o f SCUHPC and SCUHPFRC mixes (kg) meeting the flowability, cohesiveness and passing ability criteria : Different values for parameter B available in the literature : Different values for parameter C available in the literature : Equations of the viscosity of suspensions based on volume concentration of solid particles : Estimated plastic viscosity of the paste. The superplasticiser to water ratio is 0.02 (0.03 for Mix3) and the superplasticiser to cement ratio is : Mix combinations based on the seven base mixes and the first and second fibre parameters; p / / and l/ln(21d) : Volume fractions of the SCHPFRC and SCHPC mix constituents : Volume fractions of the SCUHPFRC and SCUHPC mix constituents : Plastic viscosities of SCHPC and SCUHPC mixes with and without fibres : Measured and simulated T500 for SCC mixes XXI
24 6.2: Simulated T200, T400 and leveloff time for SCC mixes : Slump flow time ( T ) for SCHPFRC and SCUHPFRC mixes with different volume fractions of steel fibre and target plastic viscosities : Lbox simulations of SCHPFRC and SCUHPFRC mixes giving T 2 0 0, T and the leveloff times : Typical mix proportions of SCHPFRC mixes with ^ = 0.5 % : Typical mix proportions of SCHPFRC mixes with #f =l% : Typical mix proportions of SCUHPFRC mixes with ffy=1.5% : Typical mix proportions of SCUHPFRC mixes with j f =2% : Typical mix proportions of SCUHPFRC mixes with #f =2.5% : Typical mix proportions of SCUHPFRC mixes with ^ = 3 % : SCUHPFRC constituents XXII
25 C hapter 1 Introduction
26 C hapter 1: Introduction 1.1 Research background Reinforced concrete is one of the most versatile and widely used construction materials on the planet. With new structural demands due to more and more ambitious design, the reinforcement in concrete structures is becoming extremely dense and clustered. With such dense rebar arrangements, it is becoming increasingly harder to pour and fully compact the concrete into the formwork. As a result of the poor placement, compaction and homogeneity of concrete, the mechanical characteristics and the visual appearance of reinforced concrete structures are affected. The aforementioned difficulties resulting from the passing and flowing restrictions introduced by high percentage of reinforcement are overcome by the use o f selfcompacting concrete (SCC). The selfcompacting concrete is a comparatively new type o f concrete that differs from the conventional vibrated concrete in that it contains a superplasticiser and a stabiliser, which contribute significantly to increasing the ease and rate of its flow. A selfcompacting concrete can fill any part of formwork only under its own weight, without the need for compaction or external vibration. It was first developed in Japan in 1988 and spread to Europe through Holland and Sweden in the 1990s. It is a good alternative to conventional concretes in structural elements of complex and difficult shapes, e.g. very thin or curved members, in which the conventional concrete maybe difficult to compact, especially in the presence of congested reinforcement. Moreover, SCC offers many health and safety benefits. The elimination of vibratory compaction on site means that the workers are no longer exposed to vibration and its related illnesses, e.g. white finger syndrome, besides providing a quieter working environment. Despite its many advantages, such as good filling ability, passing ability and segregation resistance, normal SCCs are still prone to low durability and low tensile capacity in a similar manner to conventional vibrated concrete. Over the past few decades many researchers have explored ways of overcoming the drawbacks of conventional vibrated concretes. The majority o f work done in this field is related to changing the constituents of the vibrated concrete to improve the interfacial bond between the mortar matrix and aggregates. The concretes so produced are the socalled high performance concretes (HPC). In order to produce a HPC some modifications need to be made to both the mixing and curing processes. The benefits of using HPCs are compaction Page 2
27 Chapter 1: Introduction without segregation, higher tensile capacity, toughness, early age strength, high compressive strength (from 40 MPa for normal concretes to about 80 MPa for HPCs), etc. An alternative in the advancement of concrete technology is to combine the important characteristics of the conventional vibrated HPC and the SCC to produce selfcompacting high performance concretes (SCHPC). The major disadvantage of a HPC, namely its low flowability and filling ability, is overcome by using a viscosity modifying admixture (VMA) or superplasticiser, while cement replacement materials (CRM) e.g. ground granulated blast furnace slag, fly ash and/or silica fume are used to overcome the drawbacks o f the SCC, i.e. its low strength and durability. Even the SCHPC has low tensile strength and low strain capacity. To overcome this, short steel fibres can be added to SCHPC to increase its ductility and energy absorption capacity, thereby improving its durability. Selfcompacting high performance fibre reinforced concretes (SCHPFRC) exhibit a significant strainhardening response that leads to an improvement in their tensile strength and toughness in comparison with normal SCHPCs. To improve the performance further selfcompacting ultrahigh performance fibre reinforced concretes (SCUHPFRC) can be produced through the use o f only fine quartz sands as aggregates, a high content o f cement and silica fume (or CRMs), a high dosage of an effective superplasticiser (preferably based on polycarboxylic ethers) and short steel fibres. An example of the ultrahigh performance fibre reinforced concrete (UHPFRC) is CARDIFRC. CARDIFRC is characterised by high compressive strength (in excess of 200 MPa), high splitting/flexural strength (up to 30 MPa) and high energy absorption capacity (in excess o f 17,000 J/m2). The matrix contains only very fine graded quartz sand and about 6% of short steel fibres o f two lengths (6 and 13 mm long, 0.16 mm diameter). The mix without the fibres is very dense, viscous and flowable, and thus has the potential for selfcompaction. The mixture of SCC is strongly dependent on the composition and characteristics of its constituents in the fresh state. The properties of SCC in its fresh state have a great effect on its properties in the hardened state. Therefore it is critical to understand its flow behaviour in the fresh state. As the SCC is essentially defined in terms of its flowability, the characterisation and control of its rheology is crucial for its successful production. This is even more relevant if the fibres are added to SCC. Selfcompacting high and ultrahigh performance fibre reinforced concretes (SCHPFRC/SCUHPFRC) must maintain their flow Page 3
28 Chapter 1: Introduction ability and passing ability despite the presence of a large volume fraction of fibres. This presents a challenge which makes the control of rheology crucial for the successful production o f SCHPFRC/SCUHPFRC. The flow o f all SCCs with or without fibres is best described by the Bingham constitutive model (Dufour and PijauderCabot, 2005). This model contains two material properties, namely the yield stress and the plastic viscosity. It is known however that the yield stress of SCC mixes is low in comparison with normal vibrated concretes and remains nearly constant over a large range of plastic viscosities. The viscosity o f a homogenous viscous fluid such as the cement paste can be measured accurately which cannot be said o f any SCC. 1.2 Research objectives The objectives of this thesis are as follows: To produce high and ultra high performance selfcompacting concretes with and without short steel fibres, which exhibit good flowability, good cohesiveness and passing ability. To predict the plastic viscosity o f the high and ultra high performance selfcompacting concretes with or without steel fibres from the knowledge of the plastic viscosity o f the paste alone using appropriate micromechanical models and to validate these predictive models by comparing with real test data available in the literature. To model the flow behaviour of high and ultra high performance selfcompacting concretes with and without short steel fibres in two standard test configurations, namely the slump flow and Lbox tests using appropriate computational strategies. To provide guidance for proportioning the mixes of the high and ultra high performance selfcompacting concretes with or without steel fibres that have both flow and passing ability using the computational flow modelling technique at the mix design stage. Page 4
29 Chapter 1: Introduction 1.3 Research methodology To achieve the above objectives research is undertaken in four stages: First, high and ultra high performance selfcompacting concrete mixes with and without short steel fibres are developed by trial and error. For the SCC mixes without steel fibres the fulfilment of the flow and cohesiveness criteria is checked for each trial mix design by the slump flow test. The design o f SCC trial mixes with steel fibres is additionally tested to meet the passing ability criterion. Second, the plastic viscosity of the mixes with and without steel fibres is estimated from the known plastic viscosity of the cement paste. For this, concrete is regarded as a twophase suspension of solid and liquid phases. The liquid matrix phase consists of cement paste, i.e. cement and/or any superplasticiser or viscosity modifying agent (VMA). The plastic viscosity of this liquid matrix phase is assumed to be known, as it can be measured accurately. The increase in the plastic viscosity due to the addition of a solid phase (i.e. any cementreplacement materials, fine and coarse aggregates) to this matrix is predicted from a twophase model. The model is applied in several stages. The plastic viscosity of the viscous concrete consisting of the liquid and solid phases is further increased if steel fibres are added to it. This increase is quantified using a micromechanical model. Third, a Lagrangian particlebased technique, the socalled smooth particle hydrodynamics (SPH) method, is chosen for simulating the flow of SCC with or without steel fibres. An incompressible SPH method is applied to simulate the flow of these nonnewtonian fluids whose behaviour is described by a Binghamtype model. The plastic viscosity of the SCC is predicted using the procedures described above. The basic equations solved in the SPH are the incompressible mass conservation and NavierStokes equations. The results of the numerical simulation are benchmarked against actual slump flow tests carried out in the laboratory. Fourth, the SPH simulation technique is used at the mix design stage to provide guidance for proportioning the mixes of high and ultra high performance selfcompacting concretes, which meet the flow and passing ability requirements and have the desired plastic viscosity. Page 5
30 Chapter 1: Introduction 1.4 Outline of the thesis The contents of this thesis are organised into eight chapters, followed by bibliographical references. For clarity of presentation, each chapter is divided into sections and subsections, as required. In order not to interrupt the flow of the text in the main body of the thesis, all details have been relegated to appendices. A brief overview o f the contents of various chapters follows: Chapter 2 gives a general overview of SCC and its basic properties, materials used in its production and their influence on its characteristics in the fresh and hardened states and of the relevant workability tests on the fresh SCC. Also, some practical examples of structures made with SCC will be presented. Several tools which are available to address the workability o f SCC are reviewed in Chapter 3. These tools can be classified into two main groups: an empirical group, e.g. tools that model the flow of SCC, and the second based on the measurement o f the concrete flow. Both sets of tools will be reviewed. The rheology of cement paste, SCC and the methods of measurement of their rheological characteristics will be briefly discussed. Different methods of the simulation of the flow of SCC which are available in the literature will be reviewed. Chapter 4 describes the steps taken to develop selfcompacting high and ultrahigh performance concretes with and without steel fibres. In the design of such concretes, the flowability, good cohesiveness and passing ability criteria must be met. An extensive investigation will be carried out on the proportions of solids and liquids, the type of superplasticiser, and the steel fibres needed in order to produce SCC mixes with the right flow and passing ability. Chapter 5 describes micromechanical constitutive models used to predict the plastic viscosity of the high and ultrahigh performance selfcompacting concretes with or without steel fibres from the measured plastic viscosity of the paste. The concrete is regarded as a suspension in which the solid phase is suspended in a viscous liquid phase. The liquid matrix phase consists of cement, water and any viscosity modifying agent (VMA) to which the solids (fine and coarse aggregates and fibres) are added in succession. The predictions will be correlated with the available experimental data. Comments will be made on the practical usefulness o f the predicted plastic viscosity in simulating the flow of SCC. Page 6
31 Chapter 1: Introduction Chapter 6 is devoted to the simulation of the flow of high and ultrahigh performance selfcompacting concretes with or without steel fibres. An incompressible SPH methodology is adopted. The formulations relating to incompressible SPH and coupling of SPH formulation with a suitable Bingham model to represent the rheological behaviour of SCC will be briefly discussed and numerical results for SCCs flow with and without steel fibres will be compared with some available experimental observations. The basic equations solved in the SPH are the incompressible mass conservation and NavierStokes equations. Chapter 7 uses the SPH simulation technique as a practical aid in the proportioning of the mixes of high and ultrahigh performance selfcompacting concretes with or without steel fibres. Chapter 8 summarises the main conclusions on the basis o f the research work embodied in chapters 4 to 7, inclusive and also makes recommendations for future research. The thesis concludes with an alphabetical list of references to the works in the literature, cited in the text, and appendices. Some of the work described in this thesis has been published or is in the process o f publication. For easy reference, the publications are listed below. 1. Ghanbari A, Karihaloo B L. Prediction of the plastic viscosity o f selfcompacting steel fibre reinforced concrete, Cement and Concrete Research 2009;39(12): Kulasegaram S, Karihaloo B L, Ghanbari A. Modelling the flow of selfcompacting concrete, International Journal fo r Numerical and Analytical M ethods in Geomechanics 2011 (in press) DOI: /nag Deeb R, Ghanbari A, Karihaloo B L. Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres, Cement and Concrete Composites (submitted). 4. Karihaloo B L, Kulasegaram S, Ghanbari A. Modelling the flow of selfcompacting concrete, ECCM 2010, Paris, CDROM Paper Kulasegaram S, Karihaloo, B L, Ghanbari A. Modelling the flow of selfcompacting fibrereinforced concrete, Proc 5th SPHERIC workshop, Manchester,U.K., June 2010, pp Ghanbari A, Karihaloo B L, Kulasegaram S. Prediction of the plastic viscosity of selfcompacting steel fibre reinforced concrete, Proc CONMOD2010, Lausanne June 2010, pp Page 7
32 C hapter 2 SelfCompacting Concrete
33 Chapter 2: SelfCompacting Concrete 2.1 Introduction The production of high strength concrete has always been one of the main objectives of concrete technologists. For over 20 years now, concretes with compressive strength of MPa have been used worldwide in tall buildings and bridges with long spans or in buildings in aggressive environments. Building elements made of such concretes are usually densely reinforced. The small spacing between the reinforcing bars may lead to defects in concrete (Dietz and Ma, 2000). Normally, vibration is used to achieve the required compaction, reduce the porosity and the air entrapped in the concrete. However, vibration of densely reinforced concretes is not an easy job even for skilled workers. The lack o f good vibratory compaction directly affects the mechanical characteristics of the concrete in its hardened state. Insufficient compaction will lead to the inclusion of voids, which not only results in a reduction in the compressive strength but also strongly influences the natural physical and chemical protection o f the embedded steel reinforcement afforded by the concrete (Gaimster and Dixon, 2003). If such a high compressive strength concrete is selfcompacting (SCC), the production of densely reinforced elements would be an easier task, thanks to the high homogeneity o f SCC. The selfcompacting concrete is a type of concrete which can fill the whole mould completely with a minimum of defects and which compacts under its own selfweight without vibration. The concrete so produced is sufficiently cohesive and flows without segregation or bleeding. The selfcompacting concrete was first developed in Japan (Ozawa et al., 1989) in the late 1980s to be mainly used for highly congested reinforced structures in seismic regions (Bouzoubaa and Lachemib, 2001). The hardened SCC is dense, homogeneous and can have the same engineering properties and durability as the traditional vibrated concrete. This chapter gives a general overview of SCC and its basic properties, materials used in its production and their influence on its characteristics in the fresh and hardened states. It also reviews the workability tests relevant to the fresh SCC. Also some examples of structures made with SCC will be presented. Page 9
34 Chapter 2: SelfCompacting Concrete 2.2 Historical development of selfcompacting concrete Research undertaken into underwater placement technology in the mid1980s in the UK, North America and Japan led to the production of concrete mixes with a high degree of washout resistance. This, in turn, led to the development of SCC with the concept being first initiated in Japan in the mid1980s (Gaimster and Dixon, 2003). It was recognised that the reduction in the number of skilled workers in the Japanese construction industry was leading to a reduction in the quality of construction work with subsequent knockon effects on the concrete durability (Okamura et al., 1998). A prototype of SCC was proposed in 1986 at the Tokyo University. The first model for proportioning SCC mixes was developed in 1988 using constituent materials readily used in conventional concrete (Ozawa et al., 1989). These mixes were to be used mainly for highly congested reinforced structures in seismic regions (Bouzoubaa and Lachemi, 2001). The main aims were to shorten the construction time, to avoid vibrating the confined zones which are rather difficult to reach, and to eliminate vibration noise especially at concrete product plants. The proportioning model performed satisfactorily with regard to the fresh properties and also to the longterm hardened properties, such as the shrinkage. The selfcompacting concrete technology spread to Europe through Holland and Sweden in the 1990s (Bennenk, 2005, Billberg 1999). In the beginning o f the 21st century, the SCC started to be of interest in the USA (Ouchi et al., 2003). However, the annual production of SCC indicates that challenges still need to be overcome (Thrane, 2007). The ways of producing SCC are quite different in various countries depending on the traditions and materials available. In the last two decades, the SCC has been developed further, utilizing various materials such as condensed silica fume (CSF), ground granulated blast furnace slag (GGBS) and pulverizedfuel ash (PFA). Today, the SCC is an important topic among researchers and industries in the field of concrete, although the overall production is still relatively small compared to the conventional vibrated concrete. The selfcompacting concrete amounted for less than 1% of the ready mix concrete production in Europe in 2004 (ermco.org, 2005). However, the SCC is now well established in a number of countries, such as Sweden and the USA. Page 10
35 Chapter 2: SelfCompacting Concrete 2.3 Definitions of selfcompacting concrete Researchers have defined SCC in several ways; some of these are listed below. Khayat et al (1999): a highly flowable, yet stable concrete that can spread readily into place and fill the formwork without any consolidation and without undergoing any significant segregation. Bartos and Marrs (1999): selfcompacting concrete is a type o f concrete which flows under its own weight, can fill any part of formwork without vibration (even in the presence of highly dense reinforcing bars) and maintains its homogeneity. Ozawa et al. (1989): selfcompacting concrete must have the following properties: Filling ability, i.e. without vibrating the concrete, the SCC has to fill any space within the formwork passing ability, i.e. a homogenous distribution o f the components o f SCC in the vicinity of obstacles; and resistance to segregation, i.e. the resistance of the components of SCC to migration or separation. Figure 2.1 shows how this definition is incorporated in a rational design model (Okamura et al., 2000). No Vibration SelfCompacting Concrete Resistance to Segregation Less Restriction to Design ss Restriction to Practice New Type of Structure Rational Construction System Rational Combination of Concrete & Steel Figure 2.1: Proposed rational model of Ozawa (After Ouchi, 1999) Page 11
36 C hapter 2: SelfCompacting Concrete 2.4 Basic properties of selfcompacting concrete Many workers involved in the development of SCC (Domone and Chai, 1998; Okamura, 1999; Ozawa et al., 1990) have recognised that there are three fundamental factors that govern the fresh concrete properties: (i) Properties of the mortar; (ii) Volume of coarse aggregate in the mix; (iii) Use o f a superplasticiser to enhance workability. The properties o f the paste and mortar have important effects on the SCC properties, as with conventional vibrated concrete. The water to binder ratio primarily determines the workability o f the mix, as will the proportion of sand in the mortar (Okamura, 1999). The volume content of coarse aggregate in the concrete not only affects the workability but plays a major role in the segregation resistance of the mix. Okamura and Ozawa (1995) have employed three key procedures to attain selfcompacting ability: limited coarse aggregate content, low water to powder ratio, and use of superplasticiser. Today, the new generation of superplasticisers, the polycarboxylate ethers (see Section 2.7), gives improved workability retention to the cementitious mix. These superplasticisers disperse the cement by steric stabilization, which is more powerful compared to the electrostatic repulsion of older types of plasticisers (Yamada et al., 2000, Flatt, 2004a). Figure 2.2 shows a typical comparison of mix proportioning for SCC and normal vibrated concrete. As can be seen the cementitious component of the SCC is larger than that in the conventional concrete with a consequent reduction in the volume fraction of the coarse aggregate. Page 12
37 Chapter 2: SelfCompacting Concrete Normal Vibrated Concrete V/o 10% 18% 25% 45% Cement W ater ; 1 1I' 1 % 1 1 : \ \ Fin 3 t1 1 \ 1 I 1 \ t1 1 t1 t IFines', % % c Aggregsite \ % * % Coarse Aggregate 10% 18% 8% 26% 36% 2% SelfCompacting Concrete Figure 2.2: A typical mix proportioning of SCC and normal vibrated concrete The selfcompacting concrete offers many important advantages in comparison with a conventional vibrated and high performance concrete. It can fill all the formwork spaces without internal vibration, reducing labour time and improving the surface finish. The use of SCC leads to an overall cost reduction with improvements in the quality o f the structure and construction environment. To be selfcompactable a concrete should have a paste with high deformability for ease of flow around rebars, as well as resistance to segregation between the coarse aggregate and the paste during the flow (Okamura and Ouchi, 2003a). These requirements may seem to be contradictory because for high deformability, a high water content would seem necessary, resulting in a paste with low viscosity and hence a concrete prone to segregation. The selfcompacting concrete is able to flow under its own weight and achieve full compaction, even in the presence of congested reinforcement such as in mat foundations and momentresisting frames. The hardened concrete is dense, homogeneous and can have the same engineering properties and durability as the traditional vibrated concrete. The selfcompacting concrete improves the efficiency at the construction sites, enhances the working conditions and the quality and the appearance of concrete. The key difference in the production o f SCC in comparison to other types o f high performance concrete (HPC) is the use of a superplasticiser and/or a viscosity modifying agent and cement replacement materials in its composition to effectively stabilise the rheological properties o f SCC. An alternative in the advancement o f Page 13
38 Chapter 2: SelfCompacting Concrete concrete technology is to combine the important characteristics of the conventional vibrated HPC and the SCC. As a result, new types of concrete are being developed in order to meet the increasing demand for improved mechanical properties and durability. These new types of concrete are known as selfcompacting high performance concrete (SCHPC) and selfcompacting ultra high performance concrete (SCUHPC) (compressive strengths of MPa). Figure 2.3 compares typical volume fractions o f constituents in conventional HPC, SCC and their combinations. HPC SCC aggregates 52% water+sp 10% powder 18% sand 18% water+sp coarse 18% aggregates 36% powder 18% sand 26% SCHPC SCUHPC coarse aggregates 24% sand 28% water+sp 14% powder 42% Figure 2.3: Typical volumes of constituents in normal HPC and SCCs Page 14
39 Chapter 2: SelfCompacting Concrete The application o f SCC has benefits related to: Productivity, i.e. lower production costs, and a higher casting rate; Working conditions due to the reduced noise and dust emissions; Casting conditions, i.e. casting o f denselyreinforced sections and remote casting; Environmentfriendly production, e.g. the filler and aggregates can be waste/recycled materials; Elimination of the effect of vibration (which affects the quality of normal vibrated concrete); Homogeneity o f concrete, a better visual appearance, a lower variation of strength and a more durable concrete. 2.5 How to achieve the required properties of selfcompacting concrete? As can be seen from Figure 2.4, in order to produce a nonvibrated concrete, the fresh concrete must show both high fluidity and good cohesiveness without segregation o f the constituent materials. Limiting the coarse aggregate content and reducing the water to powder ratio, will achieve high viscosity and avoid collision between the coarser particles (Utsi, 2008). The addition o f superplasticiser will ensure the flowability o f the viscous paste. High Deformability Lim ited Aggregate content SelfCom pactability Effect of HWRA High Resistance to Segregation Reduced w/pratio Figure 2.4: Methods to achieve selfcompacting ability (After Ouchi et al., 1996) Page 15
40 Chapter 2: SelfCompacting Concrete To achieve selfcompacting ability o f concrete, different design approaches are followed in different countries. These approaches aim to optimize three aspects of the fresh concrete. Firstly, the paste content; by introducing a superplasticiser that significantly affects the structure of the powders by dispersing the cement grains and reducing the water to binder ratio. Secondly, the aggregate skeleton; in order to obtain higher packing density, the maximum aggregate size is decreased and crushed aggregates are replaced with round ones. Thirdly, some cement is replaced by viscosity modifying agents and/or fillers to fill the interstices of the granular skeleton thereby increasing the viscosity o f the mix and reducing the cost o f concrete. The selfcompacting concrete can be distinguished on two levels: first, all solids (powders and aggregates) are suspended by water and superplasticiser and second, aggregates are lubricated by cement paste. An excess o f the fluid reduces the friction by separating the solids with a small layer of either water or cement paste. Figure 2.5 shows the formation o f layers o f cement paste around aggregates. The thickness o f the paste layer can be best related to the diameter of the aggregates (Oh et al., 1997). Thickness of \ excess paste Figure 2.5: Excess paste layer around aggregates (After: Oh et al., 1997) Selfcompacting concrete mixtures are usually designed with higher volumes of paste than vibrated concrete mixtures. An excess of paste has to be added to keep the solid particles apart and to reduce the friction between the aggregates. The cement paste thus has a filling, a binding, and a smearing role in the SCC (Ma et al., 2003). 2.6 D ifferen t m ix designs o f selfco m p actin g c o n c re te Three different types o f SCC can be distinguished depending on the method of providing viscosity. Page 16
41 Chapter 2: SelfCompacting Concrete 1. Powdertype SCC. This was the first proposed prototype of SCC. It is characterized by a high powder content and low water to powder ratio. The requirements for this type are (i) increasing the plastic viscosity by limiting the free water content, and (ii) using a superplasticiser to provide consistence. Because of the high powder content, powdertype SCC mixes are sensitive to changes in the constituent materials. Usually cement replacement materials are used to control the strength and heat of hydration. Due to the low water to powder ratio, such SCCs are predicted to have a high strength and shrinkage, and low permeability. Okamura and Ozawa (1995) proposed a simple mix proportioning system for this type of SCC (Figure 2.6). According to their method, the coarse and fine aggregate contents are fixed and the selfcompacting ability can be obtained by adjusting the water to powder ratio and the amount o f superplasticiser. A typical procedure is 1) The coarse aggregate content is fixed at 50% of the solid volume; 2) The fine aggregate content is also fixed at 40% of the mortar volume; 3) Depending on the properties of mortar, the water to powder ratio is in the range of ) The selfcompacting ability is achieved by adjusting the superplasticiser dosage and the final water to powder ratio. I Limited Gravel Content \ 50% of solid volume Appropriate Mortar  Limited Sand Content j 40% of mortar volume Higher Deformability Moderate Viscosity Higher dosage of SP Lower W/C Figure 2.6: A typical mix design of SCC based on the Okamura and Ozawa procedure (Brite, 2000) Page 17
42 Chapter 2: SelfCompacting Concrete 2. VMAtype SCC is characterized by a high dosage of a viscosity modifying agent (VMA), which is added primarily for increasing the plastic viscosity. Compared with the powdertype SCC, the VMAtype SCC requires a higher superplasticiser dosage or water to powder ratio to obtain the required filling ability. The powder content is less because the viscosity is controlled by the addition o f VMA. 3. Combinedtype SCC was developed to improve the robustness of powdertype SCC by adding a small amount of VMA. In such mixes, the VMA content is less than that in the VMAtype SCC and the powder content and water to powder ratio are less than those in the powdertype SCC. The viscosity is provided by the VMA along with the powder. This type o f SCC was reported to have high filling ability, high segregation resistance and improved robustness (Rozie're et al., 2007). 2.7 S u p e rp la stic ise r The demand for a high level o f workability, together with good stability o f the mix for SCC has led to the use o f a number of admixtures. The advent o f superplasticisers and the developments in the admixture technology have made the production o f SCC easier, and as a result a variety of materials may be used. There are mainly four categories of superplasticiser, namely the sulfonated melamine formaldehyde condensates (plasticiser), sulfonated naphthalene formaldehyde condensates, modified lignosulfonates, and carboxylated acrylic ester copolymers or polycarboxylic ethers (Kong et al., 2003). Figure 2.7 shows the progression in the development of admixture technology. Polymer modified Poly Super super carboxylic Plasticiser plasticisers plasticisers ethers 1960s 1970s 1980s 1999 Figure 2.7: Development in admixture technology (After Dransfield, 2003) Page 18
43 Chapter 2: SelfCompacting Concrete The advances in admixture technology have played a vital part in the development of SCC. Modem superplasticisers (based on polycarboxylic ethers) promote good workability retention and can be added at any stage of the batching cycle. They contribute to the achievement of denser packing and lower porosity in concrete by increasing the flowability and improving the hydration through greater dispersion o f the cement particles, and thus assisting in producing SCCs o f high strength and good durability Action of superplasticisers The use of superplasticisers improves the flowability o f SCC by their liquefying and dispersing actions. In addition, a superplasticiser deflocculates the cement particles and frees the trapped water by their dispersing action and hence enhances the flowability of SCC. Due to the dispersing action, the interparticle friction and, thus, the flow resistance are also decreased, thus improving the flowability o f concrete. As stated by Dransfield (2003), this is analogous to the situation where people are walking both ways along a narrow pavement. If groups of people walking in one direction hold hands, then it is hard for people walking the other way to pass, especially if they are also holding hands. If everyone stops holding hands and walking in groups, then it is easy for people going in opposite directions to move round each other and pass. Admixtures adsorb on to the cement surfaces and break up the floes, leaving individual cement grains, which can pass each other easily, making the mix more fluid (Figure 2.8). Dispersing admixture Adsorbs on cement grains Cement floes reduce fluidity Cement uniformly dispersed increasing fluidity Figure 2.8: Effect of dispersing admixtures in breaking up cement floes (After Dransfield, 2003) Page 19
44 Chapter 2: SelfCompacting Concrete 2.8 Cement replacement materials and microsilica Cement replacement materials A selfcompacting concrete requires a high amount of flowability that can easily be achieved by the addition of a superplasticiser to the concrete mixture, as stated earlier. However, for such a concrete to remain cohesive during the flow, special attention has to be paid to mix proportioning. To avoid segregation following the addition o f a superplasticiser, a simple approach is to increase the sand content, whilst at the same time to decrease the coarse aggregate content. But the reduction in the coarse aggregate content results in the use of a high volume o f cement which has the disadvantage related to a higher temperature rise during hydration and an increase in the cost. An alternative approach is to incorporate a viscositymodifying admixture to enhance the stability, i.e. cohesiveness (Khayat and Guizani, 1997). Chemical admixtures are, however, expensive, and their use may increase the cost of concrete. Although savings in labour cost might offset the increased material cost, the use of cement replacement materials (CRM) or mineral admixtures in SCC is a better way to impart high workability to the mix, as well as to reduce the total cost of SCC. Cement replacement materials, sometimes also called mineral admixtures, are added to concrete as part of the total cementitious system. They enhance selfcompacting ability, fluidity, cohesiveness, segregation resistance and limit heat generation during hydration. The CRMs may be used in addition to, or as a partial replacement of, Portland cement in concrete depending on the properties of the materials and the desired effect on concrete (Mindess et al., 2003). The mineral admixtures are generally industrial byproducts and have therefore economic and environmental benefits. The slow rate of setting and hardening associated with the incorporation of CRMs in concrete is advantageous, if durability is the primary interest. The CRMs are less reactive than cement and can reduce problems resulting from the loss of fluidity of a rich concrete. Two of the most commonly used CRMs are the ground granulated blast furnace slag (GGBS) and pulverised fuel ash or fly ash (FA). These additives can be used as binary, ternary (two CRMs in a single mix) and quaternary mixtures. Page 20
45 Chapter 2: SelfCompacting Concrete G round granulated blast furnace slag The ground granulated blast furnace slag is one of the CRMs widely used in the production of SCC. It is a byproduct from the blast furnaces used to make iron. It is classified by EN and EN (or BS 6699) according to its level o f reactivity. The powder is about 10% less dense than Portland cement. For equal mass of the total binder (i.e. cement plus GGBS) content in the concrete, the GGBS will produce a larger volume of the binder paste increasing the segregation resistance and making the concrete easier to work, pump, place and compact. Finer particles in the GGBS (compared with the Portland cement) can also reduce bleeding. The use o f GGBS as a CRM in SCC has benefits related to the protection against both sulphate and chloride attack. However a SCC made with GGBS sets more slowly. The setting time depends on the amount of GGBS used. The SCC containing GGBS gains strength over a longer period of time; this results in a lower heat o f hydration and a lower temperature rise. Depending on the desired properties, the amount of GGBS can be as high as 50 per cent by mass o f the total cementitious material content (Ramachandran et al., 1981). The use of GGBS lowers concrete permeability, thereby reducing the rate of chloride ion diffusion (Russell, 1997). A proper combination o f the Portland cement and GGBS can eliminate the need to use low alkali or sulphateresistant cements. As reported by Russell (1997), replacing the Portland cement by 2 0 to 30 per cent of GGBS by mass can enhance the strength gain when the concrete is older than 28 days. Sobolev (1999) studied the effect of adding up to 50% by mass GGBS to the cementitious material and reported that it resulted in an increase of chemical and thermal resistance. A high proportion of GGBS may affect the stability of SCC resulting in reduced robustness with problems o f consistence control, while slower setting can also increase the risk o f segregation (EU Guidelines for SCC, 2005). Druta (2003) reported no visible destruction in concrete samples containing GGBS after 140 cycles o f freezing and thawing and also a high resistance to elevated temperatures. Page 21
46 Chapter 2: SelfCompacting Concrete Fly ash Fly ash (also known as pulverised fuel ash) is a byproduct of coalfired electricity generating plants. The ash is produced during the combustion o f ground or powdered coal. Due to its pozzolanic properties, the fly ash can be used as a replacement for some of the Portland cement content in SCC. The fly ash for use in Portland cement concrete conforms to the requirements of ASTM C 618, standard specification. According to the type o f coal used in the power station, there are two classes of fly ash, i.e. class C fly ash and class F fly ash. The class C fly ash is produced from the burning of younger lignite or subbituminous coal. This class generally contains more than 20% lime (CaO). The class C fly ash is preferable in the green building application. The class F fly ash is obtained from the burning of harder, older anthracite and bituminous coal. This fly ash is pozzolanic in nature and contains less than 20% lime (CaO). The use o f fly ash as a partial replacement for Portland cement is generally limited to Class F fly ash. It can replace up to 30% by mass o f Portland cement, and can add to the final strength o f the SCC and also increase its chemical resistance and durability. Due to the spherical shape o f fly ash particles, they can also increase the workability of SCC mixtures, while reducing the water demand. The fly ash reduces segregation and bleeding and lowers the heat of hydration. Concrete mixes containing the fly ash reach their maximum strength more slowly than concretes made with only Portland cement. The investigations by Bouzoubaa and Lachemib (2001) show that the use of fly ash and blast furnace slag in SCC reduces the dosage of superplasticiser needed to obtain slump flow spread comparable to that of the concrete made with Portland cement only (Yahia et al., 1999). Also, the use o f fly ash improves the rheological properties and reduces the thermal cracking o f concrete due to the heat of hydration (Kurita and Nomura, 1998). Kim et al. (1996) studied the properties of superflowing concrete containing fly ash and reported that the replacement o f 30% cement by fly ash resulted in excellent workability and flowability. Page 22
47 Chapter 2: SelfCompacting Concrete Chindaprasirt et al. (2005) reported that the use o f fly ash increased both the initial and final setting times of fly ashcement pastes due to the smaller surface area of fly ash particles (adsorbing less free water from the mixture). Due to the higher free water content, the powder concentration decreases. The addition of lime powder (LP) enhances the rate of hydration. A ternary mixture o f fly ash and lime powder showed better flowability and deformability/workability compared to brick powder and kaolinite. The lime powder is the finest and the fly ash is the coarsest admixture. An increase of 5% in the LP content reduces the flow time and increases the relative spread o f the mix. An increase of LP content beyond 50% is not advantageous as the compressive strength begins to decrease sharply. A partial replacement of cement by fly ash results in a higher volume o f paste due to the lower density of FA. This increase in the volume of the paste reduces the friction at the fine aggregatepaste interfaces, and improves the plasticity and cohesiveness o f the mix, leading to increased workability. Therefore, the fineness of the CRMs is not the only parameter to improve the workability Microsilica Microsilica (MS) or silica fume (SF) is a byproduct of the manufacture of silicon metal and ferrosilicon alloys. It is a very fine almost pure silica (SiCh) powder collected from the exhaust gases consisting mainly of spherical particles or microspheres o f mean diameter about 0.15 microns. Each microsphere is on average 100 times smaller than an average cement grain. At a typical dosage of 10% by mass of cement, there will be 50, ,000 microsilica particles per cement grain. Because of its extreme fineness and high silica content, microsilica is a very effective pozzolanic material. Standard specifications for microsilica used in cementitious mixtures are given in ASTM C l240 and EN Microsilica is one o f the most effective and widely used fines that is added to SCC to improve its properties, in particular its compressive strength, bond strength, and abrasion resistance. It also significantly reduces the concrete permeability by blocking the capillary channels. Page 23
48 Chapter 2: SelfCompacting Concrete Microsilica increases the yield stress o f a SCC mix thus decreasing the slump flow and segregation (Carlsward et al., 2003). It also reduces the ionic strength of the pore solution leading to a reduced consistence loss (Bonen and Sarkar, 1995). In the case of Portland cement, 18% microsilica (by weight of cement) is theoretically enough for the total consumption of calcium hydroxide (Papadakis, 1999) produced during the primary reaction of cement with water. However, as the small microsilica particles also physically fill the pores, more than 25% microsilica should be added to concrete to get the densest granular mixture (Richard and Cheyrezy, 1995). An excessive use of microsilica in the SCC can be counterproductive because of the difficulty in attaining the desired workability (Hassan et al., 2010). Khayat et al. (1997) have studied the influence o f microsilica blended with cement on some of the properties of fresh and hardened concretes. The properties studied were bleeding, slump loss, compressive strength and setting time. A total of 26 mixtures were developed. One half o f the mixtures were airentrained and had watercement ratios ranging from 0.3 to 0.6. The remaining half contained non airentrained mixtures and the watercement ratios varied between 0.45 and 0.7. Their study revealed that the addition o f small percentages of microsilica, usually less than 1 0%, and of a proper amount of high range water reducing admixture (superplasticiser) could decrease the viscosity of the paste, thus reducing the water demand and the risk o f bleeding. The small particles o f microsilica can displace some of the water present among flocculated cement particles and fill some o f the voids between the coarser particles, which otherwise can be occupied by some of the mix water. This causes some gain in workability and in the densification of the fresh paste. Concrete mixtures made with blended microsilica cement exhibited substantially less bleeding than those made with type I Portland cement. In addition, mixtures made with blended microsilica cement showed 15 to 2 0 mm greater loss o f slump than concretes without microsilica. In general, concrete mixtures made with type I Portland cement and blended microsilica cement exhibited initial times of setting that were within one hour apart. When 15% of microsilica was added with a high dosage of superplasticiser, initial and final times of setting were delayed by approximately 1 and 2 hours, respectively (Liu, 2009). Regarding the compressive strength, Khayat et al. (1997) found out that after three days of curing, no effect of cement type was observed on the development of compressive strength for concretes. However, starting with the seventh day, mixtures containing blended microsilica cement exhibited Page 24
49 Chapter 2: SelfCompacting Concrete greater strength than those made with type I Portland cement. After 28 days, in nonairentrained concretes, the use of blended microsilica cement resulted in approximately 2 0 % better strength gain compared with mixtures containing only Portland cement. Similar results were obtained in airentrained concrete. Duval and Kadri (1998) studied the influence of microsilica on the workability and compressive strength o f concretes. The concretes that have been investigated had low watercement ratios (0.25 to 0.40). The type I Portland cement was replaced by 1030% by mass microsilica, and superplasticiser was added. It was found that microsilica increased the compressive strength at most by 25%, but the workability o f concretes was best when its content was between 4 and 8 %. Duval and Kadri also found out that if microsilica exceeds 15% o f the cementitious material, both compressive and tensile strengths are reduced. Carl sward et al. (2003) observed a decrease of slump flow with an increase in the microsilica content in all of their workability tests. Regarding the Theological parameters, the general tendency was an increase in the yield stress with an increase in the microsilica content. Vikan and Justnes (2003) also observed the same effect on the yield stress Benefits of CRMc In summary, the benefits of CRMs to concrete (besides the obvious economic and environmental ones) are as follows: The placing and compaction are made easier thus giving better workability; The durability o f concrete is increased because of the retardation in the early setting time with a better long term strength; The risk of thermal cracking in large pours is reduced, because of lower earlyage temperature rise due to hydration; The resistance to attack by sulphate and other chemicals is increased; The risk o f reinforcement corrosion is reduced. 2.9 Effect of fibres on the behaviour of fresh selfcompacting concrete The modem development of steel fibre reinforced concrete may have begun around the early 1960s. Polymeric fibres came into commercial use in the late 1970s; glass fibres experienced Page 25
50 Chapter 2: SelfCompacting Concrete widespread use in the 1980s, and the carbon fibres attracted much attention in 1990s. The main application o f steel fibre reinforced concrete (SFRC) is in structures subjected to potentially damaging concentrated and dynamic loads. The steel fibre reinforced concrete has been used in several areas of infrastructure and industrial applications such as airport pavements, industrial floors, overlays, and channel linings, where laboratory tests and field applications have shown SFRC to be more durable than plain concrete subjected to high velocity water flow (Aydin, 2007). Fibres can be used in the SCC to extend the range o f its application and to overcome its drawbacks, namely the brittleness, as well as the volume changes which occur during the hardening o f the material, i.e. the autogenous shrinkage. Such fibre reinforced SCCs are called selfcompacting (high or ultrahigh performance) fibre reinforced concrete (SCFRC). Fibres bridge cracks and retard their propagation. They contribute to an increased energy absorption compared with plain SCC. In the past, steel fibres have been used to replace bar reinforcement, to decrease the width o f cracks and to improve the tensile strength or the postcracking behaviour (e.g. Benson and Karihaloo, 2005a,b). Both metallic and polymeric fibres have been used in the production of SCC, but they may reduce flow and passing ability. Trials are therefore needed to establish the optimum type, length and quantity o f the fibre to give all the required properties to both the fresh and hardened SCFRC. Steel and long polymer structural fibres are used to modify the ductility/toughness of hardened SCFRC. Their length L f and quantity V f are selected depending on the maximum size of the aggregate and structural requirements. The higher the aspect ratio (Lf/df) and the volume fraction of the fibres, the better is the performance of the mix in the hardened state. On the other hand, the higher the fibre factor (V f Lf/df) the more the slump flow is decreased. Before the addition of fibres the slump flow spread should be larger than 700mm. If the fibres are used as a substitute for normal reinforcement, the risk of blockage is reduced but it should be emphasised that using SCFRC in structures with normal reinforcement significantly increases the risk o f blockage (European Guidelines for SCC, 2005) Characteristics o f the fibres The mixture composition of fibre reinforced SCC is a compromise between the requirements in the fresh and the hardened states. The shape o f the fibres differs from that o f the Page 26
51 Chapter 2: SelfCompacting Concrete aggregates; due to the long elongated shape and/or a higher surface area, the workability of SCC is affected. The practical fibre content is limited; a sudden decrease of workability occurs at a certain fibre content, which depends on the mixture composition and the fibre type used. To optimise the performance of a single fibre, fibres need to be homogeneously distributed; clustering o f fibres has to be counteracted (EU Guideline for SCC, 2005). The steel fibre is the most common fibre type in the building industry; plastic, glass and carbon fibres contribute to a smaller part to the market. Also polymer fibres are mainly used to improve the stability o f SCC, as they help prevent settlement and cracking due to plastic shrinkage o f the concrete. In high and ultra high performance SCCFRC, polymer fibres maybe additionally needed as sacrificial fibres to achieve the required fire rating in these very dense mixes. The size of the fibres relative to that of the aggregates determines their distribution. To be effective in the hardened state it is recommended to choose fibres not shorter than the maximum aggregate size. Usually, the fibre length is 24 times that of the maximum aggregate size (Groth, ). The effect of aggregate size on the fibre distribution is shown in Figure 2.9. Maximum grain size 5 mm 10 mm 20 mm E o 40 mm Fibre length Figure 2.9: Effect of aggregate size on fibre distribution (After Johnston, 1996) The selfcompacting fibre reinforced concrete can maintain its flowability in spite of the addition of fibres. The slump flow decreases with the addition of fibres, also increasing the T500 time. The degree to which the steel fibres affect the slump flow and T500 depends on the Page 27
52 Chapter 2: SelfCompacting Concrete composition of the SCC mix (Saak et al., 2001). The effect of two types of polypropylene fibres on the characteristics of SCC in the fresh state was studied by Griinewald & Walraven (2003); these two were a monofilament and a fibrillated type. The selfcompacting concrete remained selfcompacting with the fibrillated type; the slump flow decreased from 710 to 620 mm. The monofilament type, on the other hand significantly decreased the slump flow to 440 mm due to the higher surface area. The effect of fibres on the workability of SCC is summarised below: The shape of the fibres is more elongated compared with the aggregates; the surface area at the same volume is higher; Stiff fibres change the structure of the granular skeleton, while flexible fibres fill the space between them. Stiff fibres push apart particles that are relatively large compared with the fibre length (i.e. the porosity o f the granular skeleton increases); Surface characteristics o f fibres differ from that of cement and aggregates, e.g. polymer fibres might be hydrophilic or hydrophobic; Steel fibres often are deformed (e.g. have hooked or crimped ends or are waveshaped) to improve the anchorage between the fibre and the surrounding matrix. The friction between hookedend steel fibres and aggregates is higher compared with straight steel fibres Properties of fresh selfcompacting concrete The selfcompacting concrete differs from conventional concrete in that its fresh properties are vital in determining whether or not it can be placed satisfactorily (Jacobs and Hunkeler, 1999). All the aspects of workability need to be fully controlled to ensure that its ability to be placed remains acceptable. These include the flowing ability, the passing ability, and the segregation resistance. Driven by its own weight, the concrete has to fill a mould completely without leaving entrapped air even in the presence o f dense steel bar reinforcement. The components have to be homogeneously distributed during the flow and at rest. Clustering of the aggregates in the vicinity of reinforcement (blocking) and separation of water or paste affect the characteristics o f SCC in the hardened state. Page 28
53 Chapter 2: SelfCompacting Concrete Flowing ability Without vibrating the concrete, the SCC has to fill any space within the formwork; it has to flow in horizontal and vertical directions without keeping air entrapped inside the concrete or at the surface. The driving forces of this process are the weight of the concrete and the casting energy. To achieve high flowing ability, it is necessary to reduce interparticle friction among solid particles (coarse aggregates, sand and powder) in the concrete by using a superplasticiser and a lower coarse aggregate content (Khayat, 1999, Sonebi and Bartos, 2005). Adding more water could improve flowing ability by decreasing interparticle friction, but it also reduces viscosity, thus leading to segregation. Too much water also leads to undesirable influences on the strength and durability. Unlike water addition, which reduces both the yield stress and viscosity, the incorporation o f a superplasticiser not only reduces the interparticle friction by dispersing the cement particles but also maintains the deformation capacity and viscosity. It also impairs the hardened properties less than does additional water. The particle size distribution also affects the flowing ability. Interparticle friction can be reduced by using continuously graded materials, aggregates and powder (Khayat, 1999, Sonebi et al., 2001) Passing ability Passing ability is required to guarantee a homogenous distribution of the components of SCC in the vicinity o f obstacles. The minimum bar distance to avoid blocking depends on the flowing ability o f the SCC, on the maximum aggregate size, the paste content and the distribution and the shape o f the aggregates (Khayat and Roursel, 2000). Blocking results from the interaction among aggregate particles and between the aggregate particles and reinforcement; when concrete approaches a narrow space, the different flowing velocities of the mortar and coarse aggregate lead to a locally increased content of coarse aggregate (Noguchi et al., 1999, Okamura and Ouchi, 2003b). Some aggregates may bridge or arch at small openings which block the rest of the concrete, as shown in Figure Page 29
54 Chapter 2: SelfCompacting Concrete Figure 2.10: Schematic of blocking (After RILEM TC 174 SCC, 2000) A reduction in the coarse aggregate content and in its size are both effective in preventing blocking. The paste volume o f the concrete is also an important factor in blocking (Billberg et al., 2004). Blocking depends mainly on the yield stress, whereas the plastic viscosity does not influence the passing ability o f the SCC. However, a paste with sufficient viscosity also prevents local increases in coarse aggregate volume, and hence blocking is avoided. As shown in Figure 2.11, the passing ability is therefore achieved by a reduction in the coarse aggregate size and content and by the use of VMA or by a proper selection o f the powder. powder or/and VMA Consistence retention Self com pacting Concrete Figure 2.11: Schematic of ways to achieve SCC (After Liu, 2009) Segregation resistance The segregation resistance is the resistance o f the components of SCC to migration or separation. Particles having a relatively high density or a low surface to volume ratio are Page 30
55 Chapter 2: SelfCompacting Concrete more prone to segregation. The segregation resistance o f SCC can be different under static (at rest) and dynamic (during the flow) conditions Tests on fresh selfcompacting concrete The rheological tests can be performed on a SCC mix using rheometers of different types. However these tests suffer for some drawbacks; they are not suited for use at the working site, and they can be rather timeconsuming (Utsi et al., 2003). Therefore, it is important to find suitable workability test methods for continuous use outside the laboratory, and to calibrate them with rheological parameters. For the SCC, a number of empirical workability tests (slump flow test, VFunnel, LBox test, UBox test, JRing, wet sieve stability and surface settlement tests) have been proposed and established in practice (Wu et al., 2009). Two aspects of SCC, the deformation capacity and deformation velocity, are evaluated by the workability tests. In this section, the workability tests which are recommended by the EN standard (EN 2069:2010) are discussed, namely the slump flow test for flowing ability, L box and JRing tests for passing ability, and visual examination and sieve stability tests for segregation resistance Flowability test Slump flow test The slump flow is a wellestablished test method. It is usually the test that accepts or rejects a mix at the working site (Utsi et al., 2003). The slump flow test, which is a modification of the traditional slump test, in which the spread of the material is measured instead of the height reduction, is the simplest and most commonly used test for evaluating the flowability of SCC (Pashias et al., 1996). The slump flow test evaluates the deformation capacity of SCC under its own weight without external forces against the friction o f the base plate. As shown in Figure 2.12, the slump flow is the diameter of the concrete flowing over a level plate after a slump cone is lifted. The larger the slump flow spread, the greater the deformation capacity of the concrete provided that no segregation occurs. T 5 0 0, the time from lifting of the cone to the concrete spreading to a 500 mm diameter, is used to indicate the deformation rate. The higher the T value, the lower the deformation rate of the concrete. T varies from 27 seconds in the case of fresh SCC (Neophytou et al., 2010). However the T500 value can be Page 31
56 Chapter 2: SelfCompacting Concrete difficult to measure especially the small values for the very flowable concrete (Carlsward et al., 2003) Figure 2.12: Apparatus for Slump Flow test (After David and Shah, 2004). All dimensions in mm Segregation can be visually evaluated by observing the flowing process and the edge of the spread after the concrete stops. The occurrence o f unevenly distributed coarse aggregate is considered as an indication of segregation, which demonstrates that the concrete segregates during the test and may segregate after placing. However the lack o f segregation during the slump flow test cannot ensure that the mix is resistant to segregation. It is therefore insufficient to detect segregation by visual observation only. The slump flow test in some respects is similar to the slump test performed on normal vibrated concrete except that no compaction is involved. Researchers have found a relationship between the slump and slump flow tests. However as shown in Figure 2.13, the bestfit relationship diverges at higher slumps. Page 32
57 Chapter 2: SelfCompacting Concrete Slump flow (mm) 800 i Domone (1998) Khayat et al. (1996) Kurokawa et al. (1994) Slump (mm) Figure 2.13: The relationship between slump and slump flow measurements (After Domone, 2003) Bouzoubaa and Lachemi (2001) have reported that the slump flow is determined primarily by the superplasticiser dosage; the water to powder ratio and the fly ash replacement content have only a secondary effect. However, Sonebi (2004) showed that the water to binder (cement+ fly ash) ratio had the greatest effect on the slump flow for SCC incorporating fly ash Is there any relationship between rheological characteristics of selfcompacting concrete and slump flow test measurements? In the slump flow test, the concrete stops flowing when the shear stress of the sample becomes equal to or smaller than the yield stress. This confirms that the yield stress must be the dominant factor that governs the slump flow spread. Several researchers have investigated the possibility that there exists a relationship between the rheological characteristics (yield stress and plastic viscosity) of a selfcompacting concrete and measured parameters in the slump flow test (namely, the diameter of slump flow spread and T500) (e.g. Thrane, 2007; Grunewald, 2004). The yield stress is defined as the critical shear stress required to initiate the deformation (flow), while the plastic viscosity Page 33
58 Chapter 2: SelfCompacting Concrete describes the resistance to flow once the yield stress is exceeded (more details of these two rheological parameters will be given in Chapter 3). In general, both the yield stress and the plastic viscosity increase with time, as the concrete hardens (de Castro and Liborio, 2006). Roussel et al. (2005) found an analytical correlation between the slump flow spread and the yield stress o f cement pastes. Roussel and Coussot (2005), and Roussel (2006) performed threedimensional simulations of the flow o f concrete in different slump tests. They concluded that slump flow depends only on the yield stress and the density of the SCC mix. Grunewald (2004) obtained a correlation between the slump flow and yield stress for different mixes o f selfcompacting fibre reinforced concrete (Figure 2.14). Yield value (Pa) O A % wo A V Slump flow (mm) Figure 2.14: A typical relationship between slump flow diameter and yield stress for different mixes of selfcompacting concrete (After Grunewald, 2004) Carlsward et al. (2003) concluded that the slump flow is dependent on both the yield stress and the plastic viscosity of the mix. Various concrete mixtures have been examined by Utsi et al., (2003) to find the possible relations between workability and rheology. The yield stress was found to be correlated to the Page 34
59 Chapter 2: SelfCompacting Concrete slump flow spread for stiff mixes (spread less than 600 mm) but not for mixes with flow spread in excess of this value. However, Esping (2007) carried out a set of tests on SCCs and found that the slump flow spread is not a unique function of the yield stress, but rather a more complex function of both the yield stress and plastic viscosity. The results o f Tregger et al., (2008) also suggest that the slump flow spread is a not unique function o f the yield stress. Another study by Tregger et al., (2007) revealed that the plastic viscosity of SCC is linked to the time required for slump flow test to reach its final spread but no reliable correlations were found. Roussel (2007a) showed that there is no correlation between the Bingham parameters (i.e. the yield stress and plastic viscosity) and the slump flow test and suggested alternate test methods. Reinhardt and Wustholz (2006) concluded that the plastic viscosity also affected the slump flow but the influence can be negligible compared to that of the yield stress and concrete density. Moreover they have stated that other factors such as the surface tension can also affect the measurements and should not be ignored. T has a good correlation with the plastic viscosity (R2>0.70) provided there is no segregation (Figure 2.15), but rather a poor correlation with the yield stress (R2 below 0.4) (The EU guidelines for SCC). 10 T ( s ) 8 O o 6 OO 4 O O Plastic viscosity (Pas) Figure 2.15: A typical relationship between flow time (T500) and plastic viscosity of SCC (After Grunewald, 2004) Page 35
60 Chapter 2: SelfCompacting Concrete Utsi et al., (2003) also obtained a correlation between T500 and the plastic viscosity for their stiffer mixes with slump flows below 600mm. Thrane (2007) has reported that Kurokawa et al. (1994) used the viscoplastic finite element method (VFEM; see Chapter 3) and obtained a relation between the T500 and the plastic viscosity. From their experiments, Neophytou et al., (2010) conclude that T500 can only be used to estimate the plastic viscosity of a mixture with a constant yield stress, while the slump flow can be used to estimate the yield stress with constant plastic viscosity. There have been many attempts to correlate the rheological parameters of SCC to empirical test data. However correlations of this type are highly dependent on the choice of materials and the devices for measuring the rheological parameters (i.e. different types of rheometers) and therefore it is not certain whether a relationship can be easily generalised. From the above literature review, it can be concluded that the T500 time can be related to the plastic viscosity but that the slump flow spread is a function of both the yield stress and the density o f SCC Passing ability tests Lbox test The Lbox test evaluates the passing ability of SCC in a confined space. The apparatus (Figure 2.16) consists o f a long rectangular trough with a vertical column/hopper at one end. A gate is fitted to the base of the column allowing discharge o f SCC into the horizontal trough. Adjacent to the gate is an arrangement of bars which permits assessment of the blocking potential to be made. Page 36
61 Chapter 2: SelfCompacting Concrete Figure 2.16: Schematic of Lbox (top), (After Thrane, 2007), with heights at either end of horizontal trough (bottom). All dimensions in mm The heights at either end o f the horizontal trough (Hi and H 2) can be measured to determine the levelling ability. The ratio of Hi to H 2 is called the blocking ratio. If the SCC has perfect fresh properties, the blocking ratio is equal to 1. Conversely, the blocking ratio is equal to 0 if the concrete is too stiff or segregated. An expression for the H 2/H 1 ratio can be obtained if the inertia is neglected and the gate in the Lbox is lifted slowly (Thrane, 2007; Thrane et al., 2004). Also the flow speed can be measured by the time taken to reach the distance o f 200 mm (T 2 0 0) or 400 mm (T 4 0 0) from the gate. Lboxes of different sizes with different reinforcing bars and gaps were used by Bui et al. (2002), and Petersson (2003). Investigations have showed that the Lbox was sensitive to blocking and that it was more difficult for concrete to pass three rather than two bars (Sedran and De Larrard, 1999). The test depends on the operator, for example, in regard to the lifting speed o f the gate (Nguyen et al., 2006); if the gate was lifted slowly and there was no segregation, the final shape of the concrete was determined by the yield stress and there were correlations between blocking ratio to the ratio Page 37
62 Chapter 2: SelfCompacting Concrete o f yield stress to specific gravity; the difference between two results with and without steel bars was small which according to Nguyen et al. (2006) can be used to detect dynamic segregation JR ing test This test is a variation to the Lbox test. Both tests are used to measure the passing ability of SCC through congested reinforcement. It comprises o f a ring with several reinforcement bars with an adaptable gap width. Diameter of the ring is 300mm and the height is 100mm. The slump cone is placed centrally in the JRing and filled with concrete, while pressing the slump cone to the base plate. The slump cone is lifted vertically, and the final diameter of the concrete spread is measured (the average o f two diameters measured in two perpendicular directions). The average difference of heights at four different locations is calculated; the greater the difference in heights, the lesser the passing ability o f concrete. The test equipment is shown in Figure A 300mm 15mm 100mm A 300mm Figure 2.17: JRing apparatus
63 Chapter 2: SelfCompacting Concrete Segregation tests Several empirical tests have been proposed to evaluate static segregation (i.e. at rest). However, no methods have yet been proposed for dynamic segregation (i.e. during flow) Visual examination The visual examination method (PCITR, 2003) is carried out by inspecting the periphery of the concrete after measuring the slump flow spread and rating it from 0 to 3. However it is an inadequate method because it relies on the experience of the performer and fails to evaluate segregation quantitatively Sieve stability test The potential for static segregation can be evaluated by a simple sieve stability test, which measures the amount of grains passing through a 5 mm sieve after a standard period, which is called sieve segregation or segregation index. The GTM Stability Sieving test (Cussigh, 1999) is used to measure the degree of separation o f the coarse aggregates and mortar fractions. In this test, 10 litres o f fresh SCC are placed into a test container and allowed to settle over a 15 minute period. The coarse aggregate settles at the bottom and the upper part of the concrete in the container is then wet sieved and the volume o f mortar calculated. The more the segregation has occurred the more mortar passes through the sieve, indicating a higher risk of segregation after the placement of SCC Examples of structures made with selfcompacting concrete Many structures have been designed throughout the world using the SCC. However the application of SCC at the building site is not yet widespread and is mostly limited to special structures. With the SCC it is possible to solve special problems, like those occurring in the case of special shapes of the concrete elements, congested reinforcement or casting in remote areas. In the following, some of these are highlighted. It should be mentioned that some of these projects would not have been possible without using a SCC. AkashiKaikyo (Straits) Bridge (Figure 2.18): It is a suspension bridge with the longest span in the world (1,991 meters). The volume of the cast concrete in the two anchorages amounted to 290,000 m3. The concrete was mixed at the batching plant beside the site, and was pumped out to the place. It was transported 200 meters through pipes to the casting site, Page 39
64 Chapter 2: SelfCompacting Concrete where the pipes were arranged in rows 3 to 5 meters apart. In the final analysis, the use of SCC shortened the construction period by 20% (Ouchi and HibinoNagaoka, 2000). Figure 2.18: Akashi Kaikyo (Straits) Bridge (After Ouchi and HibinoNagaoka, 2000) Midsummer place in London (Figure 2.19): The structure contains elliptical columns (8.5m to 10m high) with a highly dense reinforcement. This project reduced the construction period and expenses by 40% and 10%, respectively in comparison with normal concrete. Figure 2.19: Midsummer place in London (After Goodier, 2003) Other examples are an immersed tunnel in Kobe Japan (Goodier, 2003), Bunkers Hill in Calgary, Canada (Nmai and Violetta, 1996), and Landmark tower in Minato Mirai in Yokohama Japan (Billberg, 1999). Page 40
65 Chapter 2: SelfCompacting Concrete 2.13 Concluding remarks The selfcompacting concrete homogenously fills moulds of different shapes and geometry under its own weight, without any additional compaction energy. Building elements made of high strength concrete are usually densely reinforced. The small distance between reinforcing bars may lead to defects in concrete. If the high strength concrete is selfcompacting, the production of densely reinforced building element from high strength concrete with high homogeneity would ease the task (Ma et al., 2003). The use of SCC offers great opportunity for automated precast production. Not only will it reduce the unhealthy tasks for workers, it can also reduce the technical costs of in situ cast concrete constructions, due to improved casting cycle, quality, durability, surface finish and reliability o f concrete structures and eliminate some of the potential for human error (Esping, 2007). However, the annual production of SCC indicates that challenges still need to be overcome. According to the European Ready Mixed Concrete Organization, SCC amounted for less than 1% o f the ready mix concrete production in Europe in 2004 (ermco.org 2005). This chapter gave a general overview of SCC and the basic principles involved in its design. Different mix designs of SCC were introduced, i.e. powdertype SCC, VMAtype SCC and combinedtype SCC. The influence of cement replacement materials on the characteristics o f SCC was discussed with the emphasis on the fresh state of SCC. It was concluded that CRMs enhance selfcompacting ability, fluidity, cohesiveness, segregation resistance and limit heat generation during hydration. Tests to examine the workability of SCC, i.e. flowing ability, passing ability and segregation resistance of SCC were described, along with the possibility that relationships exist between the rheological characteristics (the yield stress and the plastic viscosity) of selfcompacting concrete and parameters measured in these empirical tests (such as the diameter of slump flow and Tjoo) It was however observed that there is as yet no consensus on such relationships. The effect of fibres on the SCC was reviewed. Fibres bridge cracks and retard their propagation. They contribute to an increase in the energy absorption compared with plain Page 41
66 Chapter 2: SelfCompacting Concrete concrete. The addition of fibres to SCC will lead to benefits in the fresh state and an improved performance in the hardened state, although the fibres greatly impair the workability o f SCC because of their elongated shape and large surface area. In order to make the best use of the fibres, they need to be homogeneously distributed in the mix without clustering. It was noted that the development of SCC has been closely related to the development of superplasticisers. The latter have a profound effect on the high level of workability of the SCC together with the good stability of the mix through liquefying and dispersing actions. Nowadays, the new generation of superplasticisers  the polycarboxylate ethers  give improved workability retention to the cementitious mix (Thrane, 2007). These superplasticisers disperse the cement by steric stabilisation, which is more powerful than the electrostatic repulsion o f older types o f plasticisers (Yamada et al., 2000, Flatt 2004a). In the next Chapter, we shall review the rheology o f SCC, and in particular introduce the Bingham model for describing its constitutive behaviour. We shall also review the computational techniques that are used to simulate the flow of SCC which is a non Newtonian fluid. Page 42
67 C hapter 3 An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow
68 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow 3.1 Introduction Over the past few decades, selfcompacting concrete (SCC) technology has advanced in a similar manner to many other aspects of concrete technology. Workable SCC mixes at lower water to binder ratios have been achieved through the use o f superplasticisers, thus increasing their compressive strength. The principles of rheology can be applied in the field of workability to explain the development and use o f test methods which give a more complete understanding o f the behaviour of the SCC. Several tools are available to address the workability of SCC. These tools can be classified into two main groups: empirical group e.g. tools that model the flow of SCC, and the second based on the measurement of concrete flow. Both sets of tools will be reviewed in this chapter. The field o f fluid mechanics that studies the relation between the applied stress and the resulting deformation of a fluid is called by the Greek word Rheology. The rheology of cement paste, SCC and methods o f measurement of their rheological characteristics will be briefly discussed. Different computational methods of simulation of the flow of SCC which are available in the literature will be reviewed and the equations used in the general flow simulation will be introduced. 3.2 Classification of workability The workability o f concrete can be studied at three levels as follows (Tattersall, 1991): Qualitative: studying the general behaviour of concrete without trying to quantify it, e.g. workability, flowability, pumpability, etc. Quantitative empirical: dealing with a simple quantitative behaviour, e.g. slump flow test, Lbox test, etc. Quantitative fundamental: studying the rheological characteristics, such as plastic viscosity, yield stress, fluidity, etc. The first two classes have been dealt with in Chapter two. In the following, the third class will be examined in more detail. 3.3 Rheological characteristics of selfcompacting concrete The mixture of selfcompacting concrete is strongly dependent on the composition and characteristics o f its constituents in the fresh state. The properties of SCC in its fresh state have a great effect on its hardened state. Therefore it is critical to understand its flow behaviour in the fresh state. As the SCC is essentially defined in terms of its workability, the Page 44
69 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow characterisation and control of rheology is crucial for the successful production of this type of concrete. However the measuring techniques in its fresh state have not changed significantly in the last two decades. The slump flow has for a long time been considered to be a unique function of the yield stress of a Bingham fluid, without being influenced by its plastic viscosity (Wallevik, 2006). But, as we have seen in the previous Chapter, this is still an unresolved question. In fact, concretes with the same slump spread may flow differently and have different workability (Ferraris, 2000); this is because concrete flow cannot be described by a single parameter. For a normal concrete, researchers have found that the flow of concrete can be defined reasonably well by using the Bingham constitutive model. This constitutive model is a linear representation o f the flow using two parameters, namely the shear stress (response o f the considered concrete) against shear rate. This relationship involves two main parameters, i.e. the yield stress and the plastic viscosity. 3.4 Measuring the rheological parameters The instruments that measure the relationship between the shear stress and strain rate are called rheometers or viscometers. To obtain the rheological characteristics of general viscous liquids (such as cement pastes) and solidliquid suspensions (such as selfcompacting concretes), a rheometer is to be used. Several types of this instrument have been proposed to evaluate the plastic viscosity and yield stress o f cementitious materials. Empirical techniques have also been proposed. The most basic type is the cup method, where the time that it takes to empty a cup with a defined hole in the bottom gives a measure o f the viscosity. Other types use a penetration rod, ball, etc., where a falling object with a defined density penetrates the sample. These types o f kinematic viscometers are only appropriate for making comparative studies, as the shear rate is not fully controllable (Esping, 2007) and they are therefore excluded from this review Rheology o f cement paste For testing viscous liquids (such as cement pastes) in which the maximum particle size is about 100 pm, the rheometer used is the socalled coaxial cylinder rheometer. In this type of rheometer the annular gap between the inner and outer cylinders can be of the order of few millimetres. A BML rheometer is the most common type for measuring the rheological Page 45
70 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow properties of cement paste. As shown in Figure 3.1, the inner cylinder is rotated and the torque imposed on the stationary outer cylinder is measured; other rotating and measuring arrangements are possible. 7 T S p e e d N In n e r cylin d er i I p m 1 1 S a m p le  O u te r cy lin d er T o rq u e (7") m e a s u r e m e n t Figure 3.1: A coaxial cylinder rheometer (After Domone, 2003) Let us consider the simplest mixture o f cement and water; both the yield stress and plastic viscosity of this mixture reduce with increasing water content. Figure 3.2 shows a fanshaped family of flow curves. As a result the extent o f changes in both the yield stress and plastic viscosity are comparable. Shear stress (x) % Increasing water/cement ratio Rate o f shear strain (f ) Figure 3.2: Fanshaped curves for different watercement ratio (After Domone, 2003) Page 46
71 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow Figure 3.3 shows a typical effect of watercement ratio on the Bingham constants for cement paste which confirms that adding or subtracting water leads to similar changes in both properties. Yield stress (Pa) 1000 Plastic viscosity (Pas) 100 J Water/cement ratio Water/cement ratio Figure 3.3: Typical effect of watercement ratio on Bingham constants for cement paste (After Domone and Thurairatnam, 1988) However when superplasticisers are added, the behaviour is somewhat different. Domone and Thurairatnam (1988) have used naphthalene formaldehyde superplasticisers in pastes with three different watercement ratios. As shown in Figure 3.4, increasing the dosage of superplasticiser leads to a reduction in both the plastic viscosity and the yield stress, however the reduction in the plastic viscosity is much less than that in the yield stress. Yield stress (Pa) 100 w/c Plastic viscosity (Pa.s) Sp. dosage (% solids by wt cement) Sp. dosage (% solids by wt cement) Figure 3.4: Typical effect of superplasticiser on Bingham constants for cement paste (After Domone and Thurairatnam, 1988). Page 47
72 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow Domone (2003) combined the data in Figures 3.3 and 3.4 into a single diagram, shown in Figure 3.5. Yield stress (Pa) w/c Sp. dosage (% cement) Plastic viscosity (Pas) Figure 3.5: Yield stress vs. plastic viscosity for cement paste with different watercement ratios and superplasticiser dosage (After Domone, 2003) Rheology of selfcompacting concrete A SCC mix has some special characteristics that should be considered when choosing a rheometer. These are the size of aggregate (smaller than in conventional vibrated concrete), timedependence o f flow properties, the presence of yield stress, moderate plastic viscosity, the potential for segregation and the high sensitivity to small changes in materials and their proportions. However it should be noted that at the present time not a single rheometer exists that can take into account all of the characteristics of the SCC mentioned above. Normally there are two main types of rheometer, namely those that impose a controlled shear rate on SCC and measure its shear stress and those that do the opposite. A wide range of rheometers is commercially available, as described below Coaxial cylinder rheometers A coaxial cylinder rheometer consists of two cylinders with one cylinder rotating relative to the other. In order to ensure a homogeneous test sample, the distance between outer and inner Page 48
73 C h a p t e r 3 : A n I n t r o d u c t i o n t o t h e R h e o l o g y o f S e l f  C o m p a c t i n g C o n c r e t e a n d M e t h o d s o f Simulating its Flow cylinders must be much greater than the maximum aggregate size. Depending on the range of rotation speeds, the material rheological properties, and the ratio of outer to inner cylinder radii, a certain portion of the material in the annulus o f a coaxial cylinder rheometer may be subjected to a stress below the yield stress. Figure 3.6 is a BML coaxial rheometer. It consists o f concentric ribbed cylinders to prevent slippage at the cylinder surfaces. Axis Inner cylinder with torque cell 150 T \r Outer rotating cylinder Concrete sample Fixed cone to avoid end effects Dimensions in mm Figure 3.6: A BML rheometer (After Wallevik and Gjorv, 1990; RILEM, 2002) Parallel plate rheom eters A parallel plate rheometer consists of two horizontal plates with one plate rotating relative to the other. This device permits testing a small sample and the direct analytical calculation of its rheological parameters in fundamental units. The complicated part is the calculation of rheological parameters related to the slippage that occurs at the vertical side walls. A BT RHEOM rheometer is shown in Figure 3.7. A cylindrical sample o f concrete is sheared between two circular parallel plates. Page 49
74 C h a p t e r 3 : A n I n t r o d u c t i o n t o t h e R h e o l o g y o f S e l f  C o m p a c t i n g C o n c r e t e a n d M e t h o d s o f Simulating its Flow Axis Blades Rotating part 240 Skirts Fixed part 270 Dimensions in mm Figure 3.7: A BT RHEOM rheometer (After de Larrard et al., 1997; RILEM 2002) Im peller rheom eters The impeller rheometers are based on a mixing action in which an impeller is rotated in a bowl of concrete. They are also known as the Tattersall rheometers (after their developer) or twopoint workability testing equipment. These devices are simple to use; however, the shear rate and shear stress in the material around the impeller cannot be measured. Also the fundamental rheological parameters cannot be directly evaluated. Calibration procedures have been suggested to relate the torque versus rotation speed plot to the yield stress and plastic viscosity; however these procedures are still not universally accepted. Figure 3.8 shows two alternative impeller types that can be found in the literature: the MH system (left) and the LM system (right) for medium to high and medium to low workability mixes, respectively. Page 50
75 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow 62 Toothed gears 50? Drive shaft Drive shaft Dimensions in mm *1 360 (a) MH system (5) LM system 32 Figure 3.8: Two systems for the impeller rheometer (After Domone, et al., 1999; RILEM, 2002) 3.5 Mathematical description of selfcompacting concrete rheology All the above tests give a flow curve in the form of a relationship between the applied torque (T) and speed of rotation o f the moving part (N). For most concrete mixes, a straightline relationship of the form T=g+h.N fits the data well. Concrete and other cementbased materials, such as selfcompacting concretes, are usually considered to be a Bingham fluid, i.e. their behaviour under shear depends on the shear stress and shear rate. Considering a Bingham model, g is the yield term and h the plastic viscosity term. The relationships between g and the yield stress (r y) and between h and the plastic viscosity (//) depend on factors such as the rheometer size, the flow pattern and geometry, which are all obviously different for each rheometer. By assuming a laminar uniform flow, simple relationships have been proposed for the BML and BT RHEOM rheometers. However for the impeller rheometer, the analytical relationships are far more complex Is there any consistency in the rheological properties of concrete? The yield stress and plastic viscosity are the fundamental properties of a Bingham fluid. Logically for a given concrete mix, any rheometer should give the same values of these two Page 51
76 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow fundamental parameters. But in practice that is not the case. As reported by Domone (2003), to quantify and to try to resolve these differences, a series of comparative tests was carried out in 2000, in which all three instruments were taken to the same laboratory and used simultaneously to test a series of fresh concrete mixes with a wide range of rheological characteristics (Banfill et al., 2001). The results confirmed that the instruments did indeed give differing values of the yield stress and plastic viscosity for the same mix. Figure 3.9 is an example of how two different rheometers gave totally different responses for one and the same mix. Shear stress (Pa) Contec Viscometer S S Shear rate (1/s) Figure 3.9: Two different responses for a single SCC mix tested by two rheometers (After Feys, 2007) Effect of concrete constituents on the Bingham constants The effect of the paste content, water, superplasticiser and cement replacement materials on the yield stress and plastic viscosity of a concrete mix are discussed here. Similar to what has been observed in the cement paste, the addition of water to a concrete mix decreases both its yield stress and the plastic viscosity. Superplasticisers normally reduce the yield stress but seem to have a different effect on the plastic viscosity. Solidbased superplasticisers like naphthalenebased, lead to an increase in the plastic viscosity, while the liquidbased Page 52
77 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow superplasticisers such as Gelenium ACE 333 have the opposite effect. Replacing some cement by PulverizedFuel Ash (PFA) or Ground Granulated Blast Furnace Slag (GGBS) reduces the yield stress, but leads to a decrease, and an increase, in the plastic viscosity, respectively. Also, using more paste increases the plastic viscosity but decreases the yield stress. All these effects are summarised in Figure Yield stress Less paste Less water More paste More w ater Superplasticiser Plastic viscosity Figure 3.10: The effect of mix constituents on Bingham constants (After Domone, 2003) As stated by Carlsward et al. (2003) regarding the influence o f constituents on rheology, air and crushed aggregates primarily decrease and increase the plastic viscosity, respectively, while the addition o f silica fume predominantly increases the yield stress. Addition of water also decreases both the yield stress and plastic viscosity (see Figure 3.11). Silica CO "3 Air Water, Aggregate Plastic viscosity Figure 3.11: Effect of some constituents on the rheological characteristics of SCC (After Dietz and Ma, 2000) Page 53
78 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow All these effects, although typical, will not necessarily occur with all mixes, and the behaviour can vary according to the type and source of component materials (particularly admixtures) and the properties o f the initial mix, i.e. the starting point in Figure Also, it is difficult to predict the interactive effects of two or more variables; an example of this is shown in Figure 3.12 for mixes containing varying cement and microsilica contents. Small amounts of microsilica reduce the plastic viscosity, with almost no effect on the yield stress; however, above a threshold level of microsilica, which depends on the cement content, there is a substantial increase in the yield stress, followed by an increase in the plastic viscosity. Yield stress Cement content O ^ 3) % %  5 % 2% Microsilica replacement Plastic viscosity Figure 3.12: Bingham constants for mixes containing various amount of microsilica (After Gjorv, 1997) 3.6 Basic terms and equations used in the general flow simulation Fluid dynamics uses the concept of fluid particles whose motion is described by Newton s second law of motion. In continuum mechanics, the mathematical relations are written in the form of conservation equations. The basic governing equations o f motion for a fluid particle are the equations of mass, momentum, and energy conservation. However in the absence of heat flux in a continuum, the energy can be assumed to be identically conserved (see Section 3 7). In this Section we will derive the mass and momentum conservation equations in the Lagrangian frame o f reference that employ the material derivative (a combination o f local Page 54
79 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow and convective derivatives). Normally the derivations use either the finite control volume or an infinitesimal fluid element concept Finite control volume Consider a finite region of a flow field shown in Figure Let us assign a control volume V and a control surface S to this region. The control volume can be fixed in space and the flow pass through it or it may move with the flow in such a way that a constant number of fluid particles is always inside it. The fundamental physical principles are applied to the fluid inside the control volume to derive the equations in an integral form. The integral equations are then converted to partial differential equations. If the concept of a fixed control volume is used, the equations so obtained are called the conservation form o f the governing equations, while the concept of a moving control volume gives the nonconservation form of the governing equations (Wendt, 1992). Control surface S S Figure 3.13: Finite control volume approach with fixed control volume (left) and moving control volume (right) (After Wendt, 1992) Infinitesimal fluid element Let us consider a general flow field shown in Figure On the one hand, the fluid element should be small to be considered as a differential volume dv for the purpose of the modelling and on the other this volume has to be sufficiently large to contain a very large number of molecules in order to regard it as a continuous medium. Again the fluid element can be fixed in space and the flow pass through it or it may move with the flow in such a way that a constant number o f fluid particles is always inside it. This approach gives the partial Page 55
80 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow differential equations directly. These equations are obtained based on the fixed or moving fluid elements which yield the conservation and nonconservation forms of the equations, respectively. & Volume dv Z dv Figure 3.14: Infinitesimal fluid element approach with fixed control element (left) and moving control element (right) Material derivative The substantial derivative or the total time derivative is an important physical concept in fluid dynamics. Let us consider the infinitesimal fluid cell moving with the flow (right side of Figure 3.14) at two time instants, ti and t2. The scalar density field at time ti is given by; A =/>( *!, (3.1) At a later time, t2 this field becomes: (3.2) The function (3.2) is expanded in a Taylor s series around the first point ti (Wendt, 1992) to give P i = A + + dp_ dt (*2 * i) + 'd p ' \^ A (/2 /,) + (higher order terms) A (y2~yx)+ ^ dp'' \d z j x (3.3) Dividing both sides of (3.3) by (t2  /,) gives Page 56
81 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow Pi P\ r dp^ dx ^ dp^ \ & A V ux J\ (± 12 _ ± *1 L ) + ^2 ~~ ^1 ( A Z A )+ dp dz ( h Z h.) + 1,1, \ u z j x <2#j ' d A (3.4) The left hand side of (3.4) is physically the average time rate of change in density of the fluid element as it moves from point 1 to point 2. Ift 2 approaches ti, then lim Pi P\ h >ri \ *2 ~ *1 J D p Dt (3.5) Examining (3.5), it can be realized that in a physical sen se is the time rate of change of Dt the fluid element, i.e. the change of density as it moves through point one as opposed to r dp^ which is the time rate of change of density at the fixed point 1. By taking the limit of \ d t A the right hand side of (3.4) as t2 approaches ti, we have t 2 t, lim(~ )=v (3.6) lim(z2 ~Z )=v t2 t, Therefore (3.4) becomes D p dp dp dp dp =v + v v +v + Dt x dx y dy 2 dz dt (3.7) By considering (3.7), a general expression can be obtained for a material derivative D d d d d = +v +v +v  Dt dt x dx y dy 2 dz (3.8) Denoting Page 57
82 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow r d r d r d. x V = 1 +/ + k (3.9) dx J dy dz (3.8) can be written as r \ ^ =  + (v V) (3.10) Dtdt v V is called the convective derivative, which in physical terms defines the time rate of change as the fluid element moves from one location to another in the flow field. The substantial derivative can be used for any flow field variables, e.g. pressure Physical meaning of V v The divergence of the velocity is a term that appears frequently when dealing with fluid dynamics problems. Consider a moving control volume in a flow field (right side of Figure 3.13); this control volume contains the same particles as it moves through the flow. As the control volume moves to a different location of the fluid, its volume V and control surface S will change because at its new position a different value o f p might exist. The moving control volume with a constant mass is continuously changing its volume and shape depending on the characteristics of the flow. Consider an infinitesimal element moving at the local velocity v, with surface ds and volume A V. Figure 3.15 shows the change in the volume of the control volume AV over a time increment A t. vat Figure 3.15: Physical meaning of the divergence of velocity (After Wendt, 1992) From Figure 3.15, the change in volume is equal to the volume of the cylinder with base area ds and height (va /)n, where n is a unit vector perpendicular to the surface. This change in volume is equal to Page 58
83 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow AF = [(vaon>is (3.11) The total volume change of the entire control volume is the integral over the control surface S AV = J v A tn d S (3.12) s Dividing both sides of (3.12) by At and applying the divergence theorem yields AV At = j V v d V (3.13) V where V is the divergence operator (3.9). Note that the left side of (3.13) is the material derivative of V, because this case is dealing with the time rate of change of the control volume as the volume moves with the flow. If the control volume is shrunk to an infinitesimal fluid element with volume d V, (3.13) becomes A(SV) At = (V v) f d(sv) = (V y)sv (3.14) Finally, the velocity divergence is given by; Vv =  L ^ > (3.15) SV Dt v The RHS of (3.15) explains physically the divergence of the velocity. It expresses the fact that V v is the time rate of change of the volume of a moving fluid element per unit volume The continuity equation Consider a moving fluid element with a fixed mass 8m and volume 8V then 8 m = p 8 f (3.16) Page 59
84 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow The continuity equation is based on the conservation of mass. It implies that the time rate of change of the mass of the fluid element is zero as the element moves along with the flow. Physically, this means that the substantial derivative o f the infinitesimal mass is zero, i.e. ^ 2 = 0 (3.17) Dt The substantial derivative o f (3.17) reads D(Sm) = D ( ^ ) = 3 r D p D m = 0 Dt Dt Dt Dt Rearranging (3.18) gives r + p ± D m = o (3.9 ) Dt d / Dt v 7 The second term in (3.19) is the divergence of the velocity (see (3.15)). Therefore ^ + pv v = 0 (3.20) (3.20) is the continuity equation or the mass conservation equation in the Lagrangian form T he m om entum equations The momentum equations are based on the conservation o f momentum. The physical principle here is Newton s second law, i.e. the total force on a fluid element equals to its mass times the acceleration of the considered fluid element. Let us consider a moving fluid element as shown in Figure The fluid element with the components of the force in the x direction is shown in more detail in Figure Page 60
85 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow Figure 3.16: A fluid element with components of the force in the x direction (After Wendt, 1992) Dv jyy The acceleration o f the fluid element is, and, in x, y and z directions Dt Dt Dt respectively; where vr,vy and v z are the components o f the velocity in the same directions. The net force acting on this element follows from two sources: the body force and the surface force. Body forces act directly on the volumetric mass of the fluid; examples of this kind of force are the gravitational, electric and magnetic forces; Surface forces act on the surface of the fluid element and are divided into two subcategories, i.e. the pressure imposed by the outside fluid surrounding the fluid element, and the shear and normal stress distributions related to the time rate of change of the deformation of the element which result in a shear deformation and volume change, respectively. The face dhgc may be called as the negative face of x and the face aefb as the positive face of x since the x value for face dhgc is less than that for the face aefb. Similarly, the face abed is the negative face of y and ehgf is positive face of>\ Negative and positive faces of z are hged and efab. Note that the stress on the positive face is equal to the stress on the negative face plus the rate o f change o f that stress multiplied by the distance between the faces. The Page 61
86 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow convention will be used here that a stress is positive when it is on the positive face in the positive direction or on the negative face in the negative direction. Also, the shear stress Ty denotes a stress in the jdirection exerted on a plane perpendicular to the iaxis. Both the shear and normal stresses depend on the velocity gradients in the flow. In most viscous flows, the normal stresses (e.g. ) are much smaller than the shear stresses and are neglected; however when the normal velocity gradients (e.g. dv / dx ) are very large, the normal stresses have to be taken into account (such as inside a shock wave). With the above in mind, in the x direction, all the forces acting on the infinitesimal fluid element are: [(/>+ ^  d x )  p y fy c k + [(r + ^  d x )  T xx yfydz + ox dx [(r +  ^  d y )  r Vxdz +[(r + ^  t k )  t z,y h d y (3.21) dy dz  dxdydz + dxdydz \ dxdydz + ^ Tzx dxdydz dx dx dy dz where P is the pressure from the surrounding fluid. If the body force in the x direction is Fx, then according to Newton s second law; dv x, dv dp,,, m = pdxdydz = dxdydz + dt dt dx ^ Txx dxdydz + dxdydz + dxdydz + dx ' dy * dz * Fx (pdxdydz ) (3.22) And hence the momentum equation in the x direction is given by Dv dp dr dr p = pfr (3.23) Dt dx dx dy dz x Similarly, the y and z components can be obtained as Dv dp dr d r d r p * = _ 2 L + J2L + _ 2L + /,7r (3.24) Dt dy dx dy dz Dv dp d r dr d r _ p  = pf. (3.25) Dt dz dx dy dz Page 62
87 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow Equations (3.23) to (3.25) are called the NavierStokes equations in honour of M. Navier and G. Stokes, who obtained the equations independently in the first half of the nineteenth century. If only the gravitational force on a particle is considered, the momentum equations (3.23) to (3.25) may be written in a compact form as Dv 1 d a, = + g (3.26) Dt p dxj Note that, in (3.26) the first term in the right hand side is the total stress tensor, which is made up of two parts: the isotropic pressure P and the viscous stress x as 021) Therefore, in summary the momentum conservation equations become =   V / >+ V.T + g (3.28) Dt p p 3.7 Disregarding energy conservation equations In the case of an incompressible flow ( V.v = 0 ), r=ct, where i is the sum of internal energy and C is the specific heat. Therefore the energy conservation equations reduce to temperature equations. In these equations if the differences between the surface and free stream temperatures are small so that the fluid properties such as its density and viscosity in the conservation equations are not affected by temperature, the conservation equations for energy can be ignored. Page 63
88 C h a p t e r 3 : A n I n t r o d u c t i o n t o t h e R h e o l o g y o f S e l f  C o m p a c t i n g C o n c r e t e a n d M e t h o d s o f _ S i m u l a t i n g i t s F l o w _ 3.8 Fluid classifications Fluids may be classified in two different ways according to their response to (i) shear rate, in which case they are called Newtonian or nonnewtonian, and (ii) pressure, in which case they are called compressible or incompressible Newtonian and NonNewtonian fluids Consider a simple shear flow as shown in Figure The fluid is held between two parallel plates separated by a distance Ay and a force F is applied to the top plate. Figure 3.17: Fluid sample as tested by a parallel plate device at two time instant, ti (left) and t2>ti (right) As a result of the force F, the lower plate moves at a constant velocity vi and upper plate moves at a constant velocity vi+dvj. Assuming noslip condition at the solid boundary, the velocity o f the fluid particles close to each plate is the same as the plate velocity. The remaining fluid particles move with an intermediate velocity between vi and vi+dvi. It can be assumed that there is a linear velocity distribution in the gap between the plates as shown in Figure vi+dvi Figure 3.18: The fluid velocity profile varies linearly Page 64
89 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow For this simple case, the force is constant and is proportional to the velocity gradient, y. Therefore F /A = (3.29) The first subscript represents the direction normal to the shearing surface, while the second subscript indicates the direction o f the force (or flow). If the ratio x / y is constant, the fluid is Newtonian, otherwise it is nonnewtonian. The non Newtonian fluids can be grouped into three categories as follows: Generalized Newtonian fluids: the rate of shear at any point is obtained only by the value of the shear stress at that point and at that instant. These fluids are also known as purely viscous, timeindependent and inelastic fluids. Timedependent fluids: more complex relations are implemented to describe such fluids. The relation between the shear stress and shear rate depends on the duration of shearing and their kinematic history. Viscoelastic fluids: demonstrate properties of both ideal fluids and elastic solids. These fluids show partial elastic recovery after deformation. These categories o f fluids may be further subdivided, as shown in Figure NonNewtonian fluids TimeIndependent or Generalized Newtonian Timedependent Viscoelastic Viscoplastic e g. Bingham plastic model * Shearthinning Shearthickening Thixotropy * Rheotropy * Elongation >... Figure 3.19: Subdivision of nonnewtonian fluids Page 65
90 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow The most common type of flow behaviour observed is generalized Newtonian or time independent nonnewtonian. Figure 3.20 shows sets of qualitative flow curves on linear scales for the above three types o f nonnewtonian fluid behaviour. 3 <D i. Yield ~ pseudoplastic Bingham  plastic Pseudo plastic fluid / Newtonian fluid Dilatant fluid Shear rate Figure 3.20: Types of generalized nonnewtonian flow behaviour (After Chhabra and Richardson, 2008) Among these three, the most common type of flow behaviour is the viscoplastic one, characterized by the existence of a yield stress {ry) which must be exceeded in order for a fluid to flow. The viscosity of a fluid can be a decreasing or an increasing function of y ; such fluids are called shear thinning and shear thickening, respectively. Figure 3.21 shows these behaviours in relation to Bingham and Newtonian fluids. Page 66
91 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow Shear stress (x) Shear thinning Linear (Bingham) Yield stress Plastic viscosity Shear thickening Linear (Newtonian) ^ Viscosity Rale of shear strain (j) Figure 3.21: Behaviour of shear thinning and shear thickening fluids in relation to viscoplastic fluids behaviour (After Domone, 2003) Once the shear stress reaches this yield value, the flow curve (shear stress vs. shear rate) may be linear or nonlinear which do not pass through the origin. Over the years, some empirical equations have been proposed. The three commonly used models are described below Bingham plastic model The Bingham plastic model or simply the Bingham model is the simplest relation to show the behaviour of a fluid having a yield stress ry. It is written as T = Ty +rjy y = 0 T>T y T<T. (3.30) HerschelBulkley model This model is a generalization of the Bingham model in such a way that, upon deformation, the viscosity can be shear thinning or shear thickening (see Figure 3.21). The constitutive equation is r = ry + my y = 0 r>z\ T<T, (3.31) For n<\, the fluid exhibits shear thinning properties w=l, the fluid shows Bingham behaviour «>1, the fluid shows shear thickening behaviour Page 67
92 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow In equation (3.31), m and n are two empirical curvefitting parameters and are known as the fluid consistency coefficient and the flow behaviour index, respectively. For a shear thinning fluid, the index may have any value between 0 and 1. The smaller the value of n, the greater is the degree of shear thinning. For a shear thickening fluid, the index n will be greater than unity Compressible and incompressible fluids As previously mentioned, one can divide the flows based on their response to an external pressure. Physically, a fluid which is not reduced in volume by an increase in pressure is called an incompressible fluid, whereas the opposite is true for a compressible fluid. In an incompressible flow the ratio of the material speed to the speed o f sound in the fluid is very low (normally around 0.1); this ratio is called the Mach number. In computational fluid dynamics this classification is of prime importance in order to solve the conservation equations (see Sections and above). A problem that occurs in solving the conservation equations is introduced by the pressure term, which only appears in the momentum conservation equations (3.28) and needs to be coupled with the velocity field in the mass conservation equations (3.20). In compressible flows, this problem can be solved by adopting a suitable equation of state P = P (pyt)which gives the pressure based on density and temperature; this means that the continuity equations are used as a transport for density. However, if the flow is incompressible, the density is constant and by definition has no link to pressure. The main aim in solving an incompressible fluid flow problem is to apply the correct pressure field in the momentum equations in order to have a continuous velocity field, i.e. divergence free velocity (V v = 0). As we shall be solving an incompressible flow problem later in Chapter 6, we shall review briefly how the pressurevelocity linkage is affected through either the concept of artificial compressibility or the pressurepoisson (projection or pressure correction) equation Artificial compressibility As stated before, the main difficulty with the solution of the incompressible fluid flow equations is due to the decoupling of the mass and momentum conservation equations due to the absence of the pressure (or density) term from the continuity (or mass conservation) equations. Chorin (1968) proposed an approach to overcome this problem. He introduced an Page 68
93 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow artificial compressibility term into the continuity equations. In the absence of external forces and the deviatoric part in the momentum conservation equations, using this method the conservation equations become P Dt (3.32) Dt p p is a factor which enables the conservation equations to have a divergence free solution, i.e. to satisfy the incompressibility requirement. The artificial compressibility gives sets of equations which are hyperbolic and hyperbolicparabolic and whose solution is often less computationally expensive than that of elliptic equations (used in the pressurepoisson method; see below) PressurePoisson equation The basic idea of this method is to formulate a Poisson s equation for the pressure correction. The pressure and velocity fields are updated until they reach a divergence free state. Taking the divergence of the momentum conservation equations in the absence of a deviatoric stress gives V 2P = pv.(vv) (3.33) In order to use the pressurepoisson s equation, a projection formulation introduced by Chorin (1968) is implemented in such a way that the pressure field is applied to enforce a divergencefree velocity. The basic idea of projection method is to introduce a vector field (here velocity or velocity gradient), v = (v*,vy,vz) neglecting the divergence of the velocity field, and then to recover the incompressible nature of the flow through projection. The operation is vd=p(v) (3.34) where v^is a desired solenoidal vector field i.e. V.v = 0. The projection methods in turn are divided into exact and approximate projections. In the exact projection, the discrete divergence of a vector field is intended to be identically zero after applying the projection to a vector field. In the approximate projection, the discrete Page 69
94 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow divergence is a function of the truncated error of the scheme. In Chapter 6, we shall be using the pressurepoisson equation in order to impose exactly the incompressibility requirement. 3.9 Simulation of the flow of concrete This section briefly provides a general overview of the present computational strategies available in the literature to model the flow of fresh concrete. From the modelling point of view, the fresh concrete can be considered as a fluid when a particular degree of flowability is achieved, e.g. the slump is at least 100 mm (Ferraris et al., 2001a) and when the concrete is homogeneous. Due to its extreme flowability, the SCC in general satisfies the flow and cohesiveness requirements and can thus be modelled as a Bingham fluid (Vasilic et al., 2010). In most numerical simulations, only the steadystate of the flow is considered, i.e. thixotropy is not taken into account. Therefore the loss of workability of concrete during the flow is not modelled. However, sometimes the viscosity increases with the shear rate which means the SCCs exhibit a shear thickening behaviour (e.g. in mixing and pumping). This behaviour can be modelled by a generalization of the Bingham model, the socalled Herschel Bulkley model (see equation (3.31)). Computational modelling of flow could be used in three main ways; first, for the simulation of mould filling behaviour; second, a potential tool for understanding the rheological behaviour of concrete; and third, a tool for mix proportioning. The numerical simulation of the SCC flow could allow us to determine the minimum workability o f the fresh concrete that would ensure the proper filling of a given mould. The computational modelling techniques based on the finite element method (FEM) are used to deal with the concrete particles. In the literature, these meshbased FEM modelling techniques may be divided into two main families: homogeneous fluid simulation and nonhomogeneous fluid simulation. An alternative to modelling the concrete particles is to use methods which are based on the meshless methodology, such as the smooth particle hydrodynamics (SPH) method. Page 70
95 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow FEM modelling techniques Homogeneous fluid simulation The homogenous fluid approach has mostly been used to model the flow of fresh concrete. It refers to the simulation of ideal fluids without particle inclusions and is included in the overall framework of computational fluid dynamics (CFD) (Wendt, 1992). A numerical solution method is applied to obtain the flow characteristics by solving the governing equations o f mass, momentum and energy conservation. The important assumptions are that the segregation of the coarse particles during the flow (dynamic segregation) does not take place and that the blocking of concrete caused by particle interactions, e.g. by their interaction with the reinforcement bars, at any stage of flow is avoided. Also the smallest characteristic dimension of the flow (size of the mould or the spacing between the bars) must be large compared to the size of the largest particle (five times larger) (Spangenberg et al., 2010). Otherwise, other simulation methods must be used. In this approach a single fluid characteristic is assigned during the flow, such as the yield stress and the plastic viscosity. The Bingham model is the most common model used. The discretization methods comprise the finite volume method, the finite element method, and the finite difference method (Wendt 1992). In the past researchers have mainly used two models to simulate the fluidity tests of fresh concrete, namely the viscoplastic finite element method (VFEM) (e.g. Mori and Tanigawa, 1992), and the viscoplastic divided element method (VDEM) (e.g. Kurokawa et al., 1996). Both methods assume that concrete can be described as a homogeneous fluid with single rheological properties. As reported by Roussel et al. (2007), in the VFEM, the fresh concrete is divided into elements in which the deformation is calculated, and the flow is described by the displacement of the nodal points. In the VDEM, the domain is divided into elements and cells, which are either empty or full, and the flow is described bythe displacement of virtual markers. A few studies have been carried out on the process of casting cementitious materials using the homogeneous fluid approach. For the SCC, Thrane (2007) registered consistency between the experimental and simulated flow behaviour for the slump flow test, the Lbox test, and Page 71
96 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow the form filling tests and found reasonable agreement between the rheological parameters determined in the viscometer and those applied to simulate the flow (Bakker et al., 2010). Although these models provide the fastest way to simulate the flow of concrete, the main numerical difficulty in connection with these kinds o f simulations is the free surface displacement because fresh concrete displaying a moving free boundary requires a clear definition of the boundary conditions. Also the homogeneous fluid approach does not simulate particle blocking or dynamic segregation; therefore additional tools are needed to assess under which flow conditions there is a risk o f blocking and dynamic segregation (Thrane, 2007) Nonhomogeneous fluid simulation The aim o f this method is to carry out detailed studies of the movement, trajectory, rotation, and interaction of particles (Thrane, 2007). This type of simulation considers the difference in physical properties o f liquid and granular components used in the concrete and their effect on the flow. Based on this analogy, the flow of concrete can be dominated by either a fluidlike or a solidlike behaviour. In the case of SCC, normally the coarse aggregate is limited therefore it is reasonable to assume that it behaves as a fluid suspension. For normal concrete, the solidlike behaviour might be dominant. In this category, the standard discrete element method (DEM) is mainly used. This method divides the calculations into two steps: obtaining the contact forces between the solids, and determining the motion of each solid using Newton s second law. Noor and Uomoto (1999) used a 3D DEM developed by Chu et al. (1996) to simulate the flow of SCC in slump flow test, Lbox test and Vfimnel test. They divided the material into mortar and coarse aggregate larger than 7.5mm. As stated by Roussel et al. (2007) the result of Noor and Uomoto (1999) gave the qualitative behaviour in fresh concrete. Martys (2005) used another method called the dissipative particle dynamics (DPD) method in the field of cementitious materials which allowed for much larger time steps, as opposed to DEM. The advantages of implementing the nonhomogeneous simulation are as follows: the ability to carry out detailed studies of the particle flow and thereby to simulate the heterogeneous flow phenomena (Thrane, 2007), the scale of observation could match the size of real materials that are dealt with, and, as opposed to an homogeneous simulation, the moving free Page 72
97 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow surface of the concrete can be more easily modelled. In summary, the nonhomogeneous method aims at simulating both the macroscopic and local behaviour of granular materials and suspensions (Thrane, 2007). A limited number of studies has been performed on the form filling ability and flow patterns, but the relation between the simulations and experiments is not clear (Bakker et al., 2010). The main disadvantage of this method is related to the physical meaning, i.e. it is difficult to define physically a direct contact between solid particles that are representing the mortar phase and coarsest grains Disadvantages of meshbased numerical simulations Meshbased numerical simulation suffers from some inherent difficulties in many aspects, which limit their application to concrete simulation. In meshbased methods, the mesh generation for the problem domain is a condition for the numerical simulations. In Eulerian meshbased methods, such as the finite difference method (FDM), making grids (meshes) for complex or irregular geometry is a difficult task which usually involves additional complex mathematical transformation that could be even more expensive than solving the problem itself. Other difficulties in the fixed Eulerian grid are determining the precise locations o f the inhomogeneities, free surfaces, etc. In Lagrangian methods such as the finite element method (FEM), mesh generation is a prerequisite for the problem being modelled. The construction of mesh usually takes a significant portion of the computational effort. The treatment of large deformation is an important issue in a Lagrangian gridbased method. It usually requires special techniques like rezoning. Mesh rezoning, however, is a formidable and time consuming task which can lead to additional inaccuracy. In the whole process of concrete simulation there exist special features such as large deformations, large inhomogeneities and free surfaces. These special features pose great challenges to numerical simulations using gridbased methods Meshless particle based simulation Due to the Lagrangian nature of the SCC flow and due to the fact that an SCC mix is essentially an aggregate of particles of different sizes and shapes, the use of meshless particlebased Lagrangian numerical techniques to simulate such flows is both more appropriate and simpler than the traditional meshbased methods (e.g. Petersson, 2003, Page 73
98 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow Dufour and PijaudierCabot, 2005 and Roussel et al., 2007) reviewed above. An example of this category is the smooth particle hydrodynamics (SPH) method. The SPH is a meshless Lagrangian approach that offers considerable potential as a numerical method for modelling problems involving large deformations. Its simplicity and Lagrangian nature have been exploited in the past to model many ffeesurface fluid flows and related engineering problems (e.g. Kulasegaram et al., 2004, Cummins and Rudman, 1999 and Monaghan, 1992). The following section is devoted to a brief explanation o f SPH method and its essential properties Introduction to smooth particle hydrodynamics (SPH) The smooth particle hydrodynamics (SPH) was first introduced by Lucy (1977) and Gingold and Monaghan (1977) to solve astrophysical problems in threedimensional open space. The SPH has been extensively studied and extended to fluid flow with large deformations (e.g. Bonet and Kulasegaram, 2000; Shao and Lo, 2003). Applications o f the SPH method are very wide, ranging from computational fluid mechanics to computational solid mechanics, from microscale to macroscale and to astronomical scale, and from discrete to continuum systems (Liu and Liu, 2003) Key characteristics o f SPH method The SPH method has the following key characteristics: 1. Mesh free: The problem and boundary domains are represented by a set of arbitrarily distributed particles. No connection between these particles is needed. 2. Integral representation: All field variables such as the density, velocity, energy, etc. are represented by integral functions. The socalled kernel function is used to approximate these integral functions. 3. Compact support: The kernel approximation is then further approximated using particles. This process is called the particle approximation. It is done by replacing the integration in the integral representation of the field function and its derivatives with summations over all the corresponding values at the neighbouring particles in a local domain called the support domain (see section below). Page 74
99 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow 4. Lagrangian: The particle approximations are performed on all terms related to field variables to produce a set of ordinary differential equations in a discretized form with respect to time only. In the following all the technical terms used above are discussed in detail Nodes or particles in SPH As with other meshless methods, SPH use a set of nodes scattered within the problem domain as well on the boundaries to represent (not discretize) the configuration of the problem (Figure 3.22). ch.* Figure 3.22: Scattered nodes to represent the problem and boundary domains with two shapes of the support domain Support domain The SPH method approximates field variables only on the particles. Each particle in the SPH method has a support domain. The support domain for a field point x=(x, y, z) is the domain where the information for all the points inside this domain is used to determine the information at the point x. Page 75
100 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow The support domain in meshfree methods can be global or local. For global support domain, the entire problem domain is considered; therefore it is computationally expensive. A local support domain is usually preferred, in which only the nodes or particles that are within a local region of finite dimensions of a point are used for the approximations of the field variables at that point. The dimensions and shape of the support domain can be different. As shown in Figure 3.22 the most commonly used support domain shapes are elliptic (preferably circular). The support domain is usually taken to be symmetric, especially for points near the boundary. The concepts of support domain for a particle are closely related to the smoothing length h of that particle. The smoothing length h multiplied by a factor c determines the size of support domain in which the smoothing function applies (the terms c and h will be defined later). Therefore the support domain of a particle is governed by the region of size ch for that particle (Figure 3.22) Essential formulation o f SPH The formulation of SPH is divided into two key stages, namely the integral representation (or the socalled kernel approximation of field functions) and the particle approximation. In the following these two stages will be examined in more detail Integral representation The smooth particle hydrodynamics uses the following identity to represent an arbitrary function ^(x )in an integral form Q x') (xx')c/s;' (3.35) where the integral is taken over the volume Q and 5^. is the Kronecker delta x * x ' (336) The Kronecker delta can be replaced by a function Wy so that the integral representation of ^ becomes Page 76
101 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow ^(x) = jv (x ')JF (x x ',/*)<&' (3.37) Q where W is the socalled kernel or smoothing function. In the smoothing function, h is the smoothing length defining the domain of influence of the smoothing function W. It is worth noting that the kernel function gives only an approximation of the original function as long as it is not equal to the Kronecker delta. The kernel IT has the following properties: 1. Normalization or unity condition that states fw ( x  x,/i)dx' = l (3.38) Q 2. Kronecker delta property that is observed when the smoothing length approaches zero lim W(xx,h) = 5 ' (3.39) x >x' ' ' 3. Compact condition IF (xx',/i) = 0 if x x ' > c/i (3.40) where c is a scaling factor to normalise the kernel function. It is a parameter to define the effective nonzero of the smoothing function. This effective area is called the support domain (see Figure 3.22) and is given by x x ' < c /i (3.41) Here, the length parameter h has a similar interpretation to the element size in the finite element method Kernel function The kernel or interpolation or smoothing function usually has a bell shape with a compact support. The most commonly used kernel function in the SPH is a cubic spline Page 77
102 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow 2 4 if <\ (3.42) 0 z/f> 2 where d is the number of dimensions of the problem Particle approximation In the SPH method, the entire problem domain is divided into a finite number of particles that carry individual mass and occupy individual space. The continuous integral (3.35) can be converted to a discretized form of summation over all the particles in the support domain shown in Figure s Figure 3.23: Particle approximations using particles within the support domain of the smoothing function W for a particle at centre The process of particle approximation in the SPH is as follows. The infinitesimal volume dx' in the above integrations at the location of particle b (as shown in Figure 3.23) is replaced by the finite volume of the particle Vb. The particle b is a generic particle in the set 1, 2, N in which N is the number of particles within the support domain. Therefore the continuous Page 78
103 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow integral in (3.35) can be expressed by the following form of discretized particle approximation or (*) = X VAW  *b>h) (343) 1 = (3 44) b=1 where the assumed mass of particle b is given by = Vm (3.45) Note that Wb (x) has the unit of the inverse of volume and that Wb(*) = W { *  i i,h) (3.46) Similar to (3.44), the differential o f the function ^ (x )is given by = (3.47) b=1 Equations (3.44) and (3.47) state that the value of a function (or its differential) at any position is approximated using the average of those values o f the function at all the particles within the support domain (particles b=l, 2,..., N) of that particle weighted by the smoothing function Wb (x ). The approximation of the arbitrary function ^ (x )in terms o f the kernel function Wb (x)is shown in Figure Page 79
104 C h a p t e r 3 : A n I n t r o d u c t i o n t o t h e R h e o l o g y o f S e l f  C o m p a c t i n g C o n c r e t e a n d M e t h o d s o f S i m u l a t i n g i t s F l o w f*kx) Figure 3.24: Approximation of an arbitrary function ^ (x )in terms of kernel function Wb (x) (After Kulasegaram et al., 2002) The application of equation (3.44) to compute the approximate value for the density of a continuum leads to the classical SPH equation = (3.48) *= Corrected SPH integration The basic SPH approximations as given by equation (3.44) or (3.47) do not accurately reproduce or approximate the function ^ (x ) and V ^ (x ). Therefore, in the past, corrected SPH equations were developed to address these issues (Bonet and Lok, 1999; Bonet and Kulasegaram, 2000). The main aim of the correction techniques is to satisfy the conservation of angular momentum which, unlike the linear momentum, is not automatically satisfied. In order to correct the SPH algorithms, some work was done on the gradient of the kernel directly (Bonet and Lok, 1999), whereas others have modified the kernel function itself (Li Page 80
105 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow and Liu, 1996). Another possible way is to mix the kernel and gradient corrections (Bonet and Kulasegaram, 2000; Bonet and Lok, 1999). More information on these correction techniques and procedures can be found in Appendix A. Using the corrected gradient of the corrected kernel, the SPH equations (3.44) and (3.47) can be rewritten as ^ t o = I X < W t o (349) 6=1 = (3.50) For instance, the corrected form of the gradient of the velocity at a given point a is given by, 6=1 (3.51) where W indicates that the kernel function is corrected to satisfy the consistency conditions, and b is the neighbouring particle within the support domain o f particle a. Further, V above indicates that the gradient is corrected to reproduce linear consistency. The gradient correction used here is adopted from the mixed kernel and gradient correction. To simulate the SCC flow, an incompressible SPH methodology will be adopted in this thesis (Chapter 6). A Bingham model suitable to represent the rheological behaviour of SCC with and without fibres is developed in Chapter 5 from micromechanical principles. The formulations relating to the incompressible SPH and its coupling with the Bingham constitutive model are used in Chapter 6 to simulate the flow of SCC with and without steel fibres Incompressibility in SPH In the original simulation of incompressible flows by SPH, incompressibility was imposed through an equation of state so that the fluid was considered to be weakly compressible. In this situation, normally a large speed of sound in the medium has to be assumed so that the corresponding density fluctuations can be kept small. Page 81
106 Chapter 3: An Introduction to the Rheology of SelfCompacting Concrete and Methods of Simulating its Flow However, the artificial compressibility can cause problems with sound wave reflection at the boundaries and the high speed of sound can lead to a stringent time step constraint (Shao and Lo, 2003). As stated before, in this research a strictly incompressible SPH model will be used to simulate the flow of SCC mixes. By implementing the fully incompressible state, the time step can be larger and it can be chosen based on the fluid velocity field rather than the speed of sound. The disadvantage of this method is that the pressure is not an explicit thermodynamic variable obtained through an equation o f the state, but obtained by solving a pressure Poisson equation which might be numerically time consuming Concluding remarks The fundamental quantification of the workability of selfcompacting concrete was discussed. The techniques for measuring the rheology of the paste and the SCC using different types of rheometers were presented. The general rheological parameters of a viscous fluid were more deeply examined. Fluids were classified into two broad categories, i.e. their response to shear rate and to pressure. The former gave two classes; Newtonian and nonnewtonian, whereas the later resulted in compressible and incompressible fluids. According to the response to shear rate, the SCC can be regarded as a generalized nonnewtonian incompressible fluid. It is stated that the rheology of SCC is best describe by the Bingham model which contains two material properties, namely the yield stress ry and the plastic viscosity rj. The governing equations of the flow of concrete, i.e. conservation o f mass and momentum which will be used in the flow simulations were derived. Different methods available in the literature to simulate the flow of fresh concrete, along with some of their advantages and disadvantages were briefly reviewed. It was argued that owing to the Lagrangian nature of the SCC flow and due to the fact that an SCC mix is essentially an aggregate of particles of different sizes and shapes, the use of meshless particlebased Lagrangian numerical techniques to simulate such flows is both more appropriate and simpler than the traditional meshbased methods. Page 82
107 C hapter 4 Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres
108 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres 4.1 Introduction The ideal design of a selfcompacting concrete (SCC) mix is a compromise between two conflicting objectives. On the one hand, the SCC has to be as fluid as possible to ensure that it will fill the formwork under its own weight, but on the other, it has to be a stable mixture to prevent segregation of solids during the flow (Spangenberg et al., 2010, Su et al., 2004, Roussel, 2007b). The former is ensured by using superplasticiser and/or viscosity modifying admixtures, while the latter is achieved through the selection o f the right amount and type of powders, i.e. cement and cement replacement materials (CRM) and by striking the right balance between the solids and liquids in the mix. Steel fibres can be added to the SCCs mixes to improve the mechanical properties and the durability of the mixes in much the same manner as in vibrated concrete. However, the fibres greatly impair the workability of the SCC because of their elongated shape and large surface area. The amount of fibre that can be added to a SCC mix is therefore limited and depends on the fibre type used and the composition of the SCC mix. The maximum amount of fibre needs to be determined in such a way as to cause the least decrease in the workability, whilst maintaining good flow and passing ability. In order to make the best use of the fibres, they need to be homogeneously distributed in the mix without clustering (Grunewald and Walraven, 2003). This chapter reports on the development of selfcompacting high and ultra high performance concrete (SCHPC/SCUHPC) mixes with and without steel fibres (SCHPFRC/SCUHPFRC). The aim is to investigate how the proportions of solids and liquids, the type of superplasticiser, and the steel fibres need to be selected in order to produce SCHPFRC/SCUHPFRC mixes with the right flow and passing ability. It is found that for the mixes without steel fibres the fulfilment of the flow and cohesiveness criteria is sufficient for the mix design. However, for the design o f SCC mixes with steel fibres, they must additionally meet the passing ability criterion. The major part of this chapter has been submitted for publication to the journal Cement and Concrete Composites (see publication 3 in the list in Chapter 1). Page 84
109 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres 4.2 Development of SelfCompacting HighPerformance FibreReinforced Concrete (SCHPFRC) The original goal of this part of the investigation was to develop a selfcompacting version of a highperformance vibrated concrete (with a nominal characteristic compressive strength of 100 MPa) which has been produced regularly in the same laboratory over many years using naphthalene sulfonatebased superplasticiser. The mix proportions of this standard vibrated mix are shown in Table 4.1. The binder refers to cement plus microsilica. Table 4.1: Mix proportions (kg) of a standard vibrated highperformance mix Mix 1 Cement 500 ab y Microsilica 55 px C/J Limestone 0 5 0/ Sand < 2 mm w Coarse aggregates < 10 mm Bs Water 161 o u Superplasticiser 9 Fibres 0 Ratios Water/binder 0.29 SP/water Mix preparation The trial mixes were prepared in a planetary mixer by mixing the coarsest constituent (coarse aggregate) and the finest one (microsilica), followed by the next coarsest (sand) and next finest constituent (cement), and so on. Before each addition, the constituents were mixed for 2 minutes. To fluidise the dry mix, twothirds o f the superplasticiser (SP) was added to the water. Onehalf of this watersp mixture was added to the dry constituents and mixed for two minutes. Onehalf of the remaining watersp mixture was then added and mixed for two minutes. This process was continued until all watersp mixture was added. The remaining onethird of the SP was added and mixed for two minutes just before transferring the SCC mix into the slump cone or placing it in the moulds. Page 85
110 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres Flowability test The slump flow test was performed on trial mixes to obtain a mix with the maximum flowability and homogeneity. The horizontal spread up to 500 mm was timed. If it was different from 3 sec, or any segregation was visible, the mix proportions were judiciously altered. This trial process was continued until the mix met the flowability criterion (horizontal spread T5 0 0 of 500 mm in 3 sec) and was homogeneous with no visible segregation SCHPC and SCHPFRC mixes To achieve a selfcompacting version of the Mix 1 in Table 4.1, several trial mixes were made and tested. Table 4.2 gives the composition of these mixes and their corresponding slump flow test results. It should be noted that these mix proportions will lead to slightly different yields in terms of volume. Table 4.2: Composition of SCHPC and SCHPFRC mixes (kg) with naphthalene sulfonatebased superplasticiser Constituents (kg) Ratios Slump Mix 2 Mix 3 Mix 4 Mix 5 Cement Microsilica Limestone Sand < 2 mm Coarse aggregates < 10 mm Water Superplasticiser Fibres Water/binder SP/water Slump flow spread (mm) T 500 (sec) Comments on the contents of Table 4.2 follow: In Mix 2, the coarse aggregate content was decreased by 20% (relative to Mix 1) in order to reduce the interparticle friction. Limestone dust was added to increase the paste volume and to lubricate the aggregate particles. The microsilica content was increased by up to 30%. The Page 86
111 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres superplasticiser to water ratio was increased from 0.06 to The sand content was increased by 3%. The water to binder ratio was held unchanged at It was observed that the mix was too stiff without any horizontal flow at all. In Mix 3, the sand and coarse aggregate contents were decreased by 5% and 9%, respectively, while the SPwater ratio and waterbinder ratio were kept constant at 0.11 and 0.29, respectively. The horizontal slump flow of the mix was 540 mm but T was 4 sec, i.e. more than the required 3 sec. In the next mix (Mix 4), the paste volume was increased by adding 3% more limestone dust. This mix met the T5 0 0 criterion, and there was no visible segregation (Figure 4.1). However, the compression test on specimens made out of this mix at the age of 3 days suggested that it would fall short of the 28day target compressive strength of 100 MPa. This is a consequence of the reduction in the coarse aggregate content by nearly 28% (relative to Mix 1) in order to achieve the desired flowability and cohesiveness o f the mix. Figure 4.1: Horizontal spread of SCHPC mix 4 Page 87
112 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres The simplest way to increase the compressive strength of this SCHPC mix without having to alter any other mix proportions was to add a small amount of steel fibres to the mix. In the present study, 30 mm long Z560 Dramix fibres with crimped ends (Figure 4.2) were used. The fibres are supplied by the manufacturer as small flat packs containing more than 40 fibres temporarily held together by watersolvable glue. 0.5% by volume of these fibres were Figure 4.2: 30 nun long glued steel fibres added to Mix 4 to create Mix 5 (Table 4.2). The fibres were added progressively to the wet SCHPC mix (i.e. after all the watersp mixture had been added and mixed; see section 4.2.1) and mixed until the glue had dissolved and the fibres had dispersed uniformly in the mix. The remaining onethird of the SP was added and mixed for two minutes just before transferring the fibrereinforced mix into the slump cone. The horizontal spread up to 500 mm was timed at 3 sec, as required, although the final spread was slightly less than that of the SCHPC without fibres (560 mm against 600 mm). This selfcompacting highperformance fibrereinforced concrete (SCHPFRC) met the flowability criterion and was very homogeneous with no visible segregation (Figure 4.3). Page 88
113 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres Figure 4.3: Horizontal spread of SCHPFRC mix Influence of the type of superplasticiser It has been reported (Flatt, 2004b) that polycarboxylate etherbased superplasticisers, e.g. Glenium ACE 333, which disperse particles by steric stabilisation result in better workability than do the naphthalene sulfonatebased superplasticisers, which disperse particles by electrostatic repulsion. For this reason the naphthalene sulfonatebased superplasticiser was replaced by an equal amount of Glenium ACE 333. Table 4.3 shows the compositions of the SCHPC and SCHPFRC mixes using this SP. Page 89
114 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres Table 4.3: Composition of SCHPC and SCHPFRC mixes (kg) with Glenium ACE 333 superplasticiser Constituents (kg) Ratios Slump Mix 6 Mix 7 Mix 8 Mix 9 Mix 10 Cement Microsilica Limestone Sand < 2 mm Coarse aggregates < 10 mm Water Superplasticiser Fibres Water/binder SP/water Slump flow spread (mm) T (sec) Comments on the trial mixes of Table 4.3 follow: In Mix 6, the naphthalene sulfonatebased superplasticiser o f Mix 4 was replaced by an equal amount of Glenium ACE 333. The resulting mix was found to have a very low viscosity with a horizontal spread in excess of 850 mm and clear bleeding. This meant that either the liquid content could be decreased or the solid content could be increased. Accordingly, in Mix 7, the waterbinder ratio and SPwater ratio were reduced from 0.29 to 0.25 and from 0.11 to 0.07, respectively. Despite obtaining the horizontal slump flow of 800 mm and T5 0 0 of 3 sec, the mix was rejected because of bleeding. In a further attempt to reduce the bleeding (Mix 8), all the solid contents (except the cement) were modestly increased (by 5%), while the SPwater ratio was increased to The slump flow was 745 mm but T was equal to 5 sec. In the next trial mix (Mix 9), the SPwater and the waterbinder ratios were increased to 0.15 and 0.22, respectively. This mix had the required flowablility (slump flow of 780mm and T5 0 0 equal to 3 sec) and was cohesive. In the trial Mix 10, 0.5% by volume of 30 mm long Z560 Dramix fibres was used. The mix so produced satisfied both the flowability (the horizontal slump flow was only marginally smaller i.e. 770 mm against 780 mm) and cohesiveness criteria. Page 90
115 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres Passing ability test The trial Mixes 9 and 10 (without and with fibres) that satisfied the flowability criterion and showed no signs of segregation i.e. were highly cohesive, were subjected to the passing ability test to ensure that they were able to pass through narrow gaps that exist between reinforcing bars in a real reinforced concrete structural element. For this test, a 300 mm diameter JRing apparatus with 16 steel rods (each o f diameter 16 mm) was used, as recommended by The European Federation o f National Trade Associations (EFNRC) (efnarc.org, 2005) (see Figure 2.17 in chapter 2). This test showed that there was some blocking in the SCHPFRC Mix 10 with the bulk o f the fibres and coarse aggregates lumped in the centre of flow spread. It was therefore necessary to adjust the mix proportions. Table 4.4 gives the various trial mixes o f SCHPC with steel fibres which have been tested for passing ability in JRing apparatus. 1w Table 4.4: Composition of SCHPC mixes (kg) with 0.5% steel fibres for the JRing test Mix 11 Mix 12 Mix 13 Cement Microsilica Limestone IS 90) Sand < 2 mm m Coarse aggregates < 1 0 mm S i3 Water O u Superplasticiser Ratios Slump Fibres Water/binder SP/water Slump flow spread (mm) T 5oo (sec) In the first attempt (Mix 11) to meet the passing ability requirement, the water to binder ratio was increased from 0.22 to 0.25 and the SP to water ratio was correspondingly decreased to Most of the fibres and the coarse aggregate were still clustered in the middle o f flow spread. Page 91
116 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres Therefore, in the next trial Mix 12 the water to binder ratio was decreased to 0.23 but the SP to water ratio was correspondingly increased from 0.13 to This mix too failed to meet the passing ability requirement. It was therefore decided to reduce the amount of powder, while keeping the amount of liquids constant. Thus in Mix 13, the amount of limestone dust was reduced by about 10%. The result was a much improved mix with only a slight segregation in the middle of flow spread. In the next trial mix (Mix 14 in Table 4.5) the limestone dust content was further reduced by 10%. The coarse aggregate content was also slightly decreased, with a corresponding increase in the fine aggregate (sand). The SPwater ratio was kept constant, while the waterbinder ratio was increased to This mix (Mix 15 in Table 4.5) met the passing ability criterion based on both the EFNRC (2005) and PCI (2003) recommendations. Table 4.5: SCHPC and SCHPFRC mixes (kg) that met both flowability and passing ability tests Constituents (kg) Ratios Slump Mix 14 Mix 15 Cement Microsilica Limestone Sand < 2 mm Coarse aggregates < 1 0 mm Water Superplasticiser Fibres 0 39 Water/binder SP/water JRing flow spread Dj(mm) T5ooj(sec) 3 3 It should be mentioned that although the trial Mix 10 had satisfied both the flowability and the passing ability tests and thus did not require redesigning, it was the aim of this study to Page 92
117 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres develop a SCHPFRC mix from the same base SCHPC mix. This led to the development of Mix 14 which differs from Mix 15 only by the absence o f steel fibre. The mixes 14 and 15 (Figures 4.4 and 4.5) of Table 4.5 were flowable, homogeneous, and reached the target compressive strength 100 MPa. Figure 4.4: Flow and passing ability of SCHPC Mix 14 Figure 4.5: Flow and passing ability of SCHPFRC Mix 15 Page 93
118 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes w ith and w ithout Steel Fibres It should be mentioned that the slump and JRing tests can be performed by using an upright or an inverted cone. In this study both orientations were used and it was observed that in the inverted orientation the flow time Tsooj is slightly increased when large coarse aggregates are present. There was no discernible difference when such aggregates were absent, as in the mixes to be described below. 4.3 Development of SelfCompacting U ltra HighPerform ance Fibre Reinforced C oncrete (SCUHPFRC) In this section, the development of a SCUHPFRC will be described. The base mix is CARDIFRC mix I (Benson and Karihaloo, 2005a, b and Benson et. al., 2005). As can be seen from Table 4.6 this mix contains a total o f 6% by volume o f two types o f fibre: 6mm (5% by volume) and 13mm (1% by volume) long steel fibres (diameter 0.15mm). It is a very dense and highly viscous mix and is meant for vibratory compaction. However, the mix without the fibres is highly flowable and thus has the potential for selfcompaction. Table 4.6: Original CARDIFRC mix I (kg/m3) CARDIFRC Mix I Cement 855 C+l B Microsilica i+i Quartz Sand pm pm Water 188 V 1 Superplasticiser 28 a o Fibres 6 mm 390 (J Fibres 13 mm 78 Ratios Water/binder 0.18 SP/water 0.15 In the present development, the 6% by volume brasscoated thin fibres of the original CARDIFRC mix I was replaced by 2.5% by volume o f the cheaper 30 mm long steel Z560 Dramix fibres with 0.55 mm diameter. It was expected that such a replacement will lead to a reduction in the compressive (200 MPa) and indirect tensile (25 MPa) strengths o f the original CARDIFRC mix I, but not to its toughness because the main impact o f the long Page 94
119 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres fibres lies in enhancing the toughness of the composite. However, as 85% of the cost of the original CARDIFRC mix I is attributable to the expensive thin brasscoated fibres, the cost of the selfcompacting version using the much cheaper Dramix fibres will be substantially reduced, thus making it a highly competitive advanced cementbased construction material which can be used in many situations in which steel is currently the preferred option F low ability test Trial mixes were prepared from the original CARDIFRC mix I without fibres. The slump flow test was performed on the trial mixes to obtain a mix with the maximum flowability and homogeneity and least segregation. For the preparation o f each mix the mixing procedure used for CARDIFRC was followed (see section 4.2.1). Based on the experience with the SCHPFRC mix 15 (Table 4.5) reported above, which contained only 0.5% by volume o f the same type of fibres as envisaged in the present SCUHPFRC, it was planned to achieve a slump flow of 900 mm for mixes without steel fibres. Then 2.5% of 30 mm long steel Z560 Dramix fibres with 0.55 mm diameter were added to the mix and its flowability was checked again using the slump flow test. With the addition of steel fibres it was planned to achieve a slump of at least 500 mm and the flow time T500 of 3 sec SCUHPC and SCUHPFRC Selfcompacting ultrahigh performance concrete (SCUHPC) The constituents of CARDIFRC mix I without fibres were modified. Various water to binder ratios ( ) and SP to water ratios ( ) were tried to obtain highly flowable trial mixes. A part of the cement was replaced by ground granulated blast furnace slag (GGBS). GGBS maintains the cohesion of the SCCs mixes and hence prevents the segregation. It also reduces the heat of hydration and the cost o f the mixes. These trial mixes were then tested for flowing ability using the slump flow test. The trial mixes were prepared in both a planetary mixer (with a capacity of 81 kg) and a standard pan/liner drum mixer (with a capacity of 163 kg) to check the consistency in the results for the mixes in larger quantities. Figure 4.6 shows the procedure used to create a flowable SCUHPC. Page 95 /
120 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres Start CARDIFRC Mix I without fibres Change SPwater ratio and/or GGBS V Start trial mixing in planetary mixer Is the slump flow spread >900 mm? NO V Yes Yes Is there any segregation? No No Are the results consistent with those o f Pan mixer? Yes V SCUHPC Add fibres (see Figure 4.8) Figure 4.6: Procedure to create a flowable SCUHPC Page 96
121 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres Table 4.7 gives the composition of the trial mixes and the slump flow test results. Table 4.7: Composition of the trial mixes (kg) of SCUHPC Mix 1 Mix 2 Mix 3 Mix 4 Cement $ Microsilica Ground granulated blast furnace slag (GGBS) M 0) Quartz Sand pm C pm O Water U Superplasticiser Ratios Slump Water/binder SP/water Slump flow spread (mm) Planetary Mixer Pan Mixer 772 T5oo(sec) Planetary M ixer Pan Mixer 4 The following observations were made during the slump flow testing of the trial mixes without the steel fibres: In the first attempt (Mix 1 in Table 4.7) in the planetary mixer, a part of the cement (33.8%) in CARDIFRC mix I (without fibres) was replaced by GGBS. All other constituents were unchanged. The mix had a low flowability to the naked eye. Mix 2 was also prepared in the planetary mixer using Glenium ACE333 superplasticiser instead of the naphthalene sulfonatebased one, while keeping the SP to water ratio constant. It was observed that the horizontal slump flow increased by more than 200 mm in comparison with the old SP. However the T time was similar in both mixes. On the basis of the previous mix, it was decided to use only Glenium ACE333 SP in the remaining mixes. In Mix 3, the SP to water ratio was increased from 0.15 to 0.20 which gave a spread of 768 mm. Page 97
122 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres In the next mix (Mix 4), the GGBS content was increased by 8% while the cement content was decreased by 4%. It gave a slump flow spread o f 905 mm when mixed in the planetary mixer. To check whether it would give a similar result if mixed in large quantities this mix was prepared again in the standard pan mixer. It was observed that the slump spread was reduced. Table 4.8 gives the composition of SCUHPC mixes with a constant amount of solid constituents and a variable amount o f a viscosity modifying admixture (VMA). Table 4.8: Composition of SCUHPC mixes (kg) with a constant amount of solid constituents E a =OJ 3 M 3 O U Ratios Slump Mix 5 Mix 6 Mix 7 Mix 8 Mix 9 Cement Microsilica Ground granulated blast furnace slag (GGBS) Quartz Sand pm pm Water Superplasticiser Viscosity modifying admixture (VMA) Water/binder SP/water Slump flow spread (mm) Planetary Mixer Pan Mixer T5oo (sec) Planetary Mixer Pan Mixer In Mix 5, to increase the slump flow spread, 0.1% o f VMA (Glenium 2006L) by weight of cement was added to the mix in a standard pan mixer. This resulted in only a slight increase in the slump flow spread (785 mm against 772 mm). The amount of VMA was increased further to 5% by weight of cement in trial mix 6 which was mixed in a planetary mixer. But this step resulted in further reduction of the slump flow. Page 98
123 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres Mix 7 was prepared in the standa rd pan mixer. The superplasticiser to water ratio was increased to 0.22, while the VMA c content was held constant. But the slump spread did not reach the target value of 900 mm. In mixes 8 and 9, with new SP to w ater ratio held constant at 0.22, the content of VMA was changed to 0.1% and 0.2% by weij ght of cement. In both mixes, it was observed that the increase in the VMA content led 10 a decrease in the slump flow spread. Hence it was concluded that, the version of SC UHPC based on CARDIFRC mix I prepared in the laboratory did not require the addition of a VMA. The reasons might be as follows: Quantity of the mix: the qua mtity prepared in the laboratory is much smaller than that on an actual construction site W aterbinder ratio: onacc nstruction site, the water to binder ratio can be high and VMA is required to thicken t le paste, i.e. to enhance the plastic viscosity of the paste; W eather conditions: the n nixes were prepared and tested at room temperature (around 21 degree Celsius^ 1 when the evaporation of the liquids is practically negligible, whereas at higl tier temperatures, VMA may need to be added to compensate for evaporation. The VMA constituent was therefore discarded and it was decided to vary the water to binder ratios and SP to water ratios (Table AL9) to reach the target slump flow spread of 900 mm. Table 4.9: Effect of the variation of tllie waterbinder and SPwater ratios on the flowability of 3? SCUHPC Mix 10 Mix 11 Mix 12 Cement S / Microsilica M Ground granulated blast furnace slag (GGBS) s 4) a Quartz Sand pm ' C M pm O Water u Superplasticiser Ratios Water/binder SP/water Slum p Slump flow spread (mm) Planetary Mixer 950 Pan Mixer Tsoo (sec) Planetary Mixer 2 Pan Mixer Page 99
124 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres The detailed comments on the SCUHPC mixes presented in Table 4.9 follow: In the trial Mix 10 prepared in the standard pan mixer, the water to binder ratio was increased from 0.18 to 0.20 which gave a slump spread o f 940 mm. This was due to the increase in the water quantity which is not desirable in practice. Therefore this mix was ignored and it was decided to change the SP to water ratio, while keeping the water to binder ratio constant. For Mix 11, the SP to water ratio of 0.20 and waterbinder ratio of 0.18 were used. The slump flow spreads for the mixes prepared in the planetary and standard pan mixer were 950 mm and 820 mm, respectively. However the mix was rejected because o f the large difference in the flow spreads. In Mix 12, the SP to water ratio was increased to A slump o f 905 mm with T500 equal to 3 sec was obtained for the mix prepared in the standard pan mixer. The horizontal spread in the slump flow cone test is shown in Figure 4.7. Figure 4.7: Horizontal spread of SCUHPC mix 12 Page 100
125 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres Selfcompacting ultrahigh perform ance fibre reinforced concrete (SCUHPFRC) Mix 12 was selected as the starting mix to which 2.5% by volume of steel fibres were added. Figure 4.8 shows the procedure for achieving the SCUHPFRC. Start SCUHPC Change SPwater ratio Start trial mixing in planetary mixer Is the slump flow spread >500 mm? NO \ t Yes Yes Is there any segregation? No No Are the results consistent with those o f Pan mixer? Yes SCUHPFRC Test the passing ability Figure 4.8: Procedure for achieving the SCUHPFRC Page 101
126 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and without Steel Fibres Table 4.10 gives the composition o f the SCUHPFRC trial mixes with steel fibres. Table 4.10: Composition of SCUHPFRC mixes (kg) with steel fibres Mix 13 Mix 14 Mix 15 Mix 16 Cement Constituents (kg) Ratios Microsilica Ground granulated blast furnace slag (GGBS) Quartz Sand pm pm Water Superplasticiser Fibres Water/binder SP/water Slump flow spread (mm) Planetary Mixer 900 Slump Pan Mixer T (sec) Planetary Mixer 3 Pan Mixer The following observations were made when SCUHPFRC trial mixes with steel fibres were prepared. 2.5% by volume o f steel fibres were added to Mix 12 in the standard pan mixer giving the trial mix 13. The fibres were evenly distributed in the mixer, as can be seen in Figure 4.9. Figure 4.9: Horizontal spread of SCUHPFRC mix 13. The fibres are evenly distributed Page 102
127 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes w ith and w ithout Steel Fibres From this trial Mix 13 it became clear that the mix did not lose its workability even after the addition of 2.5% by volume fibres. The slump flow was expected to reduce by about mm after the addition of fibres but in actual fact it reduced by only 100 mm. This showed that the final mix had very good workability and the target initial slump flow of 900 mm had been overestimated. Thus a flowable mix with fibres would be possible to make even after reducing the SP to water ratio below Therefore in the next trial mix i.e. Mix 14 the SP to water ratio was reduced to 0.15 and a slump flow of 900 mm and 750 mm were achieved on mixes made in the planetary and standard pan mixers, respectively. In Mix 15, the SP to water ratio was further reduced to 0.11 which gave a slump flow of 750 mm with very good distribution of fibres, even at the edges of the slump flow. In this mix the SP to water ratio was initially chosen to be 0.1 during the mixing process. Additional superplasticiser (0.01) was added at the end to increase the workability on the basis of visual observation. The SP to water ratio was further reduced to 0.10 in Mix 16 which was made in the standard pan mixer. A slump flow of 700 mm and T equal to 3 sec were achieved. But as can be seen from Figure 4.10, the SCUHPFRC seems drier than Mix 13 (Figure 4.9) although it is still workable. Figure 4.10: Horizontal spread of SCUHPFRC mix 16 Page 103
128 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres The segregation resistance o f the SCUHPC/SCUHPFRC mixes was judged by visual inspection of concrete in the mixer and after the slump flow test. However as can be seen from Figures 4.7, 4.9 and 4.10, no segregation o f particles occurred during the tests. This is due to the fact that CARDIFRC mix I is a highly optimised mix with excellent homogeneity because of the absence of coarse aggregates (as can be seen from Table 4.5, the maximum size of the fine aggregates used is only 600 pm) Passing ability test As before, the mixes of SCUHPFRC were subjected to the passing ability test in the JRing apparatus, with the cone in the inverted orientation for it could not be placed in the ring in the upright position because of the lifting lugs attached to its base. The Mix 12 without fibres easily and smoothly flowed through the gaps between the steel rods reaching a spread of 900 mm, with the spread Tsooj timed at 3 sec (Figure 4.11). Figure 4.11: SCUHPC mix 12 flows smoothly through the gaps between the steel rods Page 104
129 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres Mix 16 could not meet the passing ability criterion as it has a lower SP to water ratio. The steel fibres block the spaces between the rods and prevent the SCC mix to pass through them. The JRing test was repeated with a SCUHPFRC mix that had a higher amount of SP. Mix 13 was selected with a SP to water ratio of The Mix 13 also did not satisfy the passing ability test. Some fibres nested around the steel bars, preventing the remaining fibres to pass through the gaps (Figure 4.12). It was therefore necessary to improve the passing ability of this mix by increasing the superplasticiser content. However, the superplasticiser content was also increased by the same amount in the base mix 13 without fibres in order to maintain commonality between the SCUHPC mixes with and without fibres. The SPwater ratio had to be increased from 0.22 of mixes 12 and 13 to 0.28 in order to satisfy the passing ability test (Figures 4.13 and 4.14). The mix proportions of these mixes, designated SCUHPC mix 17 and SCUHPFRC mix 18 are given in Table The compressive strength of SCUHPFRC mix 18 was measured at 162 MPa after 7 days of hot curing at 90 C. As expected, it is less than the compressive strength (200 MPa) of the original CARDIFRC mix I because of the reduced fibre content. Figure 4.12: SCUHPFRC mix 13 did not satisfy the passing ability test. The fibres are nested around the steel rods Page 105
130 Chapter 4: Development of SelfCompacting High and Ultra High Perform ance Concretes with and w ithout Steel Fibres Table 4.11: Mix proportions of SCUHPC and SCUHPFRC mixes (kg) meeting the flowability, cohesiveness and passing ability criteria SCUHPC Mix 17 SCUHPFRC Mix 18 Cement Microsilica g Ground granulated blast furnace slag (GGBS) a c Quartz Sand pm I pm J /2 Water J Superplasticiser Fibres 195 ios Water/binder SP/water m p JRing slump flow Dj(mm) Planetary Mixer St. Pan Mixer T5ooj (sec) Planetary Mixer St. Pan Mixer 3 3 Figure 4.13: Flow and passing ability of SCUHPC mix 17 Page 106
131 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes with and w ithout Steel Fibres Figure 4.14: Flow and passing ability of SCUHPFRC mix Concluding rem arks The development o f selfcompacting highperform ance and ultra highperformance concrete mixes is a complex process requiring the resolution o f conflicting demands o f flowability and nonsegregation. W hilst these demands can be reconciled by increasing the paste content and decreasing the large aggregate volume, the resulting selfcompacting mixes may not reach the target compressive strength. The easiest way to meet the strength requirem ent is to include steel fibres in the mix. This can however compromise the ability o f the mix to flow smoothly through gaps in the reinforcement and to cause segregation of the fibres. The extensive investigations in this chapter led to the following m ajor conclusions. Selfcompacting high and ultra highperform ance concrete mixes without fibres may be designed to satisfy only the flow ability and cohesiveness criteria using the slump flow test. However, w hen long steel fibres are present in the mixes, it is additionally Page 107
132 Chapter 4: Development of SelfCompacting High and Ultra High Performance Concretes w ith and w ithout Steel Fibres necessary to check that the mixes meet the passing ability criterion using the JRing apparatus. It can be concluded that although the mixes with fibres meet the flowability and cohesiveness criteria, as judged by the slump flow test, they may not meet the passing ability criterion. These mixes need to be more flowable than required by the slump flow test, in order to satisfy the passing ability test. In the next Chapter we shall develop micromechanical models for estimating the plastic viscosity of SCC mixes. In particular, we shall estimate the plastic viscosity of the SCHPC/SCHPFRC and SCUHPC/SCUHPFRC mixes developed above. Page 108
133 C hapter 5 Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres
134 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 5.1 Introduction The rheological study of concrete is of prime importance for the construction industry because concrete is placed in its plastic state. This is even more relevant when dealing with a selfcompacting concrete (SCC) (Heirman et al., 2008; Petit et al., 2007). However, there is as yet no systematic coverage of this topic in the literature. Part o f the reason for this may be the various ranges of particle size used in the concrete industry (as seen in Chapters 2 and 4) and the different devices used (as seen in Chapter 3) to measure the plastic viscosity (Laskar and Talukdar, 2008; Kuder et al., 2007; Westerholm et al., 2008) o f the heterogeneous concrete mix. The plastic viscosity, together with the yield stress o f the SCC mix, is needed to study the flow of concrete. The flow of SCC with or without fibres is best described by the Bingham constitutive model. As stated in Chapter 3, this model contains two material properties, namely the yield stress ry and the plastic viscosity rj. It is known, however, that the yield stress of SCC mixes is very low in comparison with normal concretes. Moreover, the yield stress of SCC mixes remains nearly constant over a large range o f plastic viscosities (Dransfield, 2003). The aim of this chapter is to develop a micromechanical basis for determining the plastic viscosity of selfcompacting high and ultrahigh performance concretes (SCHPC/SCUHPC) with and without steel fibres (developed in Chapter 4) from the knowledge of the plastic viscosity of the paste alone. The latter can be measured with a reasonable degree of confidence, whereas the measurement of the plastic viscosity of the concrete mix is fraught with many difficulties and inaccuracies, especially when steel fibres are present. The plastic viscosity o f the mixes with and without steel fibres will be estimated from the known plastic viscosity of the cement paste using micromechanical relations. The predictions of this micromechanical approach are shown to correlate very well with available experimental data. Comments will be made on the practical usefulness of the predicted plastic viscosity in simulating the flow o f SCCs. The major part of this Chapter has been published in a journal (see publication 1 in the list in Chapter 1) and also reported at an International Conference (publication 6 in the list). Page 110
135 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 5.2 Methodology Micromechanical constitutive models are used to predict the plastic viscosity of selfcompacting high and ultrahigh performance concretes with and without steel fibres from the measured plastic viscosity of the paste. The viscosity of a homogeneous viscous fluid such as the cement paste can be measured accurately, which cannot be said about nonhomogeneous viscous fluids such as SCHPFRC and SCUHPFRC. The concrete is regarded as a twophase suspension in which the solid phase is suspended in a viscous liquid phase. The liquid matrix phase consists o f cement, water and any viscosity modifying agent (VMA) to which the solids (fine and coarse aggregates and fibres) are added in succession. The plastic viscosity of this liquid matrix phase is assumed to be known. The increase in plastic viscosity due to the addition of a solid phase (i.e. any cementreplacement materials, fine and coarse aggregates) to this matrix is predicted from the twophase suspension model. The model is applied in stages; in the first stage, the solid phase is the finest solid material which could be the cementreplacement material in the viscous fluid (cement paste). In the next stage, when the second finest solid (it could be the fine aggregate) is added, the suspension from the first stage is regarded as the continuous fluid matrix phase. This procedure is continued until all the solid phase constituents have been added to make the SCC. The plastic viscosity of the viscous concrete consisting of the liquid and solid phases is further increased if steel fibres are added to it. The volume fraction of steel fibres is usually small, so that the dilute approximation is sufficient. In order to estimate the effect of the addition of steel fibres, these are treated by the rigid slenderbody approximation in a viscous medium (Russel, 1973; PhanThien and Huilgol, 1980). The main assumption in this approximation is that the fibres undergo only a rigid body motion in the viscous flow, i.e. translation and rotation, but no elastic deformation (i.e. no bending). Figure 5.1 shows the hierarchy of these twophase liquidsolid suspensions used in the estimation of the plastic viscosity o f SCC mixes based on the viscosity of the cement paste Page 111
136 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s _ used in them. At each stage, the suspension consists o f a continuous liquid phase in which is suspended a discrete solid phase. CRM (S) Fine sand (S) Coarse sand (S) Paste (L) Paste+CRM (L) Paste+CRM+ FS (L) Vci  Vc\fl (^2 ) *7c3 Coarse Aggregate Fibres Paste+CRM+ FS+CS (L) Visous concrete (L) n C4 ~ (^4 ) 7 = H c J s ( t s ) Figure 5.1: Hierarchy of twophase liquidsolid suspensions constituting a SCC mix with fibres, showing the liquid (L) and solid (S) phases in each suspension The plastic viscosity o f the ith liquidsolid suspension can be estimated from the plastic viscosity o f the preceding (il)th phase as follows = =r)c,/ nc,! (5.1) with rjco = rjpaste being the known plastic viscosity o f the cement paste. For instance, with reference to Figure 5.1, the cement replacement materials form the solid phase in the viscous cement paste in the first liquidsolid suspension. The viscosity of this suspension is calculated from the known viscosity of the cement paste. This process is repeated until all the ingredients of SCC have been accounted for. In the final fluidsolid suspension, the increase in the viscosity induced by a dilute concentration o f long steel fibres is estimated. In the following sections the relative viscosity, / ( $ ) (or rjr) which is a function o f the volume fraction o f solid phase $, will be discussed. Page 112
137 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 5.3 Plastic viscosity of selfcompacting concrete without steel fibres Selfcompacting concrete as a concentrated suspension of solid particles in a viscous liquid The SCC consists of solid aggregate particles (solid phase) suspended in the viscous paste (liquid phase). The particles are modelled as spheres. The viscous behaviour of the resulting suspension depends on the volume fraction of the solid phase. At low concentrations of the solid phase, the plastic viscosity of the suspension does not change much with the shear rate, so that it is reasonable to assume that the suspension behaves like a Newtonian fluid. The behaviour becomes nonnewtonian once the volume fraction of solids reaches a critical value, roughly equal to </>m  the maximum attainable volume concentration which will be defined later. The other parameters influencing the viscosity of the suspension are the shape, size, and distribution o f the solid phase particles, especially at high concentrations Low concentration ( ^ < 0.1) A low concentration of solid phase is also called dilute, in the sense that the particles are sufficiently far apart from one another, so that the relative motion of the fluid near one particle is unaffected by the presence of the others and the hydrodynamic interaction of the particles can be neglected (Batchelor, 1971). Einstein (see, e.g. Struble and Sun, 1995) was the first to derive the viscosity o f a dilute suspension of rigid spheres. He showed that the addition of second phase to a suspension leads to an increase in the bulk viscosity proportional to volume fraction o f particles: (5.2) is the relative viscosity, i.e. ratio of viscosity of the suspension (mortar or concrete) to that of the liquid phase (cement paste), <f>t is the volume concentration o f particles, and [77] is the intrinsic viscosity which is a measure of the effect of individual particles on the viscosity (Struble and Sun, 1995). (5.3) Page 113
138 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres A value of [77] = 2.5 is adopted when the particles are rigid and packed randomly in a hexagonal arrangement, and the distance between them compared to the mean particle diameter is large. It is also important that the movement of the particles is sufficiently slow so that their kinetic energy can be neglected. Einstein s equation has been widely used by other researchers in this field even at higher volume concentrations o f particles. Ford (as stated by Shenoy, 1999) modified Einstein s equation using a binomial expression: (5.4) As reported by Utracki (2003), Simha (1952) modified Einstein s relation to read / ($) = /(o, W>t, where / ( a, ) is the socalled shielding factor, by using a cage model and a reduced volume fraction, $ / (f>m, where (f)m is the maximum packing fraction. In this model each solid spherical particle of radius a is placed inside a spherical enclosure (cage) of radius b. A simplified version of the resulting equation for a low volume concentration can be written as: / ( * ) = * V*W (5.5) Based on the Simha calculation for concentrated suspensions, Thomas arrived at the following relation for dilute suspensions (as cited by Shenoy, 1999): f M ) = * >j v (5.6) For low volume fractions, ai= High concentration (0.1 < ^ <<f>m) At higher volume concentrations of particles, the volume fraction is not the only parameter that influences the viscosity. It is now necessary to consider the size and type of particles used and their hydrodynamic interaction. The general expression of the viscosity can be written as Page 114
139 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s (Shenoy, 1999; Utracki, 2003; Bames et al., 1993; Mittal and Kumar, 1999; Gupta, 2000; Willis and Acton, 1976) + < # * + . (57) where B (in some references this is called Huggins coefficient) and C are very sensitive to the structure of suspension. Tables 5.1 and 5.2 give the values of constants B and C that have been reported in the literature (Shenoy, 1999; Willis and Acton, 1976; Batchelor, 1977; Guth and Simha, 1936; Vand, 1948; Saito, 1950). Table 5.1: Different values for parameter B available in the literature Reference Shenoy, 1999 Shenoy, 1999 Willis and Acton, ( ) Batchelor, ( ) Guth and Simha, ( ) Vand, ( ) Saito, ( ) de Kruif, ( ) B value Table 5.2: Different values for parameter C available in the literature Reference Shenoy, 1999 Vand, ( ) de Kruif, ( ) C value The variation in the cited values of parameters B and C is the result of taking into account one or several effects appearing due to the increase in solid concentration. Thomas (as stated by Mittal and Kumar, 1999) suggested that the C term in (5.7) could be replaced by an exponential term / ( 4 ) = ^ exp(l 6.6^ ) (5.8) because the resulting expression fits the experimental data very well in the range o f ^ = In view o f the uncertainties in the parameters B and C, Krieger and Dougherty (1959), and others, have used the concept o f maximum packing fraction, (j)m for a better description o f the suspensions. (f>m corresponds to the situation in which the particles have the minimum possible separation, i.e. the void fraction (porosity) is the least and the viscosity is infinite. Page 115
140 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres The value is 0.74 for hexagonal closed packing, for random hexagonal packing and for cubic packing (Shenoy, 1999). Krieger and Daugherty (1959) proposed a generalized version of Einstein s equation; they used the maximum packing volume fraction and intrinsic viscosity parameter to a non Newtonian suspension of rigid spheres. Ball and Richmond (as stated by Barnes et al., 1993) used the results of Krieger and Dougherty but simplified their complex mathematics conceptually based on Einstein s equation. It starts from an averaging technique such that the effect of all the particles in a concentrated suspension is the sum of the effects of particles added successively. Therefore the Einstein equation (5.2) can be written in a differential form as: 4fM) = lvv4 (5.9) They have pointed out that this neglects the correlations between spheres due to their finite size. This means that when a particle is added to a relatively concentrated suspension it requires more space than its volume dfa, due to packing difficulties. Therefore dfa has to be replaced by dfa / (l  K<j>t), where K is the socalled crowding factor. The viscosity of the final suspension is then obtained by integrating the phase volume between 0 and $. This gives: JIW) = 0  * * r wr (5.10) From this equation it can be seen that the viscosity becomes infinite when ^, = 1/ K. Thus one can replace \/K by the maximum packing fraction <pm. The KriegerDougherty equation is: (5.11) <f>m is strongly dependent on the particle size distribution. Also, the intrinsic viscosity [77] and <j>m depend upon the shear rate; the former tends to decrease with increasing shear rate whereas the latter shows the opposite trend. However [77] and <f>m change in such a way that Page 116
141 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres an increase in the one leads to a decrease in the other, but the product of the two changes remains practically the same and equal, on average, to 1.92 for rigid spheres (de Kruif et al., 1985). It should be noted that the Krieger and Dougherty equation (5.11) has been successfully tested by Struble and Sun (1995) on cement paste. Frankel and Acrivos (1967) derived theoretically an equation for the viscosity of a very high concentration o f solid spheres in suspension, i.e. when $ m ) = \ r (5.12) As reported by Shenoy (1999), their aim was to derive an expression to complement Einstein s equation for dilute suspension. This equation fits the experimental data for high volume fraction o f solid particles rather well: Chong et al. (1971) obtained a single expression to cover the entire range o f volume concentrations from <f>t 0 to $, </>m which fits the experimental data well / ( * ) = i+ 4,! 4. (5.13) They added direct Brownian contribution to the viscosity in the range o f 4>J <j)m< 0.7 because it leads to a slight increase in the relative viscosity. However, it should be mentioned that the Brownian contribution can be neglected at higher volume fractions, as confirmed theoretically by Ball and Richmond (as stated by Barnes et al., 1993). Equation (5.13) reduces to Einstein s equation (5.2) at low volume fractions. The drawbacks o f applying the </>mbased relations to predict the plastic viscosity o f concrete are twofold; firstly, due to the difficulties faced in the measurement o f viscosity when ^ is large ( $» <f>m). Secondly, it is difficult to determine the maximum volume fraction accurately because of the swelling in particles, adsorbed surface, etc (e.g. Ball & Richmond in Barnes et al., 1993). Page 117
142 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Are the expressions for the viscosity of a suspension of solid particles in a viscous fluid applicable to cement paste? The theoretical expressions discussed in the previous Section are generally applicable to a suspension of solid particles in a viscous fluid at low shear rates. As previously mentioned the Krieger and Dougherty equation (5.11) has been used successfully on Portland cement paste and fits the data well (Struble and Sun, 1995). If the concrete in its fresh state is assumed to be an isotropic material then the theory applicable at low shear rates has been demonstrated experimentally by Barnes et al. (1993) to be applicable also at high shear rates. They have combined the data from Krieger (1959) and de Kruif et al. (1985) for zero and infinite shear rates and fitted these data to (5.11) as shown in Figure " o /(<*> /(#)atr»0) 10'   \ os\ 10  fa4>i) / ( $ ) aat t r y »»oo o o L ± Volume fraction q>j \ Figure 5.2: Dependency of relative viscosity on the shear rate in a suspension at zero and infinite shear rates and fit to the Krieger and Dougherty equation (After Struble and Sun, 1995) The effect of shear rate is to alter the packing arrangement. Thus, whilst the packing is random hexagonal at low shear rates, it becomes more and more like closed hexagonal at high rates. The densification of packing at high shear rates is associated with shear thinning such that the product is constant and equal to about It is clear however from Figure 5.2 that the shear rate has little influence for volume fractions less than <f>t = 0.4. However, for Page 118
143 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s comparison with test data which have been obtained at high shear rates, the values of [tj] and <j>m corresponding to the lower curve in Figure 5.2 will be used later. All the above mentioned equations for high volume fraction of particles have been the subject of experimental verification, some of them even on cementbased materials (e.g. Struble and Sun, 1995). They give similar predictions in the range o f 0.1 < < 0.4 with only the Frankel and Acrivos (1967) equation deviating slightly from the rest (Figure 5.3). 11 ~x A X X A I <*> o W / (J C / 2 > I V i i X X Al J2 "S QC m\ i * iij i*!* V olum e fra c tio n o f solid p h ase(% ) Thomas (5.8) A Krieger&Dougherty (5.11) Frankel&Acrivos (5.12) X Chong et al., (5.13) Figure 5.3: Comparison of different formulas for high volume fraction of spherical particles with (f)m =0.708 and [7] =2.71 Page 119
144 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s Other attempts to derive the viscosity of suspensions based on volume concentration of solid particles are summarised in Table 5.3. Table 5.3: Equations of the viscosity of suspensions based on volume concentration of solid Equations / \ particles References m. Mooney (1957) / ( * ) =! + f M )=  1 i  i. <t>n, Robinson (1957) Quemada (1984) V Q m ) fm )= i ^  K j j Eilers (1941) modified by Wildemuth and Williams (1984) 5.4 Effect of fibres on the viscosity of SCC The effect of a dilute concentration (up to 3% by volume) of slender steel fibres on the plastic viscosity o f the selfcompacting concrete is estimated by applying Russell s slender body approximation, as described by PhanThien and Karihaloo (1994). In this approximation, the fibres are treated as slender rigid bodies whose rigid body translation and rotation are restricted as a result o f the resistance offered by the viscous selfcompacting concrete. Because the fibre is treated as a rigid body, the resisting force may be concentrated at the centroid of the fibre as shown in Figure 5.4. Page 120
145 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres z Figure 5.4: Rigid body translation and rotation of a single fibre resisted by the viscous SCC. The resistive concentrated force (F) is shown at the centroid of the fibre The resisting force components are given by (PhanThien and Karihaloo, 1994) (5.14) where iii are the components of the displacement rate (i.e. velocity) of the fibre centroid in the x, y and z directions, and C, depends on the viscosity o f concrete, the length of fibre and its aspect ratio. It is given by: itcrjl ln(2/ ) (5.15) where rj is the plastic viscosity of the mix without fibres, and / is the length of the fibre with ld its aspect ratio. Page 121
146 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres The effective stress tensor of a dilute suspension can be written as the contribution from the matrix and the fibre fabric tensor. The fibre fabric tensor depends upon the number of fibres. The effective stress tensor of the viscous suspension with matrix designated m and fibre/ is: (5.16) where <f>f is the volume fraction of fibres and the angular brackets represent the ensemble average Replacing ensemble average by volume average For a statistically homogeneous and random distribution of a dilute concentration of fibres in the viscous matrix such that the fibres are unlikely to overlap (Figure 5.5), the ensemble average can be replaced by the volume average over a representative volume element (RVE). Therefore, the ensemble average used in (5.16) can be replaced by its equivalent volume average, so that the bulk stress for a representative volume element is changed to: (5.17) / / / A / /\ / 1 / / / / /\l / / /\ / / \ V / \ / 1 / RVE \ / )/ / / / / T / \ / / / 1 \ / l / / \ / / / / \ \ / \ / \ / / l / Figure 5.5: The ensemble average can be replaced by volume average if the fibres are homogeneously and randomly distributed Page 122
147 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Equation (5.17) consists of two parts, i.e. the matrix part v vu and the fibre part *7 If volume of a single fibre is Va, then Vf ~ ^ V a. Therefore, the fibre contribution to the a stress tensor can be written as ( 7»)/ = p I J < v * (518> «v With reference to Figure 5.4, if the body force and inertia effects are neglected then it can be shown that (5.19) where a comma denotes the covariant derivative. Therefore, (5.18) can be rewritten as ( '»)/ = f Z J ( V ; ) i1a (520) r a v 9 a Applying the divergence theorem (Gauss theorem) on (5.20) yields f V a A, (5.21) The integral is taken over the fibre surface area and the sigma sign represents the summation over the total number o f fibres in the statistically homogeneous volume V. By definition, xja iknk traction force and it can be written as F r. Therefore (5.21) becomes (522) Page 123
148 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres where Aa, F and r denote the fibre surface area, the traction force and the position vector of the centroid of the fibre in the deformed configuration (distance from origin of xyz coordinate system, Figure 5.4), respectively. There is no guarantee that the fibre tractions are symmetric, i.e. F /j * rtf j, therefore, the fibre fabric tensor is averaged over the total number o f fibres (5.23) where N is the number of fibres, r. are the components of the position vector of the centroid in the deformed configuration (see Figure 5.4), and angular brackets denote volume average R andom distribution of fibres Let us consider two fibres with unit vectors p i and pj along their length, and require that the product be p,pj = a s,j (5.24) where Sy is the Kronecker delta. This requirement is consistent with the assumption of a dilute suspension of fibres i.e. «1 so that at no instant is there a situation when two fibres overlap each other. In order to find the value of the constant Ay let us set/ = j, then the left hand side of (5.24) is equal to one, because it is a multiplication of a matrix by its transpose. Thus, A = 1/3. Finally for a random distribution of fibres (5.25) This ensures that the fibre contribution is isotropic. Page 124
149 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Calculation of the fibre fabric tensor If components of the traction forces applied on the fibres are known (i.e. F/j or r.fj) then the fibre fabric tensor can be determined using (5.23). First, note that the displacement rate components (u i ) in (5.14) can be written as (5.26) where stj is the strain rate tensor. Also from Figure 5.4 (5.27) Because pt = 8ijpj and 1^ = //?,, (5.27) can be rearranged using (5.26) as (5.28) Substitution of (5.15) into (5.14) and the application o f (5.28) gives the components of (5.23) 27rrjl3. rj = ln(2i f S*PtPj (5.29) (5.30) Substituting (5.29) and (5.30) into (5.23) yields (5.31) By definition, the volume fraction of fibres is <t>f = Nal (5.32) where a is the fibre crosssectional area and / its length. Also, the aspect ratio can be estimated as (5.33) Therefore (5.32) gives Page 125
150 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres N P = M 2 (5.34) Finally, (5.31) can be written as = W^^,kPkPj+*,tPkP'} ( As demonstrated by (5.25) for random distribution of fibres (# /?,) = ) > (5.35) can be simplified as (<t ) U + g \ (5 36) v J,f 31n(2ld) K * "> K (eji+gij) can be replaced by the equivalent engineering shear rate yl}, giving Thus the effective stress tensor (5.16) of the viscous suspension can be written as = (538) The above tensor is isotropic. In particular, the shear stress components are related to the shear rates. In view of isotropy, we can, for example, write < ^  r = (i (5 39> The other two shear stress components are likewise related to the corresponding shear rates. We may therefore drop the suffixes and write the effective viscosity of the suspension with fibres, r! y as ^y} (540) The second term on the right hand side is the contribution of the fibres to the plastic viscosity of the mix without fibres. It is clear that this contribution increases linearly with the volume fraction of fibres. The effect of the aspect ratio on this contribution is more complex, as will be demonstrated below. Page 126
151 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 5.5 Comparison of the proposed formulae with test results Extensive experimental work has been done on selfcompacting fibre reinforced concretes by Griinewald and Walraven (2003) who used a BML rheometer to measure the viscosity of many mixes. Here only the first seven optimised series (OS) of their mixes have been used and their measured plastic viscosity compared with the predictions. The mix proportions can be found in Appendix B. Some o f the main parameters were as follows: the size of coarse aggregate varied from 4 to 16mm and that o f sand from to 4mm, paste volume from 34 to 39%, paste solid content from 53 to 55.7%, water to cement ratio from 0.42 to Four types of Dramix steel fibre (RC and RL types) were used with aspect ratios o f46.3, 64.9, 78.5 and 85.7 in concentrations of 80, 100, 120 and 140 kg/m3 in the mix. The fibres replaced the aggregates so that the ratio o f sand to total aggregate remained constant Plastic viscosity of cement paste The plastic viscosity of the paste used in each of the seven SCC mixes (Griinewald and Walraven, 2003) is estimated from the data available in the literature that most closely approximates the actual paste used in the mix. It should be mentioned that the plastic viscosity of cement paste is affected by the type and dosage of superplasticiser (Lachemi et al., 2004; Mikanovic and Jolicoeur, 2008; Cyr et al., 2000), type o f cement additives (Cyr et al., 2000; Ferraris et al., 2001b), mixing sequence and time (Aiad et al., 2002; Femandez Altable and Casanova, 2006; Williams et al., 1999), besides the main factors, i.e. the water to cement ratio and amount of superplasticiser in relation to cement and water used. It appears that there is a threshold to the amount of superplasticiser beyond which the plastic viscosity of the paste actually drops. The plastic viscosity o f the paste has been estimated from the data in the literature (Lachemi et al., 2004; Chindaprasirt et al., 2008; Sun et al., 2006; Grzeszczyk and Lipowski, 1997; Nehdi and Rahman, 2004; Zhang and Han, 2000); the estimated plastic viscosity of the paste is shown in Table 5.4, based on the paste content, paste solid content (%) and water to cement ratio. Page 127
152 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s In view of the fact that the main factors that control the viscosity o f the cement paste, enumerated above, vary only marginally in the seven mixes, it is not surprising that the plastic viscosity of the pastes also varies marginally. Table 5.4: Estimated plastic viscosity of the paste. The superplasticiser to water ratio is 0.02 (0.03 for Mix3) and the superplasticiser to cement ratio is 0.01 Paste property Mixl Mix2 Mix3 Mix4 Mix5 Mix6 Mix7 Paste content (%) Paste solid content (%) Water/cement Plastic viscosity (Pas) Plastic viscosity of selfcom pacting fib re reinforced concrete Once the plastic viscosity of the paste has been estimated, the increase in the plastic viscosity due to the addition of a solid phase (i.e. cementreplacement materials, fine and coarse aggregates) to this paste is predicted from the above twophase suspension model. The model is applied in stages (see Figure 5.1); in the first stage, the solid phase is the finest solid material which is the cementreplacement material in the viscous fluid (cement paste). In the next stage when the second finest solid (i.e. fine aggregate) is added, the suspension from the first stage is regarded as the continuous fluid matrix phase. This procedure is continued to until all the constituents used in the aforementioned SCC mixes have been taken into account. The plastic viscosity increase in SCC relative to the fluid phase without fibres is thus: / ( * ) = / W ) /2 ( A )  f M ) (5 41) * = (542) Vi + V0 where n. total number of solid phases in the mix, such as coarse aggregate, sand, and cement additives; v,: volume of solid phase i; v0: volume of the continuous matrix phase in which the solid phase i is suspended; : one of the several twophase relations introduced in Section Finally, to obtain the plastic viscosity of SCC with steel fibres, the result of the application of (5.41) to the SCC mix is used in (5.40). Here, the Krieger and Dougherty equation (5.11) will be used as the function /( ^,) in (5.41) because it has been found to be the most suitable for cementbased mixes (Struble and Sun, 1995). The values of [tj] = 2.5 and </)m=0.63 were Page 128
153 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e _ C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s _ used in this study. There are in fact thirty seven different mix combinations formed from the seven basic mixes (Griinewald, 2004), depending upon the fibre type, fibre content and aspect ratio, as shown in Table 5.5 below. We have also introduced two fibre parameters, 4>f l^ and 1 / ln(2ld) as they appear in (5.40). Table 5.5: Mix combinations based on the seven base mixes and the first and second fibre parameters; <J)f ld2 and l/ln(2ld) 4ix Designation No. Submixes by OS /36.5 (Mixl) OS /39.0 (Mix2) OS /36.5 (Mix3) OS /39.0 (Mix4) OS /34.0 (Mix5) OS /36.5 (Mix6) OS /39.0 (Mix7) fibre type, content (kg/m3) l/ln(2/</) Measured plastic viscosity (Pas) Predicted plastic Error (%) and aspect ratio viscosity (Pas) 1 D45/30,80, D45/30,100, D80/30 BP,40, D80/30 BP,60, D80/60 BP,40, D80/30 BP,60, D80/30 BP,80, D80/60 BP,40, D80/60 BP,60, D80/30 BP,40, D80/30 BP,60, D80/60 BP,40, D45/30,120, D45/30,140, /30,160, D65/40,100, D65/40,120, D80/30 BP,60, D80/30 BP,80, D80/60 BP,80, /30,100, /30,120, D80/30 BP.40, D80/30 BP,60, /30,120, D80/30 BP,60, D80/30 BP,80, D80/60 BP,40, D80/60 BP,60, D45/30,120, , /30,140, D65/40,80, D65/40,100, D80/30 BP,60, D80/30 BP,80, D80/60 BP,60, D80/60 BP,80, Page 129
154 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s Com parison of the predicted and m easured plastic viscosity with respect to first fibre param eter <f>f ld2 Figure 5.6 compares the measured and predicted variation of the plastic viscosity of SCFRC as a function o f the first fibre parameter, </>f ld for all the seven base mixes (Griinewald, 2004). Mixl 200 On a o v c ce i M P Fibre param eter, 250 Mix 2 i 150 M P Fibre param eter, <pjld2 Figure 5.6: Continued Page 130
155 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s M i x S 200 M P F i b r e p a r a m e t e r, (pjlj M i x <*> o cfi pp > 'V C / 5 CQ M P F i b r e p a r a m e t e r, <p/d Figure 5.6: Continued Page 131
156 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s 350 Mix CQ 04 ^ 250 * * 200 w > J5 M P Fibre param eter, <pjid2 Mix Fibre param eter, <pjd Figure 5.6: Continued Page 132
157 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s Mix 7 ce On o u ifi u p <S) 9 n M P Fibre param eter, <pjld Figure 5.6: Comparison of the plastic viscosity with experimental results vs. first fibre parameter, <f>ld2 for the seven main mixes with M" and P indicating measured and predicted plastic viscosity Predicted vs. m easured plastic viscosity w ith respect to second fibre param eter l/ln(2/^) It can be seen from Figure 5.7 that the predicted plastic viscosity is in very good agreement with the experimental data. The trend line has a high correlation with the second fibre parameter: R2 factors are 0.96, 0.93, 0.92 and 0.85 for fibre parameter values 0.22, 0.21, 0.20 and 0.19, respectively. Page 133
158 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s ? 300 & ~ 250 oft u R2 = & Ko2 T QA J2 a. a <u "3 su Measured plastic viscosity (Pas) Measured plastic viscosity (Pas) < FP=0.19 BFP= R2 = 0.93 ft & 250 B O 200 1*5Z w a a <y t5 *3 i a Measured plastic viscosity (Pas) Measured plastic viscosity (Pas) AFP=0.21 XFP=0.22 Figure 5.7: Predicted vs. experimental plastic viscosity as a function of the second fibre parameter l/ln(2/rf) for the seven main mixes The data in Figure 5.7 can be combined into a single diagram, shown in Figure 5.8. Page 134
159 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s eft S3 CL f / 3 0 W pat > c y a X "2L 100 1Pl M easured plastic viscosity (Pas) M = P 4 FP=0.19 FP=0.20 A FP=0.21 X FP= Figure 5.8: Combination of the data in Figure 5.7 for all the second fibre parameters l/ln(2/rf) Discussion of the results It is clear from Figures 5.6 and 5.7 that the proposed micromechanical relations are able to predict reasonably accurately the plastic viscosity of SCC mixes once the plastic viscosity of the cement paste is known. The accuracy o f the predictions is all the more remarkable given that the plastic viscosity of the paste was not measured but only estimated from similar pastes in the literature. It is quite likely that the predictions would be even more accurate when the viscosity of the paste is measured. The predicted trend, namely that the viscosity increases with increasing fibre parameters </>f ld2 and l/ln(2/,) is consistent with experience which shows that the flowability o f SCC with fibres is impaired both when the fibre volume fraction and/or the aspect ratio of the fibre are increased. Some of the measured values however do not Page 135
160 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s follow this expected and correct trend which must therefore be attributed to measurement inaccuracies. 5.6 Estimation of the plastic viscosity of selfcompacting high and ultra high perform ance concretes with and w ithout steel fibres Using the procedure described above, the plastic viscosities of the SCHPC and SCUHPC mixes with and without steel fibres developed in Chapter 4 can be estimated, if the plastic viscosity of cement paste is known. Based on the water to cement and the superplasticiser to water ratios, the plastic viscosities of the cement pastes used in the SCHPFRC (Table 4.5) and SCUHPFRC (Table 4.11) are estimated to be 0.4Pas and 0.3Pas, respectively. Table 5.6 shows the volume fractions ( $ ) o f the various constituents in the selfcompacting highperformance concrete mixes with and without fibres, SCHPFRC and SCHPC, o f Table 4.5. Table 5.6: Volume fractions of the SCHPFRC and SCHPC mix constituents Constituents Volume fraction in SCHPFRC Volume fraction in SCHPC Cement Microsilica Lim estone Sand < 2 mm Coarse aggregates < 1 0 m m W ater S u p erp lasticiser Fibres Table 5.7 shows the volume fractions ( $ ) of the constituents of in the selfcompacting ultra highperformance concrete mixes with and without fibres, SCUHPFRC and SCUHPC, of Table Page 136
161 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s Table 5.7: Volume fractions of the SCUHPFRC and SCUHPC mix constituents Constituents Volume fraction in SCUHPFRC Volume fraction in SCUHPC Cem ent Microsilica Ground granulated blast furnace slag (GGBS) Quartz Sand pm pm W ater S uperplasticiser Fibres The plastic viscosities of the SCHPC and SCUHPC mixes with and without steel fibres predicted using the procedure developed above are given in Table 5.8. Table 5.8: Plastic viscosities of SCHPC and SCUHPC mixes with and without fibres Plastic viscosity (Pas) W ithout fibres With fibres SCHPC (Mixes 14 an d 15 in Table 4.5) SCUHPC (Mixes 17 and 18 in Table 4.11) P ractical usefulness o f th e p ro p o se d m icro m e c h a n ic al m odel This section will briefly discuss the practical usefulness o f the proposed model for predicting the plastic viscosity of SCC mixes with and without fibres. As stated before, the constitutive flow behaviour of SCC is best described by the Bingham fluid model which requires the plastic yield stress ry besides the plastic viscosity. It is known however that the yield stress of SCC mixes is low (around 200 Pa) in comparison with normal concretes (thousands of Pascal) and remains nearly constant over a large range o f plastic viscosities (Figure 5.9). Page 137
162 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s Yield stress Normal concrete 5: ft Highstrength concrete Pumping/underwater concrete Flowi Selfcompacting concrete Plastic viscosity Figure 5.9: The yield stress of SCC mixes is nearly constant over a large range of plastic viscosity. (After Dransfield, 2003) Thus, the constitutive relation o f a SCC mix as a Bingham fluid can be immediately written once its effective plastic viscosity which depends on the mix composition and fibre parameters, and the plastic yield stress which depends only on the paste are known. From a practical point of view, it is expedient to represent the bilinear Bingham model with its associated discontinuity at zero shear rate by a continuous function (Papanastasiou, 1987) (5.43) where m is a very large number. It can be seen from Figure 5.10 that the continuous function (5.43) approaches the bilinear function for large m. Page 138
163 C h a p t e r 5 : P r e d i c t i o n o f t h e P l a s t i c V i s c o s i t y o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s Bingham Fluid m= 50 m=500 m=5000 n=50000 Figure 5.10: A bilinear Bingham fluid constitutive model replaced by the continuous function (5.43). On the scale of the figure, the discontinuity at Ty cannot be distinguished for m=5,000 and 50,000. However, at a magnification of 100 on the horizontal scale as shown in the inset, it is clear that the continuous approximation is better for m=50, Concluding rem arks The micromechanical procedure developed in this Chapter estimates the plastic viscosity of SCC mixes with or without steel fibres from the knowledge o f the plastic viscosity of cement paste alone or of the cement paste with SP and/or VMA. The plastic viscosity of the SCC mixes developed in Chapter 4 was estimated by this procedure. In this procedure, the SCC mix is regarded as a succession o f twophase suspensions solid and liquid phases. It was noted that the influence of the discrete solid phase on the plastic viscosity o f the continuous liquid phase depends only on the volume fraction o f the solid phase ft, if it is less than 10%. This influence was captured by the Einstein equation (or many of its later modifications) which contains the intrinsic viscosity [rj\. A value of 2.5 was adopted in this study because the particles are considered as rigid spheres with a large separation between the neighbouring particles compared to the mean particle diameter. Page 139
164 Chapter 5: Prediction of the Plastic Viscosity of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres However, when the volume fraction o f the solid phase exceeds 10% but is less than the maximum possible volume fraction <j>m, then the relative viscosity depends not only on the volume fraction of the discrete solid phase but also on how it is dispersed in the fluid and on the shape of the solid particles. In this case the formula proposed by Krieger and Dougherty (1959) was used. From this study the following conclusions can be drawn. The plastic viscosity of SCC mixes can be accurately predicted from the measured viscosity of the paste alone based on micromechanical principles. The latter give expressions that are accurate for viscous suspensions containing spherical rigid particles in large concentrations and/or needleshaped steel fibres (with aspect ratio up to 85) in dilute concentrations (up to 3%). The fibres were regarded as rigid slender bodies in a viscous medium whose free translation and rotation are restrained by the viscous concrete mix. However for steel fibres in larger concentrations and/or larger aspect ratios, the assumptions that the fibres are rigid and that they are statistically homogeneously distributed in the mix need to be reexamined. The plastic viscosity, together with the yield stress of the SCC mixes with or without fibres, is needed to simulate the flow both at the mix design stage, e.g. to simulate the flow in a slump flow cone or an Lbox test, and at the industrial use stage to simulate the flow in the formwork. For this simulation, it is o f course necessary to use computational tools. In Chapter 6 we have used the relation (5.43) to simulate the flow of SCHPFRC/SCUHPFRC in the cone and Lbox tests using the meshless smooth particle hydrodynamics method (Bonet and Kulasegaram, 2000) and have compared the results with actual measurements. Page 140
165 Chapter 6 Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres
166 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 6.1 Introduction In recent years, the selfcompacting concrete (SCC) is increasingly replacing conventional concrete in the construction industry. The need for very high durability structures demands excellent flowability o f SCC into the formwork. The filling behaviour of SCC is even more difficult to predict in the presence o f reinforcing steel and in formworks of complex shape. Therefore, in order to produce high quality SCC structures it is vital to understand fully the flow characteristics of SCC. The most costeffective way to gain such an understanding is by performing numerical simulations. These will not only enable us to understand the filling behaviour but will also provide insight into how the fibres will orientate themselves during the flow of SCC containing fibres. However, in reality it is not easy to model SCC or any such heterogeneous material flow due to their very constitutive properties. Any computational model for SCC flow should be able to describe accurately the Theological behaviour of SCC and to follow the large deformation and Lagrangian nature o f the flow. A brief overview of various computational techniques used in the past to model concrete flow and their advantages and disadvantages was given in Chapter 3. The computational strategies that have been attempted in the past are meshbased numerical simulations. However, in the simulation of the flow o f fresh concrete one has to take into account special features such as large deformations, large inhomogeneities and free surfaces. These special features pose great challenges to the numerical simulation using the gridbased methods. In this chapter, a Lagrangian particlebased technique, the socalled smooth particle hydrodynamics (SPH) method is chosen for simulating the flow o f selfcompacting high and ultrahigh performance concretes (SCHPC/SCUHPC) with or without short steel fibres (developed in Chapter 4). An incompressible SPH method is implemented to simulate the flow of these nonnewtonian fluids whose behaviour is described by a Binghamtype model, in which the kink in the shear stress vs shear strain rate diagram is first appropriately smoothed out (as described in Chapter 5). The viscosity of the selfcompacting concrete mixes is predicted from the measured viscosity of the paste using micromechanical models in which the second phase aggregates are treated as rigid spheres and the short steel fibres as slender rigid bodies (see Chapter 5). Page142
167 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres The basic equations solved in the SPH are the incompressible mass conservation and Navier Stokes equations ((3.20) and (3.28)). The solution procedure uses predictioncorrection fractional steps with the temporal velocity field integrated forward in time without enforcing incompressibility in the prediction step. The resulting temporal velocity field will be used in mass conservation equation (3.20) to satisfy incompressibility through a pressure Poisson equation derived from an approximate pressure equation (3.33). The results of the numerical simulation are benchmarked against actual slump tests carried out in the laboratory. The numerical results are in excellent agreement with test results, thus demonstrating the capability of SPH and a proper rheological model to predict selfcompacting concrete flow behaviour. The major part of this Chapter has been published in a journal (see publication 2 in the list Chapter 1) and also reported at two International Conferences (publications 4 and 5). 6.2 Governing Equations Selfcompacting concrete is assumed to have the characteristics o f a viscous nonnewtonian fluid, described by a bilinear Binghamtype rheological model in which the fluid flow only initiates once the shear stress has reached a critical value called the yield stress ry. Thereafter, the shear stress varies linearly with the shear rate y, the slope being equal to the plastic viscosity rj of the SCC mix. In Chapter 5, it was demonstrated how to predict the plastic viscosity tj of selfcompacting concretes with and without short steel fibres from the measured viscosity of the paste alone using micromechanical models in which the second phase aggregates are treated as rigid spheres and the short steel fibres as slender rigid bodies. It was also argued that the yield stress t of SCC mixes is practically unchanged over a very large range of plastic viscosities (see Figure 5.9). From a computational point of view, it is expedient to approximate the bilinear Bingham constitutive relation with a kink at y  0 by a smooth function with a continuous first derivative. As shown in Chapter 5, this function is given by T = riy + zy{ \  e mf) (6.1) in which m is a very large number. Experience has showed that when m > 105 the smooth function (6.1) is practically indistinguishable from the original bilinear constitutive relation (Figure 5.10). Page143
168 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres The isothermal, Lagrangian form o f the mass and momentum conservation equations derived in Chapter 3 are repeated here:  ^ + V  v = 0 (6.2) p Dt = V P + V.T + g (6.3) Dt o o In equations (6.1), (6.2) and (6.3), p, t, v, P, g and r represent the fluid particle density, time, particle velocity, pressure, gravitational acceleration and shear stress, respectively. Equation (6.1) determines the shear stress that influences the viscous force during the fluid flow as described by equation (6.3). The threedimensional (3D) and cylindrical forms of the vector equations (6.2) and (6.3) are given below D discretisation of mass and momentum conservation equations Mass conservation equation Multiplying both side of (6.2) by p and noting that the substantial derivative (or total time derivative) of density (~ ~ ) 0311 be decomposed into the normal derivative ( ~ ) the advective derivative ( v.v p) (see (3.10)) we can write p + v.vp + p V.\ = ^ +V.(pv) (6.4) dt \ d t j For a steadystate flow, p does not change with respect to time hence the term vanishes. Therefore, in Cartesian coordinates (6.4) can be rewritten as d(p vx) d(pvy) v xj + ± = 0 (6.5) dx dy K } When additionally the flow is incompressible, p is constant and does not change with respect to space, (6.5) is further simplified to Pagel44
169 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres dv dv + 2L = 0 dx dy (6.6) Momentum conservation equations Multiplying both sides o f (6.3) by p and noting that the material derivative (or total time D \ derivative) of velocity ( ) can be decomposed into the normal derivative ( ) and the D t dt convective derivative ( v.vv ) (see (3.10)), we can write ( d v x + p(v.vv) =  V P + pg + V.t P [d t (6.7) In Cartesian coordinates, (6.7) can be written explicitly as dv. + v. dvx_ dv,. dvx + V y + v z, dx dy dz dp =  + p g. + n * r 82v. d2v. d 2v ' Z dx dy dza (6.8) ( dv. dvy ^ y + v_ + Vv + V dx y dy z dvy dz dp dx2 dy2 dz2 (6.9) r dv. dvl dv^_ dvl + v_ 4 V v dt dx y z dy dz 8P =  + t> g.+ n + ^ d2v, d2v, d2v. ^ dx2 dy2 dz2 (6.10) where rjeff is the effective viscosity o f the fluid such that T = 7v ( / ) /  In the case of a Newtonian fluid it is constant. To obtain rj^ for a Bingham fluid, both sides of (6.1) are divided by y to give T y ( l  e  ' )  = rj + r r (6.11) The right hand side of (6.11) is rjgff. y is the shear rate which is defined as r = (6.12) Page145
170 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres (6.12) states that y is the second invariant o f the rate of deformation e, given by e = ~(V v + Vvr); Vv = V v (6.13) where Vv is the velocity gradient and superscript T denotes transpose, e in explicit form is xy f dvx_ f r k fr*. dvx f r y dv2 \ dx dy dz dx dx dx 1 f r y dv y + dvx f r y dv2 2 dx dy dz dy dy dy (6.14) \ dvz dv2 f r z dvx f r y f r 7 dx dy dz _ dz dz dz _ J Discretisation of mass and momentum conservation equations in the cylindrical coordinate system Mass conservation equation A change of variables from the Cartesian equations gives the following mass conservation equation in the cylindrical coordinates r, <j>, and z 1 d, x 1 dv ( r v ) ~ = 0 r dr r d</> dz (6.15) Momentum conservation equations Similar to (6.15), the momentum conservation equations are given by r component: p ''dv dvr v dvr dv, v 2 ^  + v_ v. dt dr r d(j> dz dp  dr +*+ 1 d f r  ^ d \ 2 dvf + # v; + Pgr r dr I d r ) r 2 d<f>z dzz r 2 r 2 d</>j (6.16) (f) component: p ^ I dt v f r * v, dv v f r VrV* \ ' dr r d</> dz r J dp "l d r r fr * ' 1 5 % dv, vr ? + T r dr \ dr J r 2 d f dz2 r 2 d^> r 2 (6.17) P agel46
171 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres z component: p dv, dv, v<pdv, +v_ dt dr r d</> dp dr + I d_ r dr dv v  dv± dr dz i s Y + r L d f a V dz1 + Pgz (6.18) In modelling the flow of SCC mixes, in order to reduce the computational cost, the twodimensional (2D) and axi symmetric configurations are used here which are reduced versions of 3D and cylindrical coordinates, respectively. The discretisation of the governing equations is given below D discretisation of mass and momentum conservation equations To derive the governing equations, the z components o f (6.8), (6.9), (6.10) and (6.14) is set equal to zero. Therefore (6.6), (6.8), (6.9) and (6.14) become (6.19), (6.20), (6.21) and (6.22), respectively. dv, dvx dx dy = 0 (6.19) dv, dv. dv. _ J L + Vr  + V  V dt dx dy dp =  & + ^ f r\2 \ d v, d v. + dx1 dy^ (6.20) dv. dv dv. y +v_ ^ + v dt dx y dy dp =  % + P 8 > + T1* dx1 dy1 J (6.21) r ~dvx dvx ~ dvx dvy ~ \ 1 dx dy dx dx + 2 dvy dvy dvx dvy (6.22) dx dy dy dy y Axisymmetric discretisation of mass and momentum conservation equations A flow is axisymmetric, if the displacement takes place along the r and z axes but is independent of the ^ direction. Therefore any derivative with respect to <f>in the cylindrical coordinates vanishes. Furthermore in this case due to the irotational nature of the flow the P agel47
172 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres velocity in <f> direction (v#) is also set equal to zero. Therefore (6.15), (6.16) and (6.18) become (6.23), (6.24) and (6.25), respectively. 1 d, x dv, (rv ) +  = 0 r d r K r} dz (6.23) r component: p dp dr dv. dv,  + v + v dt r dr + Jl*r ld _ r dr dvr_ dz dv'r_ dr + d \ dz2 + Pg (6.24) z component: p dv. dvz_ + v. +v. dv^ \ dt r dr dz dp dr J_ d_ r dr dvl dr (6.25) + + P g dz2 r]eff is obtained from (6.11) after replacing xrand^ by ran d z, respectively. 6.3 Numerical solution procedure To track the Lagrangian nonnewtonian flow, a fully incompressible method is used. However, equation (6.2) is for a general compressible flow. As shown in Chapter 3, the strict enforcement of incompressibility results in a Poisson s equation for pressure correction. In order to use this pressurepoisson equation, a projection formulation introduced by Chorin (1968) and Cummins and Rudman (1999) is implemented. In this way the pressure and velocity fields are updated until they reach a divergence free state. This predictorcorrector time stepping scheme is described below Prediction step The first, prediction step is an explicit integration in time without enforcing incompressibility. Only the viscous stress and gravity terms in equation (6.3) are considered and an intermediate velocity and position are obtained by integration n+1 = V + f g + 1 VT 'I At (6.26) P J Pagel48
173 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres where v;+1= v n + Av;+1 (6.27) C l = * + v;+]a/ (6.28) Here, vmand x are the particle velocity and position vectors at time t, v*+1 and x*+1 are the intermediate particle velocity and position vectors, and Av*+1 is the change in the particle velocity vector during the time increment A / C orrection step A corrective step is next applied to enforce the incompressibility condition prior to incrementing the time. The correction step is performed by considering the pressure term in (6.3) A t V C (6.29) where v ^j is the corrected particle velocity vector at the time level n+1. As the particle density remains constant during the flow, the mass conservation (6.2) imposes the following incompressibility condition on the corrected velocity V *vn+1 = 0 (6.30) Taking the divergence o f (6.29) and noting the above incompressibility condition gives r 1 1 V v! V VP p A/ V I n+1 n+1 (6.31) which can be rewritten as y2 p «.i = T7V'vVi (632) At Once the pressure is obtained from the Poisson equation (6.32), the particle velocity is updated by the computed pressure gradient (see equation (6.29)): Pagel49
174 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres n+1 v n+1 VP y l n+l yp A/ (6.33) J Finally, the instantaneous particle position can be updated using the corrected velocity (6.34) 6.4 SPH discretisation of the governing equations There are three terms in the mass and momentum conservation equations that need to be defined in the SPH formulation, namely the divergence of velocity in the mass conservation (6.2), the gradients of pressure and viscosity terms in the momentum conservation (6.3), and the Laplacian term V2Pn+1 resulting from the enforcement of incompressibility. In following, these terms will be discretised in the SPH sense Gradient of pressure The gradient of pressure in the NavierStokes equations can be obtained by identifying ^ (x ) in (3.51) (see Chapter 3) with the pressure term P to give fe=i where a and b are the reference particle and its neighbour, respectively gradient of the corrected kernel (see Chapter 3 and Appendix A). (6.35) VW is the corrected Divergence of velocity Similarly, the divergence o f the velocity field can be calculated from 6=1 (6.36) Laplacian The Laplacian in the pressure Poisson equation (6.32) can be formulated using the divergence and gradient operators o f the SPH formulation to give P agel50
175 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres f o r.v P, Vfp, (x) = VWb (x) (6.37) 6=1 A l 6= Viscosity The viscosity term, V t in the momentum conservation equation can be written in a P similar manner to (6.36) as f \ '  V T \ P J J* fyl ~ = 2  tt»vw*w («*> 6=1 Pb where the shear stress is given by (6.1). 6.5 Time step The time step At is chosen based on the relevant stability conditions for the given problem. In the case of a Binghamtype SCC fluid flow, the time step is primarily controlled by the plastic viscosity. The time step size is generally decided by (Shao and Lo, 2003) gfo a 2r0 p y At = min VVmJ *y+ W j (6.39) where r0 is the initial particle spacing, is the maximum particle velocity, and a x and a 2 are coefficients usually in the order o f 0.1. These coefficients depend on the choice of SPH kernel functions and the nature of the engineering application. Note that the term was excluded from (6.39) because its value is close to one when m is a very large number. 6.6 Numerical simulation results In this Section, a number of numerical tests are presented to investigate the flowability and filling behaviour of the SCC mixes with and without fibres. In the case of flow of the SCC with fibres, the numerical results are compared with laboratory slump flow tests. P agel51
176 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres The SCC mixes studied are the selfcompacting high and ultrahigh performance concretes with and without fibres developed in Chapter 4 (see Tables 4.5 and 4.11). From the micromechanical model developed in Chapter 5, the plastic viscosities of the SCC mixes with and without fibres were calculated from the known plastic viscosity of the cement paste and the volume fractions o f the various fine aggregates and fibre (see Table 5.8). As mentioned previously, the yield stress o f SCC is low and practically constant over a wide range of plastic viscosities (see Figure 5.9). For the present mixes ry was chosen to be 200 Pa. The numerical simulations o f SCC flow in two different geometrical configurations are carried out. Firstly, a slump flow test is carried out on SCC mixes with and without fibres. The key difference in the model parameters between SCC mixes with and without fibres is the plastic viscosity, which, as we have seen, increases significantly in the presence of needlelike short steel fibres. However, as the volume fraction o f the fibres in the SCC mixes is usually small (0.5% and 2.5% in the present simulations) the density is only marginally increased with the addition o f fibres. The slump flow test is first simulated in an axisymmetric configuration, followed by a simulation in a 2D approximation along a vertical plane of symmetry. Finally, the flow of SCC with and without fibres is simulated in an Lbox configuration Slum p flow test Initial configuration and boundary conditions Figure 6.1 illustrates the initial configuration o f the slump cone for which numerical simulations of the flow of SCC mixes with and without fibres was carried out in both the axisymmetric and twodimensional configurations. Pagel52
177 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 0.3m 0.2m z z=0.3m AA Figure 6.1: Initial configuration of the Slump Test in the twodimensional (Top) and axisymmetric configurations (Bottom). The governing equations have to be supplemented by proper boundary conditions. On a freesurface, a zero pressure condition (i.e. atmospheric pressure) has to be met. At a wall and on the bottom plate a Dirichlet (or firsttype) boundary condition has to be imposed on the normal component of the velocity field, while Neumann (or secondtype) conditions have to be imposed on pressure. In the SPH method, the implementation o f boundary conditions is not as straightforward as in the traditional meshbased methods. A number of techniques have been developed in the past to treat the boundary conditions in SPH applications (Monaghan, Pagel53
178 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 1994; Bonet and Kulasegaram, 2000; Bonet and Lok, 1999; Cummins and Rudman, 1999; Kulasegaram et al., 2004; Koshizuka et al., 1998). In this research, a technique based on an array of dummy rigid particles is used to implement the wall boundary conditions (Koshizuka et al., 1998). The wall boundaries are initially spaced according to the initial configuration o f the problem. The dummy particles are then placed outside the wall particles. The thickness of the array containing the dummy particles depends on the kernel smoothing length h. If the smoothing length is h = 2ro, where r0 is the initial particle spacing as defined earlier, four lines o f dummy particles at a spacing o f rq between the lines is used (see Figure 6.2). The normal component of the velocities of both the wall and dummy particles is set to zero to represent a noslip boundary condition. This technique has been chosen because it is more suitable for solving the pressure Poisson equation (6.32) subject to the wall boundary conditions. Furthermore, to perform realistic simulations, it is important to allow for friction between the SCC mixes and the contacting surfaces (i.e. walls and the bottom plate). A dynamic coefficient of friction equal to 0.56 Ns/m was found appropriate (see below). Note that the unusual dimensions of this coefficient are consistent with the formulation o f the problem (see Figure 6.2). The Dirichlet and Neumann boundary conditions along the axis of symmetry and the bottom plate are shown in Figure 6.2. The boundary conditions along the slump cone wall are same as those along the bottom plate. However, as the slump cone is lifted thus exposing the mix, the boundary condition P = 0 (atmospheric pressure) is imposed on the newly formed free surfaces. The friction boundary condition is imposed on the bottom plate and on the slump cone wall when it is still in contact with the mix. The effect of friction boundary condition depends on the relative tangential velocity between the wall and the fluid flow and ensures that slip with friction boundary condition is enforced along the tangential direction of the wall. Page154
179 C h a p t e r 6 : M o d e l l i n g t h e F l o w o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s Dummy boundary particles Material particles P = 0 vm=0, dp =0 dn = 0 V =, 8P = 0 dn P=0] d P = o. P = 0 dp dn = 0, v n = 0 and Ft = c j v t dp dn = 0,vn =0 and Ft ~ cf Figure 6.2: Boundary conditions for the slum p cone (P pressure, vn  normal velocity,  tangential velocity and Cy  dynam ic coefficient of friction) Numerical test results For the numerical simulation o f the slump flow test approximately 2000 SPH particles were used to model one half o f the cone configuration shown in Figure 6.2. Figures 6.3 and 6.4 show the various stages during the numerical simulation of slump flow test o f SCUHPC mixes without fibres and w ith fibres, respectively. It is evident from these Pagel55
180 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres results that the fluidity o f the flow without fibres is much higher than that of SCC with fibres. It can also be noted in both cases that the initial profiles o f the free surfaces are influenced by the motion of the steel cone during its quick removal. For the purposes of comparison, the SCC mix with fibres was simulated using both the axisymmetric (Figures 6.4) and 2D (Figure 6.6) configurations. It can be noted from the figures that 2D flow approximation is slower than the real axisymmetric flow. Figure 6.5 shows the slump flow circles at different heights (z) along the axis o f symmetry in the axisym metric configuration. t= l sec t=2 sec Figure 6.3: Axisymmetric numerical simulation of slump flow test for SCUHPC without fibres Pagel56
181 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres «i a u *1* * 1 w I B U I S U 1.35 «4 ) 425 * 2 *15 I MS HI MS U 1 0 I ) MS t=0.5 sec t=1.5 sec 4 ) W 4 1 «4 1 «( MS 1.1 U S U MS U U S 4» 4 ) J 4 K I S U 11! U U S I I U t=2 sec t=3 sec Figure 6.4: Axisymmetric numerical simulation of slump flow test for SCUHPC with fibres»z=151.0mm ~ z=57 8 mra z=45.8mm z?=0.0 mm z=103.0inm z=78.1mm z=50.0 mm z=0.0mm t=0.5 sec t=1.5 sec Pagel57
182 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 2=97.1 mm =63.8 mm =0.0 mm =86.5 mm t=2.0 sec t=3.0 sec Figure 6.5: Plan view of axisymmetric numerical simulation of slump flow test for SCUHPC with fibres at four different heights (z) along the axis of symmetry. z=0 is at the base of the cone. «4 3 4 J5 A B 4 1 «t U S I I 11! I! U ) U AH IB 4 J J 4 ) «S I M i 11 11! 12 U S U AH t=0.5 sec t= l.5 sec IS 4 1 M S U U 4 IS 4 1 U S 4 ] U S 4 S S 4 ) 4 K K I U S 4 1 I.1S 4 2 I2 S U I J S t=2 sec t=3 sec Figure 6.6: Numerical simulation of slump flow test for SCUHPC with fibres in 2D approximation Pagel58
183 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Slump flow tests on the SCHPC and SCUHPC with and without steel fibres have been carried out in the laboratory (see Tables 4.5 and 4.11). It was decided to use only axisymmetric numerical simulations to model the slump flow test in the remaining mixes. In Table 6.1, the measured T are compared with the numerical simulations for both SCHPFRC and SCUHPFRC mixes. In fact, the only free parameter in the simulations, namely the dynamic coefficient o f friction, was adjusted until the simulated T of SCUHPFRC was very nearly the same as the measured value (Table 6.1). This adjustment suggested the dynamic coefficient o f friction o f 0.56 Ns/m between the mixes and the steel bottom plate and steel of the cone. It should be emphasized that this dynamic coefficient of friction will remain unchanged in all subsequent simulations. Table 6.1: Measured and simulated T50o for SCC mixes SCC type Volume fraction of steel fibres (%) M easured Tsoo (sec) Sim ulated Tsoo (sec) E rror (% ) SCHPFRC SCUHPFRC Fibre positions and orientations For the purpose of investigating how the fibres will reorient themselves during the flow, a slump flow simulation was performed by distributing the fibres randomly as concentrated masses and by following their velocity vectors. The number of steel fibres that will theoretically be seen in the cut section o f a particular volume is given by the theory of geometric probability or more precisely by the solution o f the socalled Buffon problem (more details can be found in Appendix C). This theory was used to calculate the number of steel fibres of the SCUHPFRC mix with 2.5% volume fraction in the vertical diametrical section o f the slump cone. The number o f steel fibres would be 3347 or half that number if symmetry is accounted for. However, as the aim here was much more modest, namely to get a qualitative idea of how the fibre particles reoriented themselves during the flow as judged by their velocity vectors, only 112 fibre particles were treated as lumped masses and randomly distributed in one half o f the diametrical section (Figure 6.2) using a random number generator. Pagel59
184 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres The random distribution o f this limited number o f lumped masses representing the fibre particles and their associated velocity vectors at various times during the flow are shown in Figure 6.6. J S L1C L IS L2A L2S LJ9 US t=0.1 sec t=0.5 sec L ia U S Page160
185 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres U 5 MS t= l. 5 sec t=3 sec Figure 6.7: Fibre distributions (dark spots) and their velocity fields (arrows) at various times during the flow of SCUHPFRC As expected the fibres reorient with the flow. The mobility (i.e. velocity) of the fibres in the bulk and of those closer to the base plate decreases more rapidly than those of the fibres closer to the free surfaces Lbox test In order to further analyse the flow characteristics o f SCC, the casting o f an Lbox is explored in this numerical test. The aim is to record how long the SCC will take to level off in the horizontal part of the L after the shutter holding back the flow has been instantaneously released Initial configuration and boundary conditions Figure 6.7 illustrates the initial geometry o f the test; the Dirichlet and Neumann boundary conditions imposed on the flow are shown in Figure 6.8. In addition to the boundary conditions illustrated in Figure 6.8, friction boundary conditions are also imposed on the walls and the base o f the Lbox, as in the slump flow test above. In the numerical simulation of Lbox casting approximately 2500 SPH particles were used to model the material shown shaded in Figure 6.7. Pagel61
186 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 0.6m 0.15m» 4 tl 0.18m o.52m Figure 6.8: Initial configuration of the Lbox concrete casting P = 0 dp = 0, v = 0,Ft = c jv t dp = 0, dn V = 0 dp = 0, v_ = 0, Ft = c fv t Figure 6.9: Boundary conditions (P  pressure, vn  normal velocity, vt tangential velocity and Cy  dynamic coefficient of friction). Pagel62
187 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Numerical test results Figures 6.9 and 6.10 illustrate the various stages during the numerical simulation of the flow of SCUHPC mixes without and with fibres in an Lbox, respectively. It can be observed from the simulations that in this numerical test the flows of both mixes with and without fibres are faster than their counterparts in the slump test, as expected due to the higher initial potential energy of the material in the Lbox simulation. Due to the rapid nature of the flow, more undulations can be observed on the free surface o f both flows. Also as expected, it is evident from the results that the flow o f SCC without fibres has higher fluidity. u u t=0.8 sec t= l.l sec Figure 6.10: Numerical simulation of Lbox casting for SCUHPC mix without fibres Pagel63 f
188 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres t=24.1 sec t= 48.2sec Figure 6.11: Numerical simulation of Lbox casting for SCUHPFRC mix Table 6.2 shows the simulated T 2 0 0, T (the time taken to reach the distance of 200 mm and 400 mm from the gate, respectively) and leveloff time for all mixes o f Chapter 4. Pagel64
189 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Table 6.2 : Simulated T20o, T400 and leveloff time for SCC mixes SCC type Volume fraction of Leveloff T2 0 0 steel fibres (%) (sec) T4 0 0 (sec) tim e (sec) SCHPC SCHPFRC SCUHPC SCUHPFRC S im u latio n tim e Slump flow tim e The simulations of slump flow until the flow stops require several hours on a 1.86 GHz Intel Core 2 CPU 6320 Pentium PC having 1.98 GB o f core memory. The typical run time for 2000 SPH particles for 0.1 second slump flow takes approximately 67 minutes. The simulation time is likely to increase significantly when the number o f particles used to represent the mix is increased. To investigate this, 4000 and 7000 SPH particles were used to model the full slump cone o f SCUHPC in 2D approximation. The typical run times for each 0.1 second flow time increment was approximately minutes and minutes for 7000 and 4000 particles, respectively. Figure 6.11 shows the flow o f SCUHPC at three times during the very early stages. As can be observed the flows are identical except that in the case of 7000 SPH particles, the surfaces of the flow are show less undulations than with 4000 SPH particles. Page165
190 C h a p t e r 6 : M o d e l l i n g t h e F l o w o f S e l f  C o m p a c t i n g H i g h a n d U l t r a H i g h P e r f o r m a n c e C o n c r e t e s W i t h a n d W i t h o u t S t e e l F i b r e s *.»  U a * 1 M S BJ< 1.1 I I S I.! 1 8 U U S M S 1 J.* (.IS U S I I I I S 1! U S ( t=0.1 sec t=0.3 sec Figure 6.12: Numerical simulation of slump flow test for SCUHPC in 2D approximation using Lbox tim e 4000 (left) and 7000 (right) particles The simulations o f the Lbox until the flow levels off require several hours on a 1.86 GHz Intel* Core1M2 CPU 6320 Pentium PC having 1.98 GB of memory. The typical run time for 0.1 second flow takes approximately 78 minutes. Pagel66
191 Chapter 6: Modelling the Flow of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 6.8 Concluding remarks The SPH is a meshless Lagrangian approach that offers considerable potential as a numerical method for modelling problems involving large deformations. A corrected incompressible SPH method was implemented to simulate the flow of SCC mixes with and without fibres. The mix characteristics of the SCC mixes have been fully incorporated implicitly through the flow viscosity which has been calculated using the micromechanical model described in Chapter 5. This enables one to model the flow accurately with SPH method. A suitable Bingham rheological model has been coupled with Lagrangian NavierStokes equations to study the flow behaviour o f SCC mixes. The proposed method can be effectively applied in the numerical simulation of SCC flow to analyse the filling behaviour o f such a highly viscous fluid. The capabilities of this methodology have been validated and demonstrated by comparing the simulation results with the slump flow test carried out in the laboratory. The numerical results were in excellent agreement with test results and confirmed that the SPH methodology is capable of predicting accurately SCC flow with and without fibres. Although the SCC flow simulations were investigated for simple geometrical formwork shapes, the proposed methodology and accompanying numerical tools can be applied for analysing the flow o f SCC with or without fibres in complex formworks. An attempt was also made to study how the fibres change their positions and orientations during the flow. For this the fibres were treated as concentrated masses randomly distributed in the mix. This gave a general idea o f the change in their centres of mass during the flow but not about their actual orientations. In the next Chapter it will be shown how the above simulation techniques are also useful for proportioning the SCC mixes at the design stage. The typical run time for 2000 SPH particles for 0.1 second slump flow takes approximately 67 minutes, whereas for 2500 SPH particles for 0.1 second Lbox flow takes approximately 78 minutes. A comparative study was carried out on simulation times and 4000 SPH particles were used to simulate the full slump cone. It was observed that the run time was considerably increased (by at least 3 times) when the number of SPH particles was increased from 4000 to Pagel67
192 Chapter 7 Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres
193 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 7.1 Introduction In the previous Chapter the numerical techniques were used to simulate the flow o f predesigned SCC with or without fibres in moulds at the application stage. The same techniques are also useful for proportioning the SCC mixes at the design stage. They provide an alternative tool for the mix design o f SCC, thus avoiding expensive and timeconsuming tests in laboratories or on site. The design tools are often more useful than the experimental methods in providing insightful and complete information through an extensive parametric study that cannot be easily performed by other means. In this Chapter, the simulations of SCC mixes are used as an aid in the mix design stage of such concretes. Selfcompacting high and ultrahigh performance concrete (SCHPC/SCUHPC) mixes with and without steel fibres (SCHPFRC/SCUHPFRC) will be designed to cover a wide range o f plastic viscosity. All these mixes will meet the flow and passing ability criteria, thus ensuring that they will flow properly into the moulds. The various steps in the design o f SCC mixes with or without steel fibres are as follows. Firstly, the slump flow test is carried out with the aid of the numerical simulation technique described in Chapter 6 on a series o f SCC mixes having different plastic viscosities and volume fractions o f steel fibre. The T500 (the time from lifting of the cone to the concrete spreading to a 500 mm diameter) for each mix is obtained with a view to investigating whether or not a correlation exists between T500 and the plastic viscosity. Secondly, in order to further analyse the flow of SCC in a mould, the flow of the same mixes is studied in an Lbox configuration, and the T200, T400 (the time taken by the mix to reach a distance o f 200 mm (T2oo) or 400 mm (T4 0 0) from the gate) and level off time are obtained, again with a view to ascertaining whether or not a correlation exists between these flow times and the mix plastic viscosity. It should be emphasized that at this stage in the mix design process the actual mix proportions are still unknown, apart from the volume fraction o f fibres and the plastic viscosity o f the mix. Finally, guidance is given for proportioning the mixes such that they will attain the given plastic viscosity and the T500, T2oo, T4 0 0, and the leveloff times. Page169
194 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 7.2 Types of SCC mixes As mentioned in Chapter 2, three different types of SCC can be distinguished depending on the method of ensuring the required plastic viscosity. These are the powdertype, the VMA type and the combined type. In this thesis two main mixes of the powder type were examined, i.e. SCHPFRC and SCUHPFRC (Chapter 4). These mixes are characterized by high powder content and a low water to powder ratio. Their selfcompacting ability was achieved by adjusting the water to binder ratio and the superplasticiser dosage. However, in view o f the high powder content, the powdertype SCC mixes are sensitive to changes in the constituent materials. This must be borne in mind during the proportioning of the mixes. Okamura and Ozawa (1995) have proposed a heuristic mix proportioning method for this type of SCC (see, Chapter 2, Figure 2.6). According to their method, the coarse and fine aggregate contents are fixed and the selfcompacting ability is obtained by adjusting the water to powder ratio and the amount o f superplasticiser. However, as the SCC base mixes used here differ in terms o f their fine constituents, type o f superplasticiser and mixing procedures (see Chapter 4 and Tables (4.5) and (4.11)), the heuristic mix design method is not very appropriate. Instead, the threestep mix design method outlined above based on the actual simulation of the mixes were used. 7.3 Slump flow test Slump flow simulations were carried out on a series o f selfcompacting high and ultrahigh performance concretes with (SCHPFRC/SCUHPFRC) and without fibres (SCHPC/SCUHPC). The volume fractions o f steel fibres were only varied out in the mixes: 0.5% and 1% in SCHPFRC mixes, and 1.5%, 2%, 2.5% and 3% in SCUHPFRC mixes. The target plastic viscosity o f SCHPC mixes was chosen in the range from 4 Pas to 12 Pas, whilst that of SCUHPC mixes was from 2 Pas to 6 Pas. The lower plastic viscosity of the latter mixes is due to the absence o f coarse aggregates in them. The target plastic viscosities of corresponding mixes with fibres were obtained using Equation (5.40). Table 7.1 gives the slump flow times (Tsoo) o f this series o f mixes obtained using the simulation technique described in Chapter 6. Pagel70
195 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres According to the latest mix design rules for selfcompacting concretes (BS EN 2069, 2010) the maximum aggregate size is limited to 40 mm and two viscosity classes are introduced: viscosity class 1 (V S1) and viscosity class 2 (VS2) depending on whether T 500 < 2 sec or T 5^ > 2 sec. The mixes considered below all belong to viscosity class 2. Table 7.1: Slump flow time (T500) for SCHPFRC and SCUHPFRC mixes with different volume fractions of steel fibre and target plastic viscosities SCC type SCHPFRC SCUHPFRC Volume fraction of fibres (%) Plastic viscosity of m ix w ithout fibres (Pas) Plastic viscosity of mix with fibres (Pas) T500 (s) Pagel71
196 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Figure 7.1 shows that the T and the plastic viscosity o f the above mixes are reasonably well correlated. 5 4 C / 3 o e in H Plastic viscosity of mix w ith fibres (Pas) Figure 7.1: Simulated TSOoVS. plastic viscosity of different mixes with steel fibres Figures 7.2 and 7.3 show fanshaped relationships between the plastic viscosity o f SCHPFRC and SCUHPFRC mixes and the steel fibre volume fraction as the plastic viscosity of the base mixes without fibres increases. <W X a 100 g u, fta u(/) ft. CA JC o g O U«A '> C <*> Volume fraction of fibres (<p%) T]nf 4 Pas T]nf= 6 Pas TInf8 Pas T]nf= 10 Pas T nf=12 Pas Figure 7.2: Fanshaped correlation between plastic viscosities of SCHPFRC and steel fibre volume fractions (%ff is the plastic viscosity of SCHPC mix without fibres) Page172
197 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres <U X a u cc Ll. CL, X» V </) o 100 T nf= 2 Pas T1nf= 3 Pas R 1?= Pas T nf~ 5 Pas T]nf 6 Pas o Volume fraction of fibres (<p%) Figure 7.3: Fanshaped correlation between plastic viscosities of SCUHPFRC and steel fibre volume fractions (unf is the plastic viscosity of SCUHPC mix without fibres) 7.4 Lbox test Next, the flow simulations o f the above mixes in the Lbox were carried out. Table 7.2 gives the simulated T2 0 0, T4 0 0 (the time taken to reach the distance of 200 mm and 400 mm from the gate, respectively) and the leveloff tim e for the SCHPFRC and SCUHPFRC mixes o f Table 7.1. Page173
198 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Table 7.2: Lbox simulations of SCHPFRC and SCUHPFRC mixes giving T2oo, T400 and the leveloff times SCC type SCHPFRC SCUHPFRC Volume fraction of fibres (% ) Plastic viscosity of mix w ithout fibres (Pas) Plastic viscosity of m ix with fib res (Pas) T2 0 0 (s) T ( s ) Leveloff tim e (s) Figure 7.4 depicts the trend between T 2 0 0, T40o, and the leveloff times and the different plastic viscosity o f the above mixes. Pagel74
199 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres The data in Figure 7.4 shows that the various times correlate well with the plastic viscosity of the mixes in the entire range o f volume fractions o f steel fibres ( %) studied. sn H Plastic viscosity of mixes with fibre (Pas) < )=0.5% C{)=1% A< >=1.5% X<p=2% X<p=2.5% cp=3% y=0.1023xft9724 * R2 = Plastic viscosity of mixes with fibre (Pas) cp=0.5% cp=l% A( >=1.5% Xcp=2% Xq>=2.5% ((>=3% tj fc? > cp=0.5% < >=T% A<p=1.5% Xcp=2% Xcp=2.5% ((>=3% Plastic viscosity of mixes with fibre (Pas) Figure 7. 4 : T 2oo> T and the leveloff times vs the plastic viscosity of mixes for various fibre volume fractions Page175
200 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 7.5 Mix proportioning The final step in the mix design process is to choose the mix proportions that will meet the flowability (slump flow test) and passingability (Lbox test) requirements. The following algorithm is used to calculate the mix proportions: 1. Assume the amount of cement and use the initial water and superplasticiser contents the same as in Tables (4.5) and (4.11) for the SCHPFRC and SCUHPFRC mixes, respectively; 2. Estimate the volume fraction o f solid particles (see below, Section 7.5.1); 3. Calculate the amount o f the finest solid particles suspended in the previous liquid suspension (in the first step it is the cement paste) according to its volume fraction; 4. Repeat step 3 until all the solid contents in the mix have been calculated; 5. Adjust the water content such that the water to binder ratio is 0.24 and 0.18 for the SCHPFRC and SCUHPFRC mixes, respectively; 6. Adjust the superplasticiser content such that the SP to water ratio is 0.14 and 0.28 for the SCHPFRC and SCUHPFRC mixes, respectively; 7. Estimate the plastic viscosity o f the new cement paste; 8. Calculate the plastic viscosity o f the new mix, based on the twophase liquidsolid suspensions shown in Figure 5.1; 9. Compare the plastic viscosity with the one used in the simulation. If the error is more than 5% repeat steps 3 to 8 ; 1 0. Estimate T500, T200, T400 and the leveloff time from their correlations with the plastic viscosity (Figures 7.1 and 7.4). It is clear that there are infinitely many mix proportion combinations that will give the same result. The choice o f mix proportions suggested here was guided by the experience gained in this research, i.e. Table (4.5) for SCHPFRC and Table (4.11) for SCUHPFRC mixes Method of estimating the volume fractions of solid particles The plastic viscosity o f the SCC mixes without fibres is calculated from (5.41) i.e. Pagel76
201 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres where /, ) can be replaced by its equivalent, relative plastic viscosity, i.e. plastic viscosity of SCC mix without fibre (v Nf ) divided by the plastic viscosity of paste ( r j ^ ). Therefore (5.41) can be rewritten as (7.1) where n: is total number of solid phases in the mix, such as coarse aggregate, sand, and cement additives; rjpast* ' ls *he plastic viscosity o f the cement paste; rjfjp: is the plastic viscosity o f SCC mix without fibres. As stated in Chapter 5, the Krieger and Dougherty equation (5.11) is the most suitable for cement pastes. Therefore (5.11) will be used here to obtain / ( $ ) The value of [7 ] = 2.5 and <f>m= 0.63 are used, as before. For a given r}m and rjpastt, equation (7.1) can be rewritten as ( )( < ig ( )...( <* )=«(7.2) where u is a constant number. The value o f $ is given by <ft = 0.63Zjc (7.3) where x = yfu and / is a factor such that /j X /2 x...xtn =1 (7.4) An example of mix proportioning is given at the end of this Chapter Typical SCHPFRC mix proportions Tables (7.3) and (7.4) give typical SCHPFRC mix proportions calculated in accordance with the procedure described above. In these tables, 4>f, t]nf (error%) and tjwf represent the volume fraction of fibre, the error in the plastic viscosity o f the base SCHPC mix without fibres (compared with the one used in simulations) and the plastic viscosity of SCHPFRC mix with fibres, respectively. P ag el77
202 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Table 7.3: Typical mix proportions of SCHPFRC mixes with ^= 0.5 % Cement m E Microsilica n at) X Limestone Sand < 2 mm ) Coarse aggregates < 10 mm s V) Water O u Superplasticiser Fibres KdUOS Water/binder SP/water TiPaste (Pas) Plastic r NF (Pas) viscosity tinf (error%) rjwf (Pas) Slump T500 (Slump flow test) (sec) T200 (Lbox test) (sec) Lbox T40o (Lbox test) (sec) Leveloff time (Lbox test) (sec) Table 7.4: Typical mix proportions of SCHPFRC mixes with <f>f= 1% Cement PO g Microsilica Limestone X a Sand < 2 mm c 1 Coarse aggregates < 1 0 mm (A Water u Superplasticiser Fibres Ratios Water/binder SP/water TJpaste (Pas) Plastic %tf (Pas) viscosity tjnf (error%) tiwf (Pas) Slump T500 (Slump flow test) (sec) T20o (Lbox test) (sec) Lbox T400 (Lbox test) (sec) Leveloff time (Lbox test) (sec) Page178
203 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Typical SCUHPFRC mix proportions Tables (7.5), (7.6), (7.7) and (7.8) give typical SCUHPFRC mix proportions calculated in accordance with the procedure described above. Table 7.5: Typical mix proportions of SCUHPFRC mixes with ^= 1.5 % Cement Microsilica S on Ground granulated blast furnace slag (GGBS) Quartz Sand pm a c 0) pm T3 Water u O Superplasticiser Fibres Ratios Water/binder SP/water r( Paste (PaS) P lastic Hnf (Pas) viscosity r NT (erroi%) tiwf (Pas) Slum p T50o (Slump flow test) (sec) T20o(Lbox test) (sec) Lbox T400 (Lbox test) (sec) LevelofT time (Lbox test) (sec) Page179
204 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Table 7.6: Typical mix proportions of SCUHPFRC mixes with <f>f = 2% Cement n S Microsilica Ground granulated blast furnace slag (GGBS) S t Quartz Sand pm a c gm V Water g u O Superplasticiser Fibres Ratios Water/binder SP/water T]Paste (PaS) Plastic T]NF(Pas) viscosity tjnf (erroi%) t]wf (Pas) Slump T500 (Slump flow test) (sec) T200 (Lbox test) (sec) Lbox T400 (Lbox test) (sec) Leveloff time (Lbox test) (sec) Table 7.7: Typical mix proportions of SCUHPFRC mixes with ^= 2.5 % Cement cn s Microsilica Ground granulated blast furnace slag (GGBS) Quartz Sand pm c pm « B Water G 0 u Superplasticiser Fibres Ratios Water/binder SP/water T lp a s te (Pas) Plastic Hn f (Pas) viscosity (erroi%) t]wf (Pas) Slump T500 (Slump flow test) (sec) T 20o (Lbox test) (sec) Lbox T 40o (Lbox test) (sec) Leveloff time (Lbox test) (sec) Pagel80
205 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Table 7.8: Typical mix proportions of SCUHPFRC mixes with ^ = 3 % Cement PO Microsilica ' Ground granulated blast furnace slag (GGBS) Quartz Sand pm a C pm g Water O u Ratios Superplasticiser Fibres Water/binder SP/water rjpaste (Pas) Plastic TjNF (Pas) viscosity tjnf (error%) tiwf (Pas) Slump T500 (Slump flow test) (sec) T 2oo (Lbox test) (sec) Lbox T400 (Lbox test) (sec) Leveloff time (Lbox test) (sec) As can be seen from Tables (73) to (78), in order to increase the plastic viscosity o f SCC mixes, the amount o f binder should be increased, whereas that o f liquids (water and superplasticiser) should be decreased. 7.6 Concluding rem arks Various SCC mixes with different plastic viscosity and steel fibres content were studied. These mixes were characterised as a pow dertype SCC. Slump flow and Lbox numerical simulations were performed on a series of mixes to test their flow ability and passing ability as measured by the T5oo (for slump flow test), T2oo, T4oo and leveloff time (for Lbox test). At this stage in the mix design process the actual mix proportions were still unknown, apart from the volume fraction o f fibres and the plastic viscosity of the mix. Pagel81
206 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Finally, guidance was given for proportioning the mixes such that they will attain the given plastic viscosity and the T5 0 0, T2 0 0, T4 0 0, and the leveloff times. This guidance followed a step by step algorithm. An example is given below to illustrate this algorithm. 7.7 An example of mix proportioning As an example o f the application o f the mix proportioning method described in Section 7.5, let us calculate the mix proportions o f a SCUHPFRC mix with <f>f =3%, assuming that the viscosity of the base SCUPHC mix without fibres is =4 Pas and that of the cement paste l S t?paste =030 Pas 1. The amount of cement (c) is assumed to be 520 kg/m3. The initial amount of water (w) and superplasticiser (sp) are the same as in Table (4.11) i.e. 188 kg/m3 and kg/m3, respectively. 2. In order to estimate the volume fractions o f microsilica <j>ms, GGBS </>g, fine quartz sand (9300 pm) (psx and coarse quartz sand ( pm )^2 we proceed as per the algorithm above. We first use Equation (7.1) as follows. nm,=riraaea 1 paste ((0.63)4) x0.63 f, ^2.5x0.63 ^ ^ ^2.5x0.63 f ^ ^2.5x ** K 0.63 j x 0.63 [(0630 ( )( ^,) ( ^ ) ] 1  fis2 \ 0.63 (7.5) Substituting r/^ =4 Pas and rjpaste =0.30 Pas into (7.5) yields «= ( ^ ) ( ) ( ^ ) ( 063A 2 ) = (7.6) Therefore x = ( /m = (7.7) Pagel82
207 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Using (7.3) i.e. ^ = t x with ti=34/33, t2=3 3 /3 4, t3=6 / 5 and ti=5/6 (note that tit2t3t4=l), (7.6) gives the following volume fractions o f solid phases 6 = ms <!>g = = ^ 2 = (7.8) There is an infinite choice in the selection o f t,s, as mentioned before. 3. The amount of finest solid particle i.e. microsilica (ms) suspended in cement paste is calculated according to its volume fraction ( ^ ) to give m s 4m. ms = f \ c w sp m s P c Pw Pspj (7.9) Using p c =2950 kg/m3, p w=1000 kg/m3, p v =1070 kg/m3 and p ^ = kg/m3 in (7.9) gives the amount of microsilica as ms= 227 kg/m3. 4. Step 3 is repeated until all the solid contents in the mix have been calculated i.e. GGBS (g), fine quartz sand (9300 pm )(sl) and coarse quartz sand ( pm) (s2 ). The amounts o f GGBS ( p g =2400 kg/m3) and of the quartz sands ( p sl = p s2 =2650 kg/m3) work out to be g =359 kg/m3, 57=261 kg/m3and 52=796 kg/m3. 5. The amount of water is adjusted such that waterbinder ratio is Therefore w= 195 kg/m3. 6. The amount of superplasticiser is adjusted such that SPwater ratio is Therefore sp=55 kg/m3. 7. The value o f plastic viscosity o f cement paste in relation to the original cement paste used in Table 4.11 is estimated to be 0.29 pas. 8. The plastic viscosities o f SCC mix with and without fibres are calculated according to procedures described in Chapter 5. This gives 77^ =8.9 Pas. Pagel83
208 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres 9. This value o f plastic viscosity is compared with the one used in the simulation (i.e. Tjm =4 Pas). This gives an error in r NF > 5% which is not acceptable. Therefore steps 3 to 8 have to be repeated with a lower trial amount of cement in order to reduce the plastic viscosity. 3 (repeat): try cement=450 kg/m3, giving ms=214 kg/m3. 4 (repeat): calculate corresponding g =339 kg/m3, 57=246 kg/m3 and 52=750 kg/m3. 5 (repeat): the amount of water is w=176 kg/m3. 6 (repeat): the amount o f superplasticiser is sp=49 kg/m3. 7 (repeat): viscosity o f cement paste is calculated as 0.30 Pas. 8 (repeat): the plastic viscosity o f new mix will be t1nf=4.32 Pas. 9 (repeat): the error in the plastic viscosity is 7.4% which is again not acceptable. Therefore steps 3 to 8 have to be repeated again with a new trial amount of cement. 3 (repeat): try cement=480 kg/m3, gives ms=220 kg/m3. 4 (repeat): repeat the previous step yields: g=348 kg/m3, sl=253 kg/m3 and s2=770 kg/m3. 5 (repeat): the amount o f water is w= 184 kg/m3. 6 (repeat): the amount o f superplasticiser is sp= 52 kg/m3. 7 (repeat): viscosity o f cement paste is calculated as 0.29 Pas. 8 (repeat): the plastic viscosity o f new mix will be tinf=4.01 Pas. 9 (repeat): the error in the plastic viscosity is 0.4% (<5%) which is acceptable. 10. T500, T200, T400 and leveloff times are estimated based on their correlation with plastic viscosity (see Figures (7.1) and (7.4)). Table 7.9 gives the SCUHPFRC constituents. Pagel84
209 Chapter 7: Guidelines for Mix Proportioning of SelfCompacting High and Ultra High Performance Concretes With and Without Steel Fibres Table 7.9: SCUHPFRC constituents Cement 480 m g Microsilica i f Ground granulated blast furnace slag (GGBS) 348 SmJ a Quartz Sand pm 253 G a pm :O V) r* Water 184 K9 o u Superplasticiser 52 Ratios Fibres 234 W ater/binder 0.18 SP/water 0.28 r Paste (Pas) 0.29 Plastic T]NF (Pas) 4.01 viscosity t)n f (error%) 0.4 tiwf (Pas) Slump T5 00 (Slump flow test) (sec) 3.7 T2 0 0 (Lbox test) (sec) 2.5 Lbox T4 0 0 (Lbox test) (sec) 7.6 Leveloff time (Lbox test) (sec) Rem arks on the choice o f tj As mentioned previously, for a given viscosity o f the paste, there are many (theoretically infinitely many) mix combinations that will lead to the desired viscosity of the SCUHPC. This is reflected in the choice o f tj. The best starting point is to choose ti=t2=t3=t4= l and to check the error in the resulting viscosity o f the mix. If this error is more than the acceptable limit (5%) then the new trial values o f tj need to be chosen such that tit2t3t4=l and the process of mix proportioning repeated until the error in the viscosity t n f is less than 5%. Pagel85
210 C hapter 8 Conclusions and Recommendations for Future Research
211 Chapter 8: Conclusions and R ecom m endations for Future Research 8.1 Conclusions The main conclusions on the basis o f the research work embodied in Chapters 4 to 7, inclusive, are summarised below: The development o f selfcompacting highperformance and ultra highperformance concrete mixes is a complex process requiring the resolution of conflicting demands of flowability and nonsegregation. Whilst these demands can be reconciled by increasing the paste content and decreasing the large aggregate volume, the resulting selfcompacting mixes may not reach the target compressive strength (Chapter 4). The easiest way to meet the strength requirement is to include steel fibres in the mix. This can however compromise the ability o f the mix to flow smoothly through gaps in the reinforcement and to cause segregation o f the fibres (Chapter 4). Selfcompacting high and ultra highperformance concrete mixes without fibres may be designed to satisfy only the flowability and cohesiveness criteria using the slump flow test. However, when long steel fibres are present in the mixes, it is additionally necessary to check that the mixes meet the passing ability criterion using the JRing apparatus (Chapter 4). The micromechanical procedure developed in Chapter 5 estimates the plastic viscosity of SCC mixes with or without steel fibres from the knowledge of the plastic viscosity of cement paste alone or o f the cement paste with SP and/or VMA. In this procedure, the SCC mix is regarded as a succession o f twophase suspensions solid and liquid phases (Chapter 5). It was noted that the influence of the discrete solid phase on the plastic viscosity of the continuous liquid phase depends only on the volume fraction of the solid phase $, if it is less than 10%. This influence was captured by the Einstein equation (or many of its later modifications) which contains the intrinsic viscosity [tj] (Chapter 5). However, when the volume fraction o f the solid phase exceeds 10% but is less than the maximum possible volume fraction f m9 then the relative viscosity depends not only on the volume fraction o f the discrete solid phase but also on how it is dispersed in the fluid and on the shape o f the solid particles. In this case the formula proposed by Krieger and Dougherty (1959) was used (Chapter 5). Page 187
212 Chapter 8: Conclusions and R ecom m endations for Future Research The fibres were regarded as rigid slender bodies in a viscous medium whose free translation and rotation are restrained by the viscous concrete mix (Chapter 5). The plastic viscosity, together with the yield stress of the SCC mixes with or without fibres, is needed to simulate the flow both at the mix design stage and at the industrial use stage to simulate the flow in the formwork. However the yield stress of SCC mix is practically unchanged over a large range o f plastic viscosity (Chapter 5). The SPH is a meshless Lagrangian approach that offers considerable potential as a numerical method for modelling problems involving large deformations. A corrected incompressible SPH method was implemented to simulate the flow o f SCC mixes with and without fibres (Chapter 6). A suitable Bingham rheological model was coupled with Lagrangian NavierStokes equations to study the flow behaviour o f SCC mixes (Chapter 6). The capabilities o f this methodology were validated by comparing the simulation results with the slump flow test carried out in the laboratory. The numerical results were in excellent agreement with test results and confirmed that the SPH methodology is capable o f predicting accurately SCC flow with and without fibres (Chapter 6). An attempt was also made to get a qualitative idea of how the fibres change their positions and orientations during the flow. For this a limited number o f fibres were treated as concentrated masses randomly distributed in the mix. This gave a general idea of the change in their centres of mass during the flow but not about their actual orientations (Chapter 6). Several powdertype high and ultra highperformance SCC mixes with different plastic viscosity and steel fibre content were proportioned using the SPH simulations as a mix design tool (Chapter 7). Guidance was given for proportioning the mixes such that they will attain the given plastic viscosity and the T5oo, T 2 0 0, T 4 0 0, and the leveloff times. This guidance was presented as a step by step algorithm for ease of use (Chapter 7). Page 188
213 Chapter 8: Conclusions and Recom m endations for Future Research 8.2 Recommendations for future research In most practical applications o f SCHPFRC/SCUHPFRC using 30mm long Dramix steel fibres, the volume fraction o f steel fibres is usually less than 3% for workability reasons. In this case the dilute concentration approximation of slender steel fibres made in Chapter 5 is adequate. The expressions derived in Chapter 5 are accurate for needleshaped steel fibres with aspect ratio up to 85 in dilute concentrations. The fibres were regarded as rigid slender bodies in a viscous medium whose free translation and rotation are restrained by the viscous concrete mix. However, for steel fibres in larger concentrations and/or larger aspect ratios, the interaction of steel fibres needs to be considered. In this case the assumptions that the fibres are rigid and that they are statistically homogeneously distributed in the mix need to be reexamined. The flow o f SCHPFRC/SCUHPFRC affects the orientation of the fibres. To exploit the foil potential o f SCHPFRC/SCUHPFRC, the orientations of the fibres need to be monitored during the flow. In this thesis, only a limited number o f fibres was treated as lumped masses and randomly distributed in the diametrical section using a random number generator. However, in order to find the actual orientations of the fibres during the flow, it is necessary to treat all the fibres in the mix not as lumped masses but as slender bodies. In this thesis, the Lbox was simulated in a 2D configuration. However, in order to understand folly the flow o f SCHPC/SCUHPC with or without fibres, a foil 3D simulation is required. The run time was considerably increased (by at least 3 times) when the number of SPH particles representing the SCC mix was increased from 4000 to The simulation algorithm should be modified in order to accelerate the run times, thus reducing the computational cost. This can be done by either rearranging the memory allocations for each argument or using parallel computations. Page 189
214 R eferences
215 References Aiad, I., Abd ElAleem, S. and ElDidamony, H., 2002, Effect of delaying addition of some concrete admixtures on the rheological properties of cement pastes, Cement and Concrete Research, Vol. 32, pp ASTM C l240 and EN 13263, Silica fumes for use in concrete, mortar and grout. Definitions, specifications and conformity criteria. Aydin, A.C., 2007, Self compact ability o f high volume hybrid fibre reinforced concrete, Construction and B uilding M aterials. Vol. 21, No. 6, p.p Bakker, P., Ramohalli Gopala, V., Lycklama a Nijeholt, J.A., Koenders, E., Grunewald, S. and Walraven, J., 2010, Simulation and testing o f the grout backfill process in a casestudy related to a nuclear waste disposal gallery in selfcompacting concrete (SCC). In: Proceedings o f the 2010 In tern a tion a l R ILE M Symposium on SelfC om pacting Concrete. Design, production and placement o f selfconsolidating concrete eds. Khayat KH. and Feys. D. Canada; pp Banfill, P.B.G., Beaupre, D., Chapdelaine, F., de Larrard, F., Domone, P.L., Nachbaur, L., Sedran, T., Wallevik, J.E. and Wallevik, O., 2001, In Ferraris, C.F. and Brower, L.E. (eds), Comparison o f concrete rheometers: In tern a tion a l tests a t LC PC (Nantes, France) in October NISTIR 6819, National institute o f standards and technology, Washington, USA, October. Barnes, H. A., Hutton, J. F. and Walters, K., 1993, A n introduction to rheology, Elsevier, pp Bartos, P.J.M., Marrs, D.L., 1999, Development and testing o f selfcompacting grout for the production o f SIFCON, Proceedings o f intern a tion a l w orkshop on high perform ance fib re reinforced cement com posites, eds H.W. Reinhardt and, A.E. Maaman, Germany, pp Batchelor, G.K., 1971, The stress generated in a nondilute suspension of elongated particles by pure straining motion, Jo u rn a l o f F lu id M echanics D igital A rchive, Vol. 46, pp Batchelor, G.K., 1977, The effect o f Brownian motion on the bulk stress in a suspension of spherical particles, Jo u rn a l o f F lu id M echanics D igita l A rchive, Vol. 83, pp Page 191
216 References Bennenk, I. H. W., 2005, Selfcompacting concrete  five years of experience with SCC in the netherlands, in P roceedings o f the 18th B IB M International Congress, Amsterdam, pp Benson, S.D.P. and Karihaloo B.L., 2005a, CARDIFRC Development and mechanical properties. Part I: Development and workability. M agazine o f Concrete Research, Vol. 57, No. 6, pp Benson, S.D.P. and Karihaloo, B.L., 2005b, CARDIFRC Development and mechanical properties. Part HI: Uniaxial tensile response and other mechanical properties, M agazine o f Concrete Research, Vol. 57, No. 8, pp Benson, S.D.P., Nicolaides, D and Karihaloo, B.L., 2005, CARDIFRC Development and mechanical properties. Part II: Fibre distribution. M agazine o f Concrete Research, Vol. 57, No. 7, pp Billberg, P., 1999, Selfcompacting concrete for civil engineering structuresthe Swedish experience, Report no 2:99, Sw edish C em ent a n d C oncrete R esearch In stitute, Stockholm, pp Billberg, P., Petersson, O., Westerholm, M., Wustholz, T. and Reinhardt, H., 2004, Summary report on work package 3.2: Test methods for passing ability, pp Bonen, D. and Sarkar, S.L., 1995, The superplasticiser adsorption capacity of cement pastes, pore solution composition, and parameters affecting flow loss. Cement a nd Concrete Research, Vol. 25, No.7, pp Bonet, J and Lok, T.S., 1999, Varational and momentum aspects of smooth particle hydrodynamics formulations, C om puter M ethods in A pplied M echanics and E ngineering, Vol. 180, pp Bonet, J. and Kulasegaram, S., 2000, Correction and stabilization of smooth particle hydrodynamic methods with application in metal forming simulations, International Journal o f Num erical M ethods in Engineering, Vol. 47, pp Page 192
217 References Bouzoubaa, N. and Lachemib, M., 2001, Self compacting concrete incorporating high volumes of class f fly ash: preliminary results, C ement and Concrete Research, Vol. 31, No. 3, pp Brite, E.R., 2000, Self compacting concrete, proposal No. BE , No. 10, pp Bui, V.K., Akkaya, Y. and Shah, S.P., 2002, Rheological model for selfconsolidating concrete, A C IM aterials Journal, Vol. 99, No. 6, pp Carlsward J, Emborg M, Utsi S, Oberg P., 2003, Effects of constituents on the workability and rheology of selfcompacting concrete. In: The 3 rd International RILEM Symposium on SelfC om pacting C oncrete, Wallevik OH, Nielsson I, editors, RILEM Publications S.A.R.L, Bagneux, France, pp Chhabra, R.P., Richardson, J.F., 2008, N onnew tonian flo w a n d applied rheology engineering applications, Elsevier second edition, pp Chindaprasirt, P., Hatanaka, S., Chareerat, T., Mishima, N. and Yuasa, Y., 2008, Cement paste characteristics and porous concrete properties, C onstruction and Building M aterials, Vol. 22, pp Chindaprasirt, P., Jaturapitakkul, C. and Sinsiri, T., 2005, Effect of fly ash fineness on compressive strength and pore size o f blended cement paste, Cement a nd Concrete Com posites, Vol. 27, No. 4, pp Chong, J. S., Christiansen, E. B. and Baer, A. D., 1971, Rheology of concentrated suspensions, Journal o f A pplied Polym er Science, Vol. 15, pp Chorin, A.J., 1968, Numeical solution o f the NavierStokes equations, M athematics o f Com putation, Vol. 22, pp Chu, H, Machida, A. and Suzuki, N., 1996, Experimental investigation and DEM simulation of filling capacity o f ffesh concrete, Transactions o f the Japan Concrete Institute, Vol. 16 pp Crofton, M. W., 1885, probability, E ncyclopedia B rittanica, 9th ed., Vol. 19, pp Page 193
218 References Cummins, S J. and Rudman, M., 1999, An SPH projection method, Journal o f C om putational P hysics, Vol. 152, No. 2, pp Cussigh, F., 1999, Selfcompacting concrete stability, P roceedings o f F irst RILEM International Symposium on S e lf C om pacting C oncrete, Stockholm, A. Skarendahl September. Cyr, M., Legrand, C. and Mouret, M., 2000, Study of the shear thickening effect of superplasticizers on the rheological behaviour o f cement pastes containing or not mineral additives, Cement a n d C oncrete R esearch, Vol. 30, pp David, B. and Shah, S. P., 2004, Concrete constructionfresh and hardened properties o f selfconsolidating concrete, P rogress in Structural E ngineering and M aterials, Vol. 7, pp de Castro, A.L. and Liborio, J.B.L., 2006, Initial rheological description o f high performance concretes, M aterials Research, Vol. 9, pp de Kruif, C.G., van Iersel, E.M.F., Vrij, A. and Russel, W.B., 1985, Hard sphere colloidal dispersions: Viscosity as a function o f shear rate and volume fraction, The Journal o f Chem ical Physics, AIP, pp de Larrard, F., Hu, C., Sedran, T., Szitkar, J.C., Joly, M., Claux, F. and Derkx, F., 1997, A new rheometer for softtofluid fresh concrete. A C I M aterials Journal, Vol. 94 No Dietz, J. and Ma, J., 2000, Preliminary examinations for the production of selfcompacting concrete using lignite fly ash, LACER No. 5, pp Domone, P. L., 2003, Fresh concrete, in A dvanced concrete technology, eds. J Newman, B S Choo, Elsevier, Vol. 2, Ch 1. Domone, P.L. and Thurairatnam, H., 1988, The effect of water/cement ratio, plasticizers and temperature on the rheology o f cement grouts, A dvances in Cement Research, Vol. 1, No. 4, pp Domone, P.L., Chai, H., 1998, The slump flow test for high workability concrete, Cement and Concrete Research, Vol. 28, pp Page 194
219 References Domone, P.L., Xu, Y. and Banfill, P.F.G., 1999, Developments o f the twopoint workability test for highperformance concrete. M agazine o f Concrete Research, Vol. 51, pp Dransfield, J., 2003, Admixtures for concrete, mortar and grout, In: A dvanced concrete technology, eds. Newman J and Choo BS. Elsevier, Vol. 2, Ch 4. Druta, C., 2003, Tensile strength and bonding characteristics of selfcompacting concrete. M.Sc. Thesis, Louisiana state university and agricultural and mechanical college. Dufour, F. and PijaudierCabot, G., 2005, Numerical modelling of concrete flow: homogeneous approach, In tern a tion a l Jo u rn a l fo r N um erical and A nalytical M ethods in G eomechanics, Vol. 29, pp Duval, R. and Kadri, E.H., 1998, Influence o f silica fume on the workability and the compressive strength o f highperformance concretes, C ement a nd Concrete R esearch, Vol. 28, No. 4, pp Eilers, H., 1941, The viscosity o f emulsions o f highly viscous substances as function of the concentration, Coloid Zh, Vol. 97, pp EN and EN (or BS 6699), 2006, Ground granulated blast furnace slag for use in concrete, mortar and grout, definitions, specifications and conformity criteria. EN 2069:2010, Concrete. Additional rules for selfcompacting concrete (SCC), published April Esping O., 2007, Slump flow values versus Bingham parameters for high flowable mortars and concretes, P roceedings o f the 5th In tern a tion a l R ILE M Sym posium SCC, Ghent, Belgium, pp European guidelines for selfcompacting concrete, specification, production and use, 2005, pp FemandezAltable, V. and Casanova, I., 2006, Influence of mixing sequence and superplasticiser dosage on the rheological response of cement pastes at different temperatures, Cem ent and C oncrete Research, Vol. 36, pp Page 195
220 References Ferraris, C.F., 2000, Comparison of concrete rheometers, International tests at LCPC (Nantes, France) October, National Institute o f Standards and Technology (USA), pp Ferraris, C.F., de Larrard, F.and Martys, N.S., 2001a, Fresh concrete rheology: recent developments. M a teria ls science o f concrete VI, In: S. Mindess, J. Skalny (Eds.), Proceedings, American Ceramic Society. December 2001, American Ceramic Society, Westerville, OH, pp Ferraris, C.F., Obla, K.H. and Hill, R., 2001b, The influence of mineral admixtures on the rheology of cement paste and concrete, C ement a n d C oncrete Research, Vol. 31, pp Feys, D., Heirman, G., De Schutter, G., Verhoeven, R., Vandewalle, L. and Van Germet, D., 2007, Comparison o f two concrete rheometers for shear thickening behaviour of SCC, Magnel Laboratory for Concrete Research, Ghent University, Belgium, pp Flatt, R.J., 2004a, Dispersion forces in cement suspensions, Cement a nd Concrete Research, Vol. 34, No. 3, pp Flatt, R.J., 2004b, Towards a prediction o f superplasticized concrete rheology, M aterials and Structures, Vol. 37, pp Frankel, N.A. and Acrivos, A., 1967, On the viscosity o f a concentrated suspension of solid spheres, Chem istry and E ngineering Science, Vol. 22, pp Gaimster, R. and Dixon, N., 2003, Selfcompacting concrete, in Advanced concrete technology, eds. J Newman, B S Choo Elsevier London, Vol. 3, Ch 9. Gingold, R.A. and Monaghan, J. J., 1977, Smoothed Particle Hydrodynamics, theory and application to nonspherical stars, M onthly N otices o f the R oyal A stronom ical Society, Vol. 181, pp Gjorv, O.E., 1997, Concrete workability: a more basic approach needed, in selected research studies from Scandinavia, report TVBM3078, Lund institute of technology, pp Goodier, C.I., 2003, Development o f selfcompacting concrete, Structures B uilding, Vol. 156, Issue SB4, pp Page 196
221 References Groth, P., 2000, Fibre reinforced concretefracture mechanics methods applied on selfcompacting concrete and energetically modified binders. Ph.D. thesis, Department of civil and mining engineering division o f structural engineering Lulea University of technology Lulea, Sweden. Griinewald, S. and Walraven, J. C., 2003, Rheological measurements on selfcompacting fibre reinforced concrete, P roceedings o f the 3rd International RILEM Symposium on Self Compacting Concrete, eds. O. Wallevik, I. Nielsson, pp , RILEM S. A.R.L, France. Griinewald, S., 2004, Performancebased design o f selfcompacting fibre reinforced concrete, Ph.D. Thesis o f Delft university (Netherlands), pp Grzeszczyk, S. and Lipowski, G., 1997, Effect of content and particle size distribution of highcalcium fly ash on the rheological properties o f cement pastes, Cement a n d Concrete Research, Vol. 27, pp Gupta, R. K., 2000, P olym er a n d com posite rheology, M organtown, USA, CRC Press, pp Guth, E. and Simha, A. R., 1936, Viscosity o f suspensions and solutions, K olloidz, Vol. 74, No Hassan, A.A.A, Lachemi, M. and Hossain, K.M.A., 2010, Effect of metakaolin on the rheology of selfconsolidating concrete. In: P roceedings o f the 2010 International RILEM Symposium on SelfC om pacting C oncrete. Design, production and placement of selfconsolidating concrete eds. Khayat KH. and Feys. D. Canada; pp Heirman, G., Vandewalle, L., Van Gemert, D. and Wallevik, O., 2008, Integration approach of the Couette inverse problem o f powder type selfcompacting concrete in a widegap concentric cylinder rheometer, Jo u rn a l o f N onn ewtonian F luid M echanics, Vol. 150, pp Jacobs, F. and Hunkeler, F., 1999, Design of selfcompacting concrete for durable concrete structures. Proceedings o f SelfC om pacting Concrete Stockholm, Sweden, pp Page 197
222 References Johnston, C.D., 1996, P roportioning, m ixing a n d placem ent o f fibrerein forced cements and concretes, P roduction M ethods a n d W orkability o f C oncrete, Edited by Bartos, Marrs and Cleland, E&FN Spon, London, pp Khayat, K.H. and Z. Guizani., 1997, Use o f viscositymodifying admixture to enhance stability of fluid concrete, A C I M aterials Journal, Vol. 94, No. 4, pp Khayat, K.H. Ghezal, A. and Hadriche, M.S., 1999, Factorial design models for proportioning selfconsolidating concrete, M aterials and Structures, Vol. 32, pp Khayat, K.H., 1999, Workability, testing, and performance o f selfconsolidating concrete, A C IM aterials Journal, Vol. 96, No. 3, pp Khayat, K.H., M.Vachon, and M. C. Lanctot., 1997, Use o f blended silica fume cement in commercial concrete mixtures, A C I M a terials Journal, Vol. 94, No. 3, pp Khayat, K.H., Roussel, Y., 2000, Testing and performance o f fibrereinforced selfconsolidating concrete, First Int. Symposium on SCC, Stockholm, edited by Skarendahl and Petersson, RILEM publications PRO 7, pp Kim, J.K., Han, S.H., Park, Y.D., Noh, J.H., Park, C.L., Kwon, Y.H. and Lee, S.G., 1996, Experimental research on the material properties o f super flowing concrete, In: P. J.M. Bartos, D.L.Marrs, D.J.Cleland (Eds), P roduction M ethods a n d W orkability o f C oncrete, E&FN Spon London, pp Kong, H.J., Bike, G. S. and Li V.C., 2003, Development of selfconsolidating engineered cementitious composite employing electrosteric dispersion/stabilization, Cement and Concrete Com posites, Vol. 25, pp Koshizuka, S., Nobe, A. and Oka, Y., 1998, Numerical analysis of breaking waves using moving particle semiimplicit method, In tern a tio n a l Journal fo r N um erical M ethods in Fluids, Vol. 26, pp Krieger, I.M. and Dougherty, T.G., 1959, A mechanism for nonnewtonian flow in suspensions o f rigid spheres, Journal o f Rheology, Vol. 3, pp Page 198
223 References Kuder, K.G., Ozyurt, N., Mu, E.B. and Shah, S.P., 2007, Rheology of fibrereinforced cementitious materials, C em ent and C oncrete Research, Vol. 37, pp Kulasegaram, S., Bonet, J., Lewis, R.W. and Profit, M., 2002, mould filling simulation in high pressure die casting by meshless method, WCCMV, F ifth w orld congress on com putational m echanics July 712, 2002, Vienna, Austria Eds.: H.A. Mang, F.G. Rammerstorfer, J. Eberhardsteiner. Kulasegaram, S., Bonet, J., Lewis, R.W. and Profit, M., 2004, A variational formulation based contact algorithm for rigid boundaries in twodimensional SPH applications, Com putational M echanics, Vol 33, pp Kurita, M. and Nomura, T., 1998, Highflowable steel fibrereinforced concrete containing fly ash, Proceedings, S ixth C AN M ET/AC I intern a tion a l conference on fly ash, silica fume, slag, and natural p o zzo lan s in concrete, SP178, V. M. Malhotra, ed., American Concrete Institute, Farmington Hills, Michigan, pp Kurokawa, Y., Taniwawa, Y., Mori, H. and Komura, R., 1994, A study on the slump test and slumpflow test of fresh concrete, T ransactions o f the Japan C oncrete In stitute, Vol. 16, pp Kurokawa, Y., Tanigawa, Y., Mori, H. and Nishinosono, Y., 1996, Analytical study on effect of volume fraction o f coarse aggregate on Bingham s constants of fresh concrete, Transactions o f the Japan C oncrete Institu te, Vol. 18, pp Lachemi, M., Hossain, K.M. A., Lambros, V., Nkinamubanzi, P.C. and Bouzoubaa, N., 2004, Performance of new viscosity modifying admixtures in enhancing the rheological properties of cement paste, C ement a n d C oncrete R esearch, Vol. 34, pp Laskar, A.I. and Talukdar, S., 2008, Rheological behaviour of high performance concrete with mineral admixtures and their blending, C onstruction and B uilding M aterials, Vol. 22, pp Li, S.F. and Liu, W.K, 1996, Moving least square Kernel Galerkin method (II) Fourier analysis, C om puter M ethods in A p p lied M echanics and Engineering, Vol. 139, No. 4, pp Page 199
224 References Liu, G.R. and Liu, M.B., 2003, Sm oothed pa rticle hydrodynam ics: A m eshfree p a rticle m ethod, published by World Scientific Publishing Co. Pte. Ltd, Singapore. Liu, M., 2009, Wider application o f additions in selfcompacting concrete. Ph.D. thesis. Department of civil, environmental and geomatic engineering, University College London, pp Lucy L.B., 1977, Numerical approach to testing the fission hypothesis, A stronom ical Journal, Vol. 82, pp Ma, J., Dietz, J. and Dehn, F., 2003, Ultra high performance self compacting concrete (2003) pp , In: SelfC om pacting C oncrete, P roceedings, 3rd Intern. R ILE M Symp. Eds. O. Wallevik and I Nielsson, RILEM Publications S.A.R.L. August 1720, Martys, N.S., 2005, Study o f a dissipative particle dynamics based approach for modelling suspensions, Journal o f R heology, Vol. 49, No. 2, pp Mikanovic, N. and Jolicoeur, C., 2008, Influence o f superplasticisers on the rheology and stability of limestone and cement pastes, C em ent a n d Concrete R esearch, Vol. 38, pp Mindess, S., Young, J. F. and Darwin, D., 2003, H ighperform ance construction m aterials: science and applications, Second Edition, Prentice Hall USA, pp Mittal, K. L. and Kumar, P., 1999, H andbook o f m icroem ulsion science and technology, CRC Press, pp Monaghan, J.J., 1992, Smoothed particle hydrodynamics, A nnual Review o f A stronom y a nd A strophysics, Vol. 30, pp Monaghan, J.J., 1994, Simulating free surface flows with SPH, Journal o f C om putational Physics, Vol. 110, pp Mooney, M., 1957, The viscosity o f a concentrated suspension o f spherical particles, Journal o f C olloid Science, Vol. 6, pp Mori, H. and Tanigawa, Y, 1992, Simulation methods for fluidity of fresh concrete, memoirs of the school of engineering, Nagoya University, Vol. 44, pp Page 200
225 References Morton, R. R. A., 1966, The expected number and angle of intersections between random curves in a plane, Jo u rn a l o f A p p lied P robability, Vol. 3, pp Nehdi, M. and Rahman, M.A., 2004, Estimating rheological properties of cement pastes using various rheological models for different test geometry, gap and surface friction, Cement and Concrete Research, Vol. 34, pp Neophytou, M.K.A, Pourgouri, S., Kanellopoulos, A.D., Petrou, M.F., Ioannou, I, Geoigiou, G. and Alexandrou, A., 2010, Determination o f the rheological parameters of selfcompacting concrete matrix using slump flow test, Jo u rn a l o f ap p lied rheology, Vol. 20 DOI: /ApplRheol Nguyen, T., Roussel, N. and Coussot, P., 2006, Correlation between lbox test and rheological parameters o f a homogeneous yield stress fluid, C ement and C oncrete Research, Vol. 36, No. 10, pp Nicolaides, D., 2004, Fracture and fatigue o f CARDIFRC, Ph.D. Thesis, Department of Civil Engineering, Cardiff University, pp Nmai, C. and Violetta, B., 1996, The use o f flowing concrete in congested areas, C oncrete International, Vol. 18, No. 9, pp Noguchi, T., Oh, S. and Tomosawa, F., 1999, Rheological approach to passing ability between reinforcing bars o f selfcompacting concrete, In: The 1st International R ILE M Symposium on SelfC om pacting C oncrete, Skarendahl A, Petersson O, editors, RILEM Publications S.A.R.L, France pp Noor, M.A. and Uomoto T., 1999, Threedimensional discrete element simulation of rheology tests of selfcompacting concrete, In: P roceedings o f the 1st International RILE M Symposium on SelfC om pacting C oncrete, Skarendahl A, Petersson O (eds). RILEM: Cachan, pp Oh, S. G., Noguchi, T and Tomosawa, F., 1997, Evaluation o f pass ability o f selfcompacting concrete by visualization model, P roceedings o f Japan Concrete In stitute, Vol. 19, N o.l. pp Page 201
226 References Okamura, H. and Ouchi, M., 2003a, Applications of selfcompacting concrete in Japan. In: The 3rd In tern a tion a l R ILE M Symposium on SelfC om pacting Concrete, Wallevik OH, Nielsson I, editors, RILEM Publications S.A.R.L. Bagneux France, pp Okamura, H. and Ouchi, M., 2003b, Selfcompacting concrete, Journal o f A dvanced Concrete Technology, Vol. 1, No. 1, pp Okamura, H. and Ozawa, K., 1995, Mix design for selfcompacting concrete, Concrete Library o f JSCE, Vol. 25, pp Okamura, H. Ouchi, M. Hibino, M. and Ozawa, K., 1998, A rational mixdesign method for mortar in selfcompacting concrete, The 6th Exist A siap acific Conference on Structural Engineering & C onstruction, Vol. 2, pp Okamura, H., 1999, Self compacting concrete development, present use and future, Proceedings o f F irst R ILE M In tern a tio n a l Symposium on S e lf C om pacting C oncrete, Stockholm, September, pp Okamura, H., Ozawa, K., Ouchi, M., 2000, Self compacting concrete, Structural C oncrete, Vol 1, pp Ouchi M, Hibino M and Okamura H., 1996, Effect o f superplasticiser on selfcompact ability in fresh concrete, transportation research record, lo u m a l o f the Transportation Research Board, Vol. 1574, pp Ouchi, M. and HibinoNagaoka, M., 2000, Development, applications and investigations of selfcompacting concrete, Kochi University o f Technology, Japan, pp Ouchi, M., 1999, Stateoftheart report on selfcompact ability evaluation, P roceedings of the International W orkshop on SelfC om pacting C oncrete (CDROM ), Kochi, Japan, March 1999, Also available from concrete engineering series, No. 30, Japan society of civil engineers, pp Ouchi, M., Nakamura, S., Osterson, T., Hallberg, S. and Lwin, M., 2003, Applications of selfcompacting concrete in Japan, Europe and the United States, ISHPC, p 25. Page 202
227 References Ozawa, K. Maekawa, K. Kunishama, M and Okamura, H., 1989, Development of high performance concrete based on the durability design o f concrete structures, Proceedings o f the 2nd E asta sia a n d P a cific C onference on Structural E ngineering and C onstruction (EASEC2), Vol 1, pp Ozawa, K., Maekawa, K., Okamura, H., 1990, High performance concrete with high filling capacity, P roceedings o f R ILE M In tern a tion a l Symposium on A dm ixtures fo r Concrete: Improvement o f P roperties, ed. E Vasquez, Barcelona, pp Papadakis, V.G., 1999, Experimental investigation and theoretical modelling of silica fume activity in concrete, C em ent a n d C oncrete R esearch, Vol. 29, pp Papanastasiou, T.C., 1987, Flows o f materials with yield, Journal ofr h eo log y, Vol. 31, pp Pashias, N., Boger, D., Summers, J. and Glenister, D., 1996, A fiftycent rheometer for yield stress measurement, Journal ofr heology, Vol. 40, pp PCI, 2003, Interim guidelines for the use o f selfconsolidating concrete in precast prestressed concrete institute member plants, pp Petersson, O., 2003, Simulation o f selfcompacting concrete  laboratory experiments and numerical modelling o f testing methods, j ring and 1box tests, In: Proceedings of the 3rd International R ILE M Symposium, Pro 33, Wallevik O, Nielsson I (eds). RILEM: Cachan, pp Petit, J.Y., Wirquin, E., Vanhove, Y. and Khayat, K., 2007, Yield stress and viscosity equations for mortars and selfconsolidating concrete, Cement a nd Concrete Research, Vol. 37, pp PhanThien, N. and Huilgol, R.R., 1980, A micromechanic theory o f choppedfibrereinforced materials, Journal o f F ibre Science and Technology, Vol. 13, pp PhanThien, N. and Karihaloo, B.L., 1994, Materials with negative poisson's ratio: A qualitative microstructural model, Journal o f A pplied M echanics, Vol. 61, pp Page 203
228 References Quemada, D., Models for rheological behaviour of concentrated disperse media under shear. In: A dvances in R heology (eds. B. Mena, A. GarciaRejon, C. Rangel Nafaile), Universidad Nacional Autonama de Mexico, Mexico City, pp Ramachandran, V. S., Feldman, R. F. and Beaudoin, J. J., 1981, Concrete Science, Heyden and Son Ltd London, ISBN , pp Reinhardt, H.W. and Wustholz, T., 2006, About the influence o f the content and composition of the aggregates on the rheological behaviour o f selfcompacting concrete, M aterials and structures, Vol. 39, pp Richard, P. and Cheyrezy, M., 1995, Composition o f reactive powder concrete, C ement and Concrete Research, Vol.25, No.7, pp RILEM (2002), Workability and rheology o f fresh concrete: compendium of test. Report of technical committee TC145WSM. Bartos, P.J.M., Sonebi M. and Tamimi, A.K. (eds), RILEM, Paris, pp RILEM TC 174 SCC, 2000, Self compacting concrete Stateoftheart report o f RILEM technical committe 174SCC. Skarendahl A, Petersson O, editors, RILEM Publications S.A.RL., France. Robinson, J.V., The viscosity o f suspension o f spheres: sediment volume as a determining parameter. Transactions o f the Society ofr heology, Vol. 1, p. 15. Roussel, N., 2006, A theoretical frame to study stability o f fresh concrete, M aterials and Structures, Vol. 39, No. 285, pp Roussel, N., 2007a, A thixotropy model for fresh fluid concretes: Theory and applications, Proceedings o f the 5 th In tern a tio n a l R ILE M Symposium SC C , pp , Ghent, Belgium. Roussel, N., 2007b, Rheology o f fresh concrete, from measurements to predictions o f casting processes, M aterials a n d Structures, Vol. 40, pp Roussel, N., and Coussot, P., 2005, fiftycent rheometer for yield stress measurements: From slump to spreading flow, Journal ofr heology, Vol.49, No. 3, pp Page 204
229 References Roussel, N., Geiker, M.R., Dufour, F.,Thrane, L.N. and Szabo, P., 2007, Computational modelling o f concrete flow : general overview, Cement a nd C oncrete Research, Vol.37, pp Roussel, N., Staquet, S., D'Aloia Schwarzentruber, L., Le Roy, R. and Toutlemonde, F, 2007, SCC casting prediction for the realization o f prototype VHPCprecambered composite beams, M aterials and Structures, Vol. 40, No. 9, pp Roussel, N., Stefani, C. and Leroy, R., 2005, From minicone test to abrams cone test: measurement of cementbased materials yield stress using slump tests, Cement and C oncrete Research, Vol. 35, No. 5, pp Roziere, E., Granger, S., Turcry, Ph., and Loukili, A., 2007, Influence of paste volume on shrinkage cracking and fracture properties o f self compacting concrete, Cement and C oncrete Com posites, Vol. 29, No. 8, pp doi: /j.cemconcomp Russel, W.B., 1973, On the effective moduli o f composite materials: Effect of fiber length and geometry at dilute concentrations, Zeitschrift fu r Angew andte M athematik und P hysik (ZAM P), Vol. 24, pp Russell, H. G., 1997, High performance concretefrom buildings to bridges, Concrete International, Vol. 19, No. 8, pp Saak W.A., Jennings H.M. and Shah S.P., 2001, New methodology for designing SCC, A C I M aterials Journal, Vol. 98, pp Saito, N., 1950, Concentration dependence o f the viscosity o f high polymer solutions. I, Journal o f the P hysical S o ciety o f Japan, Vol. 5, pp Sedran, T. and De Larrard, F., 1999, Optimization o f self compacting concrete thanks to packing model, P roceedings o f F irst R ILE M International Symposium on S e lf C om pacting Concrete, Stockholm, September, pp Shao, S. and Lo, E.Y.M., 2003, Incompressible SPH method for simulating Newtonian and nonnewtonian flows with a free surface, A dvances in W ater Resources, Vol. 26, pp Page 205
230 References Shenoy, A.V., 1999, R heology o ffille d polym er system s, Springer USA, pp Simha, R., J., 1952, Mathematics o f solidliquid suspension, Journal o f A pplied P hysics, Vol. 23, pp Sobolev, K. G., 1999, High performance concretes, Dundee, Scotland. 4th International Conference  C reating w ith C oncrete, 610 September 1999, Edited by Ravindra K Dhir and Kevin A Paine, pp Sonebi, M. and Bartos, P., 2005, Filling ability and plastic settlement of self compacting concrete, M aterials and structures, Vol. 35, pp Sonebi, M., 2004, Medium strength selfcompacting concrete containing fly ash: Modelling using factorial experimental plans, C em ent an d C oncrete R esearch, Vol. 34, No.7, pp Sonebi, M., Zhu, W. and Gibbs, J., 2001, Bond o f reinforcement in selfcompacting concrete, Cement and Concrete Research, Vol. 35, No. 7, pp Solomon, H., 1978, Geometric probability. Society for industrial and applied mathematics, USA. Spangenberg, J., Roussel, N., Hattel, J.H., Thorborg, J., Geiker, M.R., Stang, H. and Skocek, J., 2010, Prediction o f the impact o f flowinduced inhomogeneities in selfcompacting concrete (SCC). In: P roceedings o f the 2010 In tern a tio n a l R ILE M Symposium on S elf Com pacting C oncrete. Design, production and placement of selfconsolidating concrete eds. Khayat KH. and Feys. D. Canada; p Struble, L. and Sun, G.K., 1995, Viscosity o f portland cement paste as a function of concentration, A dvanced C em ent B ased M aterials, Vol. 2, pp Su, N, Hsu, K.C. and Chai, H.W., 2004, A simple mix design method for selfcompacting concrete, Cem ent and C oncrete Research, Vol. 31, pp Sun, Z., Voigt, T. and Shah, S.P., 2006, Rheometric and ultrasonic investigations of viscoelastic properties o f fresh Portland cement pastes, Cement and Concrete Research, Vol. 36, pp Page 206
231 References Tattersall, G.H., 1991, W orkability a n d qu a lity control o f concrete, E&FN Spon, London, pp The European Guidelines for selfcompacting concrete; specification, production and use. www. efnarc. or s Thrane, L., Szabo, P., Geiker, M., Glavind, M. and Stang, H., 2004, Simulation of the test method 1box for selfcompacting concrete, Annual Transactions o f the N ordic Rheology Society, Vol. 12, pp Thrane, L.N., 2007, Form filling with selfcompacting concrete. Ph.D. Thesis concrete centre danish technological institute department o f civil engineering department of chemical engineering technical university o f Denmark. ISBN Tregger, N., Ferrara, L. and Shah, S.P., 2007, Empirical relationships between viscosity and flow time measurements from minislump tests for cement pastes formulated from SCC, Proceedings of the 5th In tern a tion a l R ILE M Symposium SC C 2007, Ghent, Belgium, pp Tregger, N., Ferrara, L. and Shah, S.P., 2008, Identifying viscosity of cement paste from minislumpflow test, A C I M aterials Journal, Vol. 105, pp Utracki, L.A., 2003, Polym er B lends H andbook, Springer London, pp Utsi, S., 2008, Performance based concrete mix designaggregate and micro mortar optimization applied on selfcompacting concrete containing fly ash. Ph.D. Thesis, Lulea, Sweden: division o f structural engineering, Lulea University o f Technology, pp Utsi, S., Emborg, M and Carlsward, J., 2003, Relation between workability and rheological parameters, In: P roceedings o f the 3rd In tern a tion a l R ILE M Symposium, Pro 33, Wallevik O, Nielsson I (eds). RILEM: Cachan, pp Vand, V., 1948, Viscosity o f solutions and suspensions, n, experimental determination of the viscosity & concentration function o f spherical suspensions, The Journal o f P hysical and C olloid C hemistry, Vol. 52, pp Page 207
232 References Vasilic, K., Roussel, N., Meng, B. and Kuhne, H.C., 2010, Computational modeling of SCC flow through reinforced sections in selfcompacting concrete (SCC), In: Proceedings o f the 2010 International R ILE M Symposium on SelfC om pacting Concrete. Design, production and placement of selfconsolidating concrete eds. Khayat KH. and Feys. D. Canada; pp Vikan, H. and Justnes, H., 2003, Influence o f silica fume on rheology of cement paste, Proceeding o f intern a tion a l symposium. SelfC om pacting C oncrete, Reykjavik, Iceland, August, 2003, pp Wallevik J.E., 2006, Relationship between the Bingham parameters and slump, Cement and Concrete Research, Vol. 36, pp Wallevik, O.H. and Gjorv, O.E., 1990, Development of a coaxial cylinders viscometer for fresh concrete, eds. Wiereg, H.J., P ro p erties o f F resh C oncrete, Chapman and Hall. London, pp Wendt, J. F. (1992), C om putational flu id dynam ics, an introduction, Springer London, pp Westerholm, M., Lagerblad, B., Silfwerbrand, J. and Forssberg, E., 2008, Influence o f fine aggregate characteristics on the rheological properties o f mortars, Cement a nd Concrete Com posites, Vol. 30, pp Williams, D.A., Saak, A.W. and Jennings, H.M., 1999, The influence of mixing on the rheology of fresh cement paste, C ement a n d C oncrete R esearch, Vol. 29, pp Wildemuth, C.R. and Williams, M.C. 1984, Viscosity o f suspensions modelled with a sheardependent maximum packing fraction, R heologica A cta, Vol. 23, pp Willis, J. R. and Acton, J. R., 1976, The overall elastic moduli of a dilute suspension of spheres, The Q uarterly Jo u rn a l o f M echanics a n d A p p lied M athematics, Vol. 29, pp Wu, Z., Zhang, Y., Zheng, J. and Ding, Y., 2009, An experimental study on the workability of selfcompacting lightweight concrete, C onstruction B uilding m aterial, Vol. 23 pp Page 208
233 References www. ermco. org., 2010, European readymixed concrete industry statistics Yahia, A., Tanimura, M., Shimabukuro, A. and Shimoyama, H., 1999, Effect of limestone powder on rheological behaviour o f highly flowable mortar, Proceeding o f Japan Conference, Vol. 21, No. 2, pp Yamada, K., Takahashi, T., Hanehara, S. and Matsuhisa, M., 2000, Effects of the chemical structure on the properties o f polycarboxylatetype superplasticiser, Cement and Concrete Research, Vol. 30, No. 2, pp Zhang, X. and Han, J., 2000, The effect o f ultrafine admixture on the rheological property of cement paste, C ement a n d C oncrete R esearch, Vol. 30, pp Page 209
234 Appendix A A.1 Corrected S P H integration The basic SPH approximations as given by equation (3.44) or (3.47) do not accurately reproduce or approximate the functions ^ ( x ) and V ^( x ). Therefore, in the past, corrected SPH equations were developed to address these issues (Bonet and Lok, 1999; Bonet and Kulasegaram, 2000). The main aim o f the correction techniques is to satisfy the conservation of angular momentum which, unlike the linear momentum, is not automatically satisfied. For two neighbouring particles, a and b, it can be shown (Bonet and Lok, 1999) that the angular momentum is preserved if Z (***J vb; K ) = i b=l Pb (A.1) where xa and xfc are the position vectors of particles a and b, respectively. In order to correct the SPH algorithms, either the gradient o f the kernel is addressed directly (Bonet and Lok, 1999) or the kernel function itself is modified (Li and Liu, 1996). Another possible way is to mix the kernel and gradient corrections (Bonet and Kulasegaram, 2000; Bonet and Lok, 1999). In following these methods are discussed in more detail. A. 1.1 Gradient correction The kernel gradient is modified by introducing a correction matrix L such that VWi (i) = 'LVWb ( j.) (A.2) In (A.1), if general SPH equation (for any particle i.e. without subscript a) is used and the term VWb (x) is replaced by its corrected one (A.2), we have 2 ^ ( i t * ) L V» ;(* ) = I (A.3) b=\ Pb Therefore, L is given by (A.4) Page 210
235 A. 1.2 Kernel correction The kernel can be modified to ensure that polynomial functions up to a given degree are exactly interpolated. The linear kernel correction is given by Wb(x ) = Wb ( * )a ( * ){ l+ * ( * ) ( *  *»)} (A.5) For any linear field, such as velocity, the correction formulation is N m ',o + v lx = X (v o + vi * (.) ^ W (A. 6) 6=1 Pb The following completeness conditions must be satisfied ^ f r b(,i) = l (A. 7) 6=1 Pb m. 6=1 Pb (x ~ x<.) ^ ( x) = (A8> The vector parameter, P(jc) is obtained by substituting (A.5) into (A.8) Z ~ ( x  x i. K ( x) P(x)= Pb (A.9) Z ~ i (x  xi,)(8,(x  xi, ) ^ ( x) 6=1 Pb Substituting (A.5) into (A.7) gives the scalar parameter, a ( x ) as a ( i ) = jj {l + p(x)(x xk)}»;(x) 6=1 Pb As can be seen from (A.9) and (A. 10) both a(x) and p(x)are functions of x and therefore make this correction expensive in terms o f the computational time. A possible way to make the correction less time consuming is by ignoring p (x ), i.e. the kernel is corrected by using a constant rather than a linear correction. Therefore the interpolation of the field function v(x) becomes Page 211
236 v W = Z v<.^(*) tp b (A. 11) where W fx l WbW = ^ T ~ (A12) fcf a A. 1.3 Combined kernel and gradient correction Another possible correction technique is by mixing the kernel and gradient corrections described above. The corrected gradient o f the corrected kernel is given by V ^ (x ) = LVf*;(x) (A. 13) VWb (x) can be obtained by differentiation o f (A. 12) to give Z ^ ( s ) H A (A. 14) where m. Similar to (A. 14), the correction matrix L is given by L = (A. 16) Note that, in (A. 16), the term xis no longer required since only the constant kernel is used instead of a linear one. Using the corrected gradient of the corrected kernel, the SPH equations (3.44) and (3.47) can be rewritten as * /W. <A17) b=1 Pb Page 212
237 v#(») Z *?» ; ( * ) (A. 18) 6=1 A> Page 213
238 Appendix B Mix compositions of the reference mixes of series OS used in Chapter 5 (after Grunewald, 2004) Mix 1 Mix 2 Mix 3 Mix 4 Mix 5 Mix 6 Mix 7 CEM ffl 42.5 N CEM I 52.5 R i Water SP CUGLA (20% solid) LR SP CUGLA (35% solid) HR * "< Fly ash to G Fly ash O (J Sand ( mm) round CA (416mm) round Ratios Water/Cement Water/Binder Page 214
239 Appendix C Number of steel fibres cut by the diametrical vertical section of the slump cone (after Nicolaides, 2004) The number of steel fibres that will theoretically be seen in one cut section of the particular volume is given by the theory o f geometric probability or more precisely by the solution of the socalled BufFon problem in three dimensions (Solomon 1978). Although the proof of the particular problem is beyond the scope o f the current work, some basic points are described below. The original problem called the the BufFon needle problem is about the probability of a needle (line segment) o f length / that is dropped at random on a set of equidistant parallel lines in a plane that are d units apart, / < d intersecting a line (see Figure C.l). The problem is solved by considering a finite number o f possible positions for the needle as equally likely outcomes and then treating the limiting case as a representation o f the problem. This includes a definition o f randomness for the distance x o f the needle s midpoint to the nearest line and the acute angle q> formed by the needle and a perpendicular form the midpoint to the line. The solution is obtained by computing the ratio of favourable outcomes to the total set of outcomes and passing to the limit. Figure C.l: BufFon needle problem in twodimensions BufFon s problem is also extended to those situations where the needle is larger than the shortest distance between grid lines, and therefore multiple intersections can be seen. However, a more general extension o f the problem is the one provided by Morton (1966), who proved an important and remarkable result on the expected number of intersections and distribution o f angles o f intersections for a random set o f rectifiable curves in the plane. Page 215
240 The three dimensional situation takes as its point of departure a result by Crofton (1885) which shows that if a line is repeatedly placed at random over a plane containing a closed figure, the average length o f the chord E(c) intersected by the figure will be, x area E(c) = 7t : pen meter (C.l) no matter what the shape o f the figure, as long as its boundary is a convex curve. However, before this result could be employed for estimating volumesurface area ratios it required the following modifications: 1. it had to be made applicable to line segments; 2. a simple procedure for measuring chord length had to be found; 3. it had to be extended to cover nonconvex figures (e.g. figures with reentrant comers); 4. it had to be extended to provide an estimate not only of the areaperimeter ratio in the focal plane under observation but the volumesurface ratio in the three dimensions of which the observed focal plane is a twodimensional representation. The first three of these modifications were accomplished by a single device. A line of finite length, say /, was considered and the number o f times each o f the two end points fell in the interior of a plane figure was counted. This number was denoted by E (/z) for hits and the number of times the line intersected the perimeter o f the figure was denoted by E (c) for cuts. Then, in a very large number o f throws it will be found that / M = (C.2) E(c) perimeter for all closed figures including the nonconvex ones. The fourth and important modification was provided by a mathematical result. When a line of length / is placed at random in threedimensional space containing a closed figure, for a very large number of throws it may be shown that Page 216
241 E(h) volume / ^  = (C.3) E(c) surface area This result satisfied condition 4. Since placing a line at random in three dimensions could be shown to be formally equivalent to placing a plane at random in three dimensions and placing the line at random on the resulting twodimensional plane section. If the space contains a series o f figures o f different volumes and surfaces, then E(h) y volumes / ttk E (c) = 4^X su rfa ^ c e areas <C 4) Here E(ti) is the number o f hits, i.e. the number of times each of the two end points of the line fall in the interior o f the plane closed figure and E(c) is the number of times the line intersects the perimeter o f the figure. As in two dimensions, this result applies irrespective of whether the closed figure is convex or not. The above theoretical result is used here to calculate how many 30 mm long steel fibres will be cut by the diametrical vertical section o f the slump cone. Volume of truncated cone = V =? J (R Z+ r2 +Rr)= ^ ^ (loo x50) = mm3 Volume of each fibre with 0.55 mm diameter and 30 mm length = mm Number of fibres (2.5 % by volume) in the truncated cone = x = v J Let us subdivide the cone volume into cubes o f 40 mm side, thus (C.4) becomes ^ E(h) _/aa 8 v 30x ) ' =4x =>E(h) = E(c) E(c) 6x1600 w 9 w w» \ w \ 64000x2.5 Number of fibres in a 40 mm cube  E(h) + Eye) = ]qqx^ ^ 7 ~ Therefore, the number o f fibres cut by 40 x 40 mm section is E(c) = 119 Area of the diametrical vertical section o f slump cone is mm2. Page 217
242 Therefore the number o f fibres that will be cut by the diametrical vertical section ^  x =
243 Appendix D Data Sheets and Health and Safety Sheets
244 Health and Safety Information  Blue Circle Portland Cements o This datasheet provides the information required by the Chemicals (Hazard Information and Packaging) Regulations. HEALTH & SAFETY INFORMATION BLUE CIRCLE PORTLAND CEMENTS IRRITANT Autumn I d e n t i f i c a t i o n o f Substance/ Supplier Section An odourless w hite to grey p o w d er mainly insoluble in w ate r. W h e n w a te r is a d d e d it b ecom es a b in d e r f o r co n stru c tio n applications. This d atash eet eppfces to th e following Blue Circle cem ents. Portland (CEM 1) cem ents M astercrete Original Extra Rapid Cem ent Procem Portland Limestone C em ent Fenocrete SuVacrete Snow crete Phoenix M icrocem CEM blend. Lafarge Cement United Kingdom Manor Court Chilton 0X11 ORN Technical helpline: Composition/Information on Ingredients 2.1. Chemical Description The principal constituents of th ese cem ents a re calcium silc ate s. a lu m in a tes, fe rro  alum inates an d sulfates. Small a m o u n ts of alkalis, lime a n d chlorides are also p re sen t to g e th er w ith tra ce am o u n ts of chrom ium com pounds. A dditional co n stitu en ts m ay also be p re s e n t e g p u lv e rized fu e l a sh, limestone, a n d g ran u lated blastfu rn ace slag. CAS: Hazardous Ingredients a} The lime, calcium silicates a n d alkalis w ithin th e c e m e n t a te partially soluble and w h en m ixed w ith w a te r will g ive rise to a potentially h azardous alkaline solution. b) H exavalent chro m iu m s a lts in th e s e cem en ts are soluble an d w h e n m ixed w ith w ater, w ll give rise to a patentiaby hazardous solution. 3. Hazards Identification W hen cem en t is m ixed w ith w a te r such as w hen m aking co n crete o r m ortar, o r w hen th e cem ent becom es dam p, a strong alkaline s o lu tio n is p ro d u c e d. If th is co m es in to co n tact w ith th e eyes o r skin it m ay cause serious b u rn s a n d ulceration. T he eyes are partictjarty vulnerable a n d d a m a g e will increase w ith contact tim e. Strong alkaline solutions in co n tact w ith th e skin te n d to d a m a g e th e nerve endings first b efore dam aging th e skin, therefore chemical b u m s ca n dev elo p w ith o u t pain being felt a t th e tim e. C em en t m o rtar a n d c o n c re te mixes m ay until set ca u se b o th irritant a n d allergic contact derm atitis: Irritant c o n ta c t d e rm a titis is d u e to a com bination of th e w etn ess, alkafinity a n d abrasiveness o f th e constitu en t m aterials. A le rg ic c o n ta c t d e rm a titis is c a u sed mainly by th e sensitivity of a n individuals skin to hexavalent chrom ium salts. 4. First Aid Measures Eye Contact W'ash eyes im mediately w ith clean w ater fo r a t least 15 m inutes a n d seek m edkal advice w ithout delay. Skin Contact W ash th e affected are a thoroughly with s o a p a n d w a te r b e fo re co ntinuing. If irritation, pain o r o th e r skin tro u b le occurs, seek m edical advice. C lothing co n tam in ated by w e t cem ent, concrete or m ortar should b e removed an d w ashed thoroughly before use. Ingestion Do not induce vomiting. W ash out m outh w ith w a te r an d g ive p a tie n t p lenty of w a te r to drink. Inhalation If irritation occurs, m ove to fresh air. If n o se o r airw ays becom e inflam ed seek m edical advice. 5. Fire Fighting Measures C em ents are not flam m able an d will n o t faclitate com bustion w ith other materials. 6. Accidental Release Measures 6.1. Personal Precautions (See 8.3. overleaf) 6 2 Method of Cleaning Recover th e spillage in a dry state if possfcle M inimise generation of airborne dust. The p roduct can be slurried by th e addition of w a te r b u t will subsequently s e t as a hard m aterial. K eep children aw ay fro m clean up operation. 7. Storage and Handling 7.1. Storage Bags should be stacked in a safe an d stable m anner. 72. Handling W hen handling cem ent bags due regard should b e paid to th e risks outlined in th e M anual Handling O perations Regulations. Som e b ag s m ay have a small am ount of cem ent o n th e o u te r surface. A ppropriate personal protective clothing (see 8.3) should therefore be used w h ist handling 7.3. Control of Hexavalent Chromium From 17 January 2005, those cem ents which naturally contain m ote th a t 2 ppm of soluble hexavalent chrom ium (chrom ium (VI)) by dry w eight of cem ent, w ll b e tre a te d w ith a chem ical reducing ag e n t (such as ferrous sulate) that maintains th e level of hexavabnt chrom ium in th e cem ent to below 2 ppm by dry weigh* of cem ent. The effectiveness of th e reducing a g e n t red u ces w ith tim e, th e re fo re c e m en t b ag s a n d /o r delivery d o cu m en ts will co n tain inform ation on th e period of tim e ('shelf life') for w hich th e m anufacturer h as established th a t th e reducing a g e n t will co n tin u e to limit th e level of hexavalent chrom ium to less than 2 ppm> by dry w eight o f cem ent. They w ll also indicate th e a p p ro p ria te sto rag e conditions for maintaining th e effectiveness of the reducing agent. Blue C ircle" is a b ra n d o f J U F A R G E BLUE CIRCLE PORTLAND CEM ENTS Page 220
245 BLUE CIRCLE PORTLAND CEMENTS If c e m en ts a re incorrectly s to re d, o r u s e d after the end of th e declared shelf We th e level of hexavalent chrom ium m ay rise above 2 ppm by dry w e ig h t o f c e m e n t, w ith a consequent increase in th e potential risk of allergic contact derm atitis. Note: W hite P ortland c e m e n t is typically low in soluble hexavalent chrom ium a n d would be exem pt from these requirem ents 8. Exposure Controls 8.1. Workplace Exposure Umits (WELV WEL* 8hr Tim e W e ig h ted A verage (TWA) Total inhalable d u st 10 m g tn 3 8 h r TWA Respirable dust 4mg/m3 8 h r TWA 8.2. Engineering Control Measures Where reasonably practicable, d u st exposures shook) be controled by engineering m ethods Recommended Protective Equipment Respiratory Protection Suitable respiratory protection should b e w orn to ensure th a t personal exposure is less than the WEL. Hand and Skin Protection Protective cbthing should b e w orn w hich ensures th a t c e m e n t, o r a n y c e m e n t/ w ate r m ixture e g c o n c re te o r m o rtar, does net com e into contact w ith th e skin. In som e circum stances s u c h a s w h e n laying concrete, w aterp ro o f troc&ers an d w ellngtons m ay b e necessary. Particular care should be ta k en to en su re that w et concrete does not e n ter th e boots and persons do not kneel o n th e w et concrete so as to bring th e w e t concrete into contact w ith unprotected skin. Should w e t m ortar o r w e t co n c re te g e t inside boots, gloves o r o th e r p rotective d o th in g th e n th is p ro te c tiv e clo th in g should b e immediately rem oved a n d th e skin thoroughly w ash ed as w ell a s t h e protective dothing/footw ear Eye Protection D ustproof g o g g le s sh o u ld b e w o rn w herever th e re is a risk of c e m e n t pow der or any cem ent/w ater mixtures entering the eye. 9. Physical/Chemical Properties 9.1. Physical Data Physical state M ean particle size O dour Particulate micron Not applicable (N/A) ph ph o f w e t c e m e n t Viscosity Freezing point Boiing point Melting point Flash point Explosive properties N/A N/A N/A N/A Not flam m able N ot explosive D ensity kg/m 3 Solubility m /a 9.2. Chemical Compounds M ainly a m ixture of: 3 C a 0.S j0 2.2 C a0.s i C ao A bo,. 4 C ao A JjO j, F ^O j.c as O * C ontains less than 1 % crystalline silica. 10. Stability and Reactivity C onditions co n trib u tin g to chem ical instabifity: N one. H azardous decom position products: N one. Special precautions: N one. 11 Toxkologica I Information Short Term Effects Eye Contact C e m e n t is a severe eye irrita n t Mild ex p o su res ca n c a u se soreness. G ross exposures o r untreated mild exposures c a n lead to chem ical b u rn in g a n d ulceration of th e eye. Skin C e m e n t p o w d e r o r a n y c e m e n t/w a te r m ix tu re m a y c a u s e irrita n t c o n ta c t derm atitis, allergic (chrom ium ) derm atitis, a n d /o r b urns. Ingestion T he sw allow ing o f sm all a m o u n ts o f c e m e n t o r any c e m e n t/w a te r m ixtures is unlikely to c a u se a n y sig n ifican t reactio n. Larger d o s e s m ay result in irritation to th e g a stro intestinal tract. Inhalation C em ent pow der m ay cause inflam m ation of m u c o u s m e m b ran es Chrome Effects R e p e a te d ex p o su res in ex cess o f th e WEL h a v e b e e n lin k ed w ith rhinitis a n d c o u g h in g. Skin e x p o s u re has b e e n linked to allergic (ch ro m iu m ) d e rm a titis. A llergic d e rm a titis m o re co m m o n ly arise s th r o u g h c o n ta c t w ith c e m e n t/w a te r m ix tu res th a n d ry c e m e n t. 12. Ecological Information Aquatic Toxicity Rating LCSO aquatic toxicity rating not determ ined. T he a d d itio n o f c e m e n ts t o w a te r w il, h o w ev er, ca u se th e ph to rise a n d m ay th e refo re b e toxic to a q u a tic life in som e circum stances Biological Oxygen Demand (BOD) Not applcable. 13. Disposal Considerations D ispose o f em p ty b ag s o r surplus ce m ent to a p la ce au th o rised to ac cep t builder's w aste (nonhazardous m aterials landfif). K eep o u t o f th e reach o f children. 14. Transport Information CU nification fo r conveyance: Not required. 15. Regulatory Information Chemicals (Hazard Information & Packaging) Regulations Classification: Irritant. 1SJ. Risk Phrases C ontains chrom ium (VI). M ay produce an allergic reaction. Risk of serious dam age to eyes. Contact w ith w et cem ent, w et concrete o r w et m ortar m ay cause imitation, derm atitis o r b u m s. C ontact betw een cem ent p ow der an d b ody fluids (eg sw e at an d eye fluid) m ay also cause skin an d respiratory irritation, derm atitis o r bum s. R 37/38/41/ Safety Phrases Avoid eye an d skin contact by w earing suitable eye protection, clothing an d gloves. Avoid breathing dust. Keep out of reach of children. O n c o n ta c t w ith ey e s o r skin, rinse im m edately w ith plenty of clean w ater. Seek medical advice after eye contact. S 2/22/24/25/26/37/ Legislation and Other Information CONIAC H ealth H azard Inform ation S heet N o 26, C em ent. Health & Safety at W ork Act C ontrol of S ubstances H azardous to Health (Regulations). HSE G uidance N ote EH40 (W orkplace Exposure Limits). Any authorised m anual o n First Aid by S t Johns/St Andrews/Red Cross. Manual Hancfcng Operations Regulations Environmental Protection Act. J l a f a w g e J E v C E M E N I U n t. d Kingdom A leading company... and a leading brand Th* information in this dates h**t is accurate at fit tim t of printing, but Lafarge C tm tn t UK ieser.«the right to amend detafs as part of their product development programme HS:3:1CV06 o la* f wit* Page 221
246 Elkem Microsilica CONCRETE Guidance for the Specification of Silica Fume C1T)5 General Information General Silica Fume (also often termed condensed silica fume and microsilica) is a powerful pozzolanic material and has been used as an addition to concrete for som e 30 years. However, until more recentty only a few international standards have been available for the specification of the material. This datasheet reviews the main standards and provides advice on how silica fume should be specified History The first patent for a Silica Modified Cement' was granted n the USA in 1946 This was long before the first fullscale filtering came online. In 1986, Canada drew uo a Standard for Supplementary Cementing Materials  which included silica fume This was revised in In 1995, ASTM produced a Standard for the American market place and this undergoes almost annual review A new European Standard is under approval and will probably be issued in 20C5. These are the three main standards in global use, but many countnes have now issued national standards for silica fume of which som e are shown in Table 1. Each should be checked for the date and only the latest edition used when specifying the silica fume Elkem Microsilica*1 Elkem Materials produce Elkem Microsilica* which conforms to the mandatory requirements of the relevant standards from : American Society for Testing and Materials European Committee for Standardisation Kindly se e our Product Datasheets. Standardisation Criteria In order that the silica fume is of a suitable quality to use in concrete, a certain number of parameters have been set. vvhi e som e of the values set may vary in National* Standards, die limits discussed here are considered the norm. Silicon Dioxide (S i0 2)  minimum 85% While lower content fumes may be used under som e National Standards, this is considered the lowest level for effective reaction in concrete use. Specific Surface Area to m2.kg SSA defines me size of the particles. The higher the value, m e smaller the sphere size. A normal number is around 20 0C0 Out of range high values could have negative physical effects in the fresh concrete L oss on Ignition  maximum 4 to 6% This is the amount of organic contaminant in the material. The lower this figure, the higher the quality. The 6% value is derived from the standard for fly ash. itransm&sicr Electron Microscopy} picture of sites \ime Retained on 45 micron sie v e  up to 10% The oversize' partcles in the fume These may be agglomerates or crystalline material The lower this figure, the higher the quality. This is probably the most variable figure, with tolerance being up to 10%. depending on the standard used Pozzolanic Activity Index The reactivity of the silica fume This figure also varies from standard to standard depend ng on the design of the test mix and curing conditions. A good silica fume will always give a figure above 100% at 28 days. Mix Proportioning Due to the wide and varied nature of all the constituents of concrete  cements, aggregates, admixtures etc  it is not feasible to give exact proportions for specific mixes  especially on a global' basis however, a review of past projects, and the mixes used, can give an insight into the level of silica fume dosage that may be advantageous for certain applications. These are quite simply, starting points for mix designs until sufficient local information has been determined. In almost al circumstances silica fune concrete is produced using a piasticiser or suoerplasticiser Table 2 sets out examples of the percentages that are suitable for the types of mixes given Dosage levels will be relative to the environmental conditions and the performance requirements, hence the ranges given and the stress on trial mix work. The table shows areas of overlap. SEkem Page 222
247 Manoasory chemcal and physical requirements # A m erican AST* C T 7 f i E uropean EM I 0 5,. J L G 0 v < $ A C anadian CAK'CSA A Japan ese JIS A C0 C hinese GBJT1873S Brazilian NBR 13356:1357 Korean KS f Vietnam ese TCXOVN 312CC3 Indian IS 15398:2003 > 6S.G >65 >95 >95 >65 >95 >85 >85 >85.0 * o, w <2.0 <1.0 <3.0 <3.0 a w 03 < <0.3 FraeCaO W «1.0 <1.0 MgO(% <5.0 <50 Free Si W <0.4 AvaUftOeattals (ka.o equivsent 14} Report <1.5 <1.5 Moisture!<4) <3,0 <3.0 <3.0 <3.0 <3 JD <3.0 lom or igntt %) < <6.0 <5.0 <6 3 <6,0 <5.3 <5.0 <4.0 Specific surface (rn 'grami * >15» 15 >15 >15 3ul» 3er»lty l? leralfted Pczzotamc Activity index (%} Repal * 135 e?0. scoe. curing > SIS ounng > 99 7C > St 3 curfrg * «233 51C cjrng > 9 s e m scce cunng > 7a > 27 :c cums Retained or 45 mtcrco sieve W <10 <10 <10 < <10 vartet on from sve'age on 45 micror sieve isootnt*;. <5 < 5 Denetyikger;. ^epai Actoc svs expane or * <02 Foaming Mo tear ry T.sas (Vpdnts deviation from declarec In eiwiy) <2 <2 water requirement ratio % <125 Table 1. Corrycanson of m ail international smca fume standards. Please no! that the tabie jives the mandator/ chemrca! and physical requirements. Some of the standards also contaei opional requirements Where there are blanks, no mandatory requirements erist. A low permeability concrete may also give high strength, and a high strength shotcrete will also give a very low permeability This is where the fine tuning of the mix design comes in, to achieve both fresh and hardened performance. This may include the use of blended cements, retarding and other admixtures, different aggregate types or the use of hot/cold weather concreting techniques (chilled or hot water, flaked ice, etc.) Elkem Materials offers technical and practical assistance in determining mix parameters and designing silica fume concrete mixes. This knowledge has been established from many diverse projects worldwide. A p p licatio n D o sag e level *\ % Pum oing Aid 23 Normal Concrete 47 S e t Com pacting C oncrete High Strength 7 10** Low P e m e a b i ity * * U nderw ater Shotcrete ' The silica fume percentage is a ways given ai i dry weight by weight of the cementilic^s naxenals T* higher percentages n ay be sed under specfic conditions 10 achieve certain perfoma^ce csacteristics Table 2 General recommended oosage levels ofsrhca fume The information given on this datasheet <s accurate to the te s t knowledge qf Elkem Materiak. The information is offered n rfwur guarantee, and Elkem Materials accepts no tiebfsty ferary direct or morrect damage hem its use. The iifbnrat on *3 subject to change without notfoe. Far latest update or further rtormatron or assistance please contact your local representative the internet address or the emaii aooress grven on this datasheet. CONCRETE GENERAL INFORMATION NOVEMBER 2005 Contact/representative: E ken Mterosilica«is a registerec *racen3rt anc belongs to Skem ASA Materials Elkem Materials Internet vvww.concrete ellien.com enail: micros ca materials nem no Page 223
248 REVISION DATE: 03y04X)6 The Chemical Company SAFETY DATA SHEET Glenium Ace IDENTIFICATION OF THE SU BSTANCE /PREPARATION AND COMPANYi'UNDERTAKING PRODUCT NAME Glenium Ace 333 APPLICATION SUPPLIER Admixture for precast concrete BASF Construct o" Chemicas Albany House Sw "ton Ha 1Road Sw "ten Ms Chester M27 4DT (+44) NOTE : I" cases of emergency outside wondng hours, se ~e eehone Number above. Fo ow instructions from reccnced message. (+44) COMPOSITION/INFORMATION ON INGREDIENTS COMPOSITION COMMENTS Aqueous solution containing pcrycarboxylate ether 3 HAZARDS IDENTIFICATION Not regartiec as a heath or environments hazard under current legisatior. 4 FIRSTAID M EASURES INHALATION Moi/e t"e exposed oe<rsco to fres" air at once =rov :e 're s " air wanth a"d rest preferaby n a ccxnfortaoeuprghtstt'gposition. Set rredica atte"tion if any discomfort cont e s INGESTION DO NOT NDUCE VOMITING NEVER MAKE AN UNCONSCIOUS PERSON VOMIT OR DRINK FLUIDS! Rinse mouth thorcug y. Prcrrpty get affect ec person tc diin«large volumes of water to dilte the swallowed chemical. Cbta ' medical advice Provide rest warmth and fresh air. SKIN CONTACT Remove affocteo person Y or source cf contain a te . Remove cc"tarrinated clothing. Wash the s:in immec 3tely wit" soap 3"d water. Get medical stterto" if irrtat'on persists after washing. EYE CONTACT Mane s.re to encve any co'tact lenses from r e eyes before rins ~g. Promptly wash eyes wth plenty of water w~ e liftg the eye ds. Conti"* to r"se fc' at least 15 rr utes. Get meaica attention if any discomfort contres 5 FIREFIGHTING M EASURES EXTINGUISHING MEDIA T"is product is net Yarn mace. Use fireext nguis" ing media apprcp'ate for surrounding mate* a s SPECIAu FIRE FIGHT NG PROCEDURES No spec fc Yre fghting procedure g ven. 6 ACCIDENTAL RELEASE M EASURES PERSONAL PRECAUTIONS Wear protectve dcthing as d e s c c e d in S ectc" 8 of t" s safety data sheet ENVIRONMENTAL PRECAUTIONS Avoid subsoil cere ration Pevem product from ente' "g dra *s Do "ot contaminate surface water SPiLL CLEAN UP METHODS Wear etessary protective equipment. Stop leak if possioe without risk. Absorb verm culite, dry s a 'd or earth ad p ate into conta "ers F sh wth plenty of water to cean spillage area. Dc not contaminate water sources or sewer 1 / 3 Page 224
249 Glenium Ace HANDLING AND STORAGE USAGE PRECAUTIONS Avoid spilling, skin and eye contact. Observe good "custrial hyg e e practices. STORAGE PRECAUTIONS Keep in original container. Protec against Freezing Store Between 5 and 3C Degrees C 8 EXPOSURE C O NTRO LS/PERSO NAL PROTECTION PROTECTIVE EQUIPMENT ENGINEERING MEASURES No particular ventilaton reqirenets. RESPIRATORv EQUIPMENT If ventiaton s irtsuffctent suitable respratory protecton must be provided. HAND PROTECTION Use protective gloves. Rubber gloves are recommended EYE PROTECTION Use approved safety goggles or face shield. OTHER PROTECTION Wear appropriate clot" ing to prevent any possoility of skin contact HYGIENE MEASURES DO NOT SMOKE IN WORK AREA! Was" at die end of eac" work shift a nc before eat  a. srroking and us ng die toilet Wash promptly if skin becomes wet or contaminated. Promptly remove any cothing mat becomes contaminated. When us "g do no: ea t drink or smoke. 9 PHYSICAL AND CHEMICAL PROPERTIES ~ APPEARANCE COLOUR ODOUR Liquid Brown Characteristic SOLUBILITY M scble wit" water. MELTING POINT (*C) 0 RELATIVE DENSITY 20 c VAPOUR PRESSURE rv'a mbar phvalue. CONC. SOLUTION STABILITY AND REACTIVITY STABILITY Stable under norma temperature conditons and recommended use. CONDITIONS TO AVOID Avoid excessive heat for pro long ec perocs of time HAZARDOUS DECOMPOSITION PRODUCTS None ocher than those associated with the packaging 11 TOXICOLOGICAL INFORMATION TOXIC DOSE 1  LD 50 > 2000 mg. kg (ora rat) TOXICOLOGICAL INFORMATION No loxiogica data s ava able for die f " shed product polycarboxylates GENERAL INFORMATION Not irritating HEALTH WARNINGS No spec lie health warnings noted. Other Health Effects May case se'sitisadon to susceptible persons LD50/LC50 va ues m entc"ed referes to drvdual raw materials: 21 3 Page 225
250 Glenium Ace ECOLOGICAL INFORMATION ECO OXICfTY T"efe s no C3ta ava at) e for the prctict itse f. The ECSC.LC5D' 1C50 values men: oned fete's tc ndivrfual 'a* r3 ten a s: pc vcarboxvlates T"e pnoc u c shcuid no: be allowed tc enter d '3 's or water courses or be cepos ted w e re it can affect ground or surface waters 13 DISPOSAL C ONSIDERATIO NS DISPOSAL METHODS C spcse of waste a c residues in acconoance wth local authority require'nents. WASTE C U SS : Offspecficatc" batches and "usee p rcccs organic wastes other than t"ose ne"tic"ec in TRANSPORT INFORMATION ROAD TRANSPORT NO^ES RAIL TRANSPORT N C E S SEA TRANSPOR' NQTES Net class fied fc' road transport. Net class fied fc' rail traspcrr Net class fied fc' sea transport 15 REGULATORY INFORMATION RISK PHRASES SAFETV PHRASES ENVIRONMENTAL LISTING NC NC Not classified. Not classified. Rvers ;=reve"*jon of adltion) A c Cc"troi of Pollution {Special Waste Reguiato"s) A c EU DIRECTIVES System o 'sp eefe "formaton reating to Cangercus Reparations 'EEC. Dangerous Preparations Cirective ISsSAS.'EEC. STATUTORv INSTRUMENTS C "en cais >Hazard Infornsticn and Pac.agmg; Regulations. Control of Sbstances Hazardos tc Health. APPROVED CODE OF PRACTICE C assifcation and ^selling of Substances anc Pneps'aticns Dange'ous for Supply GUIDANCE NC^ES Work pace Exposure Limits EH40. Introductic" to Local E x"a.st Ve"tilation HS;3)37. CHIP fo' everyone HSG* *06/. 16 OTHER INFORMATION ISSUED BY HS&E Manager. REVISION DATE 03'04'06 REV. NC'REPL SDS GENERATED lsse 1 SDS NO SDS / 3 Page 226